of 124 /124
There have been tremendous improvements in iron and steelmaking processes in the past twenty years. Productivity and coke rates in the blast furnace and the ability to refine steel to demanding specifica- tions have been improved significantly. Much of this improvement is based on the application of fun- damental principles and thermodynamic and kinetic parameters which have been determined. Whereas, many future improvements will be forthcoming in steelmaking equipment, process improve- ments resulting from the application of fundamental principles and data will likewise continue. In this chapter the basic principles of thermodynamics and kinetics are reviewed and the relevant thermodynamic data and properties of gases, metals and slags relevant to iron and steelmaking are presented. These principles and data are then applied to ironmaking, steelmaking and secondary refining processes. These principles and data are also used in subsequent chapters in this volume. In writing this chapter, an attempt has been made to limit the discussion to an average level suit- able for the students of metallurgy pursuing graduate or post-graduate education as well as for those with some scientific background engaged in the iron and steel industry. It is assumed that the reader has some basic knowledge of chemistry, physics and mathematics, so that the chapter can be devoted solely to the discussion of the chemistry of the processes. 2.1 Thermodynamics 2.1.1 Ideal Gas A gas which obeys the simple gas laws is called an ideal gas satisfying the following relation: PV=nRT (2.1.1) where n is the number of mols and R the universal molar gas constant. For one mol of an ideal gas at 273.16K and l atm pressure, the value of the molar gas constant is: For pressure in Pa (Nm –2 Jm –3 ) and volume in m 3 , R = × × × = 1.01325 10 22.414 10 273.16 8.314 J mol K 5 -3 -1 -1 R . . = × = 1 0.08205 l atm mol K -1 -1 22 414 27316 Chapter 2 Fundamentals of Iron and Steelmaking E.T. Turkdogan, Consultant: Pyrometallurgy & Thermochemistry R.J. Fruehan, Professor, Carnegie Mellon University Copyright © 1999, The AISE Steel Foundation, Pittsburgh, PA. All rights reserved. 37
• Author

pecmett
• Category

## Documents

• view

271

4

Embed Size (px)

### Transcript of Funda Iron & Steel

There have been tremendous improvements in iron and steelmaking processes in the past twenty years.Productivity and coke rates in the blast furnace and the ability to refine steel to demanding specifica-tions have been improved significantly. Much of this improvement is based on the application of fun-damental principles and thermodynamic and kinetic parameters which have been determined.Whereas, many future improvements will be forthcoming in steelmaking equipment, process improve-ments resulting from the application of fundamental principles and data will likewise continue.

In this chapter the basic principles of thermodynamics and kinetics are reviewed and the relevantthermodynamic data and properties of gases, metals and slags relevant to iron and steelmaking arepresented. These principles and data are then applied to ironmaking, steelmaking and secondaryrefining processes. These principles and data are also used in subsequent chapters in this volume.

In writing this chapter, an attempt has been made to limit the discussion to an average level suit-able for the students of metallurgy pursuing graduate or post-graduate education as well as forthose with some scientific background engaged in the iron and steel industry. It is assumed that thereader has some basic knowledge of chemistry, physics and mathematics, so that the chapter canbe devoted solely to the discussion of the chemistry of the processes.

2.1 Thermodynamics

2.1.1 Ideal Gas

A gas which obeys the simple gas laws is called an ideal gas satisfying the following relation:

PV=nRT (2.1.1)

where n is the number of mols and R the universal molar gas constant.

For one mol of an ideal gas at 273.16K and l atm pressure, the value of the molar gas constant is:

For pressure in Pa (≡ Nm–2 ≡ Jm–3) and volume in m3,

R = × × × =1.01325 10 22.414 10273.16

8.314 J mol K5 -3

-1 -1

R..

= × =1 0.08205 l atm mol K -1 -122 414

27316

Chapter 2

Fundamentals of Iron and SteelmakingE.T. Turkdogan, Consultant: Pyrometallurgy & ThermochemistryR.J. Fruehan, Professor, Carnegie Mellon University

Ironmaking Volume

In a gas mixture containing n1, n2, n3... number of mols of gases occupying a volume V at a totalpressure P, the partial pressures of the constituent gaseous species are as given below.

(2.1.2)

P = p1 + p2 + p3 + ... (2.1.3)

The following equations are for a given mass of gas at constant pressure, volume and temperature:

Constant pressure (isobaric) (2.1.4)

Constant volume (isochoric) (2.1.5)

Constant temperature (isothermal) P1V1 = P2V2 = P3V3... (2.1.6)

Generally speaking, deviation from the ideal gas equation becomes noticeable with easily liquefi-able gases and at low temperatures and high pressures. The behavior of gases becomes more idealwith decreasing pressure and increasing temperature. The nonideality of gases, the extent of whichdepends on the nature of the gas, temperature and pressure, is attributed to two major causes: (1)van der Waals’ forces and (2) chemical interaction between the different species of gas molecules oratoms.

2.1.2 Thermodynamic Laws

2.1.2.1 The First Law

The first law of thermodynamics is based on the concept of conservation of energy. When there isinteraction between systems, the gain of energy of one of the systems is equal to the loss of theother system. For example, the quantity of heat required to decompose a compound into its ele-ments is equal to the heat generated when that compound is formed from its elements.

2.1.2.1.1 Enthalpy (heat content) The internal energy of a system includes all forms of energy otherthan the kinetic energy. Any exchange of energy between a system and its surroundings, resultingfrom a change of state, is manifested as heat and work.

When a system expands against a constant external pressure P, resulting in an increase of volume∆V, the work done by the system is

w = P∆V = P(VB – VA)

Since this work is done by the system against the surroundings, the system absorbs a quantity ofheat q and the energy E of the system increases in passing from state A to state B.

∆E = EB – EA = q – P∆V = q – P(VB – VA)

Upon re-arranging this equation, we have

(EB + PVB) – (EA + PVA) = q

The quantity E + PV is represented by a single symbol H, thus

∆H = q = (EB + PVB) – (EA + PVA) (2.1.7)

The function H is known as enthalpy or heat content.

There are two fundamental thermochemical laws which express the first law specifically in terms ofenthalpy. The first principle derived by Lavoisier and Laplace (1780) states that “the quantity of heatrequired to decompose a compound into its elements is equal to the heat evolved when that com-pound is formed from its elements”; i.e. the heat of decomposition of a compound is numerically

P

T

P

T

P

T 1

1

2

2

3

3

= = L

VT

VT

VT

1

1

2

2

3

3

= = L

pn

P11=

n + n + n +

1 2 3 K×

Fundamentals of Iron and Steelmaking

39

equal to its heat of formation, but of opposite sign. The second principle is that discovered by Hess(1840); it states that “the heat of reaction depends only on the initial and final states, and not on theintermediate states through which the system may pass.”

2.1.2.1.2 Heat Capacity The heat capacity of a substance is defined as the quantity of heat required toraise the temperature by one degree. The heat capacity of 1 g of a substance is called the specificheat. The heat capacity of 1 g-molecule (abbreviated as mol) is called the molar heat capacity.

The variation of energy, at constant volume, and of enthalpy, at constant pressure, with tempera-ture gives the heat capacity of the system, thus

(2.1.8)

(2.1.9)

For an ideal gas the difference between the molar heat capacities at constant pressure, Cp, and con-stant volume, CV, is equal to the molar gas constant.

Cp – CV = R (2.1.10)

Because of experimental convenience, the heat capacity is determined under conditions of constantpressure (usually atmospheric).

From the temperature dependence of heat capacity at constant pressure, the enthalpy change isobtained by integrating equation 2.1.9.

(2.1.11)

Above 298 K, the temperature dependence of Cp is represented by:

Cp = a + bT – cT–2 (2.1.12)

(2.1.13)

where the coefficients, a, b and c are derived from Cp calorimetric measurements at different tem-peratures.

In recent compilations of thermochemical data, the H values are tabulated at 100 K intervals forthe convenience of users.

2.1.2.1.3 Standard State The enthalpy is an extensive property of the system, and only the changein heat content with change of state can be measured. A standard reference state is chosen foreach element so that any change in the heat content of the element is referred to its standardstate, and this change is denoted by ∆H°.

The natural state of elements at 25°C and 1 atm pressure is by convention taken to be the referencestate. On this definition, the elements in their standard states have zero heat contents.

The heat of formation of a compound is the heat absorbed or evolved in the formation of 1 g-molof the compound from its constituent elements in their standard states, denoted by ∆H°298.

2.1.2.1.4 Enthalpy of Reaction The change of enthalpy accompanying a reaction is given by the dif-ference between the enthalpies of the products and those of the reactants.

∆H a bT cTT

= + −( )−∫ 2

298

dT

Η − Η =Τ ΤΤ

Τ

2 1

1

2o o C dT p∫

Cp =

∂Η∂Τ p

CE

T V

V

= ∂∂

Ironmaking Volume

For an isobaric and isothermal reaction,

A + B = C + D (2.1.14)

the enthalpy change is given by:

∆H = (∆H°C + ∆H°D) – (∆H°A + ∆H°B) (2.1.15)

By convention, H is positive (+) for endothermic reactions, i.e. heat absorption, and H is negative (–) for exothermic reactions, i.e. heat evolution.

Temperature effect:

(2.1.16)

(2.1.17)

The following are some examples of the special terms of the heat of reaction.

Enthalpy or heat of formation Fe + 1⁄2O2 → FeOHeat of combustion C + O2 → CO2Heat of decomposition 2CO → C + CO2Heat of calcination CaCO3 → CaO + CO2Heat of fusion (melting) Solid → LiquidHeat of sublimation Solid → VaporHeat of vaporization Liquid → VaporHeat of solution Si(l) → [Si] (dissolved in Fe)

2.1.2.1.5 Adiabatic Reactions When a reaction occurs in a thermally insulated system, i.e. no heatexchange between the system and its surroundings, the temperature of the system will change inaccordance with the heat of reaction.

As an example, let us consider the internal oxidation of unpassivated direct reduced iron (DRI) ina stockpile, initially at 25°C. The enthalpy of reaction at 298K is

(2.1.18)

The heat balance calculation is made for 1000 kg Fe in the stockpile with 150 kg FeO formed inoxidation. The heat absorbed by the stockpile is 150 × 103/72 × 267 kJ and the temperature rise iscalculated as follows:

Q = [nFe(Cp)Fe + nFeO (Cp)FeO](T − 298)nFe = 17,905 g-mol for 1000 kg FenFeO = 2087.7 g-mol for 150 kg FeOCp (Fe) = 0.042 kJ mol–1K–1

Cp (FeO) = 0.059 kJ mol–1K–1

∴ Q = 557,416 = (752 + 123) (T − 298)

With this adiabatic reaction, the stockpile temperature increases to T = 935K (662°C).

The moisture in the stockpile will react with iron and generate H2 which will ignite at the elevatedstockpile temperature. This has been known to happen when DRI briquettes were not adequatelypassivated against oxidation.

2.1.2.2 The Second Law

The law of dissipation of energy states that all natural processes occurring without external inter-ference are spontaneous (irreversible processes). For example, heat conduction from a hot to a cold

Fe O FeO H kJ mol+ → = − −12 2 298

1267, ∆ o

∆ ∆ ∆H H C dTT p

To o= + ( )∫298

298

∆ ∆ ∆Σ Σ Σ ΣH H products H C products C dTT p p

To o o= ( ) − ( ) + ( ) −[ ]( )∫298 298

298

reactants reactants

Fundamentals of Iron and Steelmaking

part of the system. The spontaneous processes cannot be reversed without some change in the sys-tem brought about by external interference.

2.1.2.2.1 Entropy The degree of degradation of energy accompanying spontaneous, hence irreversible,processes depends on the magnitude of heat generation at temperature T and temperatures betweenwhich there is heat flow.

The quantity q/T is a measure of degree of irreversibility of the process, the higher the quantityq/T, the greater the irreversibility of the process. The quantity q/T is called the increase in entropy.In a complete cycle of all reversible processes the sum of the quantities Σq/T is zero.

The thermodynamic quantity, entropy S, is defined such that for any reversible process taking placeisothermally at constant pressure, the change in entropy is given by

(2.1.19)

2.1.2.3 The Third Law

The heat theorem put forward by Nernst (1906) constitutes the third law of thermodynamics: ‘theentropy of any homogeneous and ordered crystalline substance, which is in complete internal equi-librium, is zero at the absolute zero temperature.’ Therefore, the integral of equation given abovehas a finite value at temperature T as shown below.

(2.1.20)

The entropy of reaction is

∆S =ΣS(products) – ΣS(reactants) (2.1.21)

and the entropy of fusion at the melting point Tm is

(2.1.22)

2.1.2.4 Gibbs Free Energy

From a combined form of the first and second laws of thermodynamics, Gibbs derived the freeenergy equation for a reversible process at constant pressure and temperature.

G = H – TS (2.1.23)

The Gibbs free energy is also known as the chemical potential.

When a system changes isobarically and isothermally from state A to state B, the change in the freeenergy is

GB – GA = ∆G = ∆H – T∆S (2.1.24)

During any process which proceeds spontaneously at constant pressure and temperature, the freeenergy of the system decreases. That is, the reaction is thermodynamically possible when ∆G < 0.However, the reaction may not proceed at a perceptible rate at lower tempertures, if the activationenergy required to overcome the resistance to reaction is too high. If ∆G > 0, the reaction will nottake place spontaneously.

As in the case of enthalpy, the free energy is a relative thermodynamic property with respect to thestandard state, denoted by ∆G°.

The variation of the standard free energy change with temperature is given by:

(2.1.25)∆ ∆ ∆ ∆∆

G H C dT T S TC

TdTT p

Tp

To o o= + − −∫ ∫298

298

298

298

∆ ∆S

HTm

m

m

=

S C dT p

T

= ( )∫0

ln T

dSdHT

= ( )=C

TdT = C d ln Tp

p

Ironmaking Volume

2.1.2.4.1 Generalization of Entropy Change of Reaction

1. When there is volume expansion accompanying a reaction, i.e. gas evolution, at con-stant pressure and temperature the entropy change is positive, hence, ∆G decreaseswith an increasing temperature.

C + CO2 = 2CO∆G° = 166,560 – 171.0TJ (2.1.26)

2. When there is volume contraction, i.e. gas consumed in the reaction, at constant pres-sure and temperature the entropy change is negative, hence ∆G increases with anincreasing temperature.

H2 + 1⁄2S2 = H2S∆G° = –91,600 + 50.6TJ (2.1.27)

3. When there is little or no volume change the entropy change is close to zero, hencetemperature has little effect on ∆G.

C + O2 = CO2∆G° = 395,300 – 0.5TJ (2.1.28)

2.1.2.4.2 Selected Free Energy Data For many reactions, the temperature dependence of ∆H° and ∆S°are similar and tend to cancel each other, thus the nonlinearity of the variation of ∆G° with the tem-perature is minimized. Using the average values of ∆H° and ∆S°, the free energy equation is sim-plified to

∆G° = ∆H° – ∆S°T (2.1.29)

The standard free energies of reactions encountered in ferrous metallurgical processes can be com-puted using the free energy data listed in Table 2.1.

2.1.3 Thermodynamic Activity

The combined statement of the first and second laws for a system doing work only against pres-sure gives the following thermodynamic relation.

dG = VdP – SdT (2.1.30)

At constant temperature G = VdP and for 1 mol of an ideal gas V = RT/P; with these substitutedin equation (2.1.30) we obtain

(2.1.31)

Similarly, for a gas mixture

dGi = RT d(ln pi) (2.1.32)

where pi is the partial pressure of the ith species in the gas mixture, and Gi partial molar free energy.

In a homogeneous liquid or solid solution, the thermodynamic activity of the dissolved element isdefined by the ratio

(2.1.33)

In terms of solute activity, the partial molar free energy equation is

dGi = RT d(ln ai) (2.1.34)

Integration at constant temperature gives the relative partial molar free energy in solution

Gi = RT ln ai (2.1.35)

aiT

=

vapor pressure of component (i) in solutionvapor pressure of pure component

dG RTdPP

RT d P= = ( )ln

Fundamentals of Iron and Steelmaking

In terms of the relative partial molar enthalpy and entropy of solution

(2.1.36)

which gives

(2.1.37)

or

(2.1.38)

2.1.3.1 Solutions

A solution is a homogeneous gas, liquid or solid mixture, any portion of which has the samestate properties. The composition of gas solution is usually given in terms of partial pressuresof species in equilibrium with one another under given conditions. For liquid solutions, as liq-uid metal and slag, the composition is given in terms of the molar concentrations of compo-nents of the solution.

The atom or mol fraction of the component i in solution is given by the ratio

where ni is the number of g-atoms or mols of component i per unit mass of solution, and n the totalnumber of g-atoms or mols. Since the metal and slag compositions are reported in mass percent,ni per 100g of the substance is given by the ratio

where M i is the atomic or molecular mass of the component i.

Noting that the atomic mass of iron is 55.85g, the atom fraction of solute i in low alloy steels isgiven by a simplified equation

(2.1.39)

In low alloy steelmaking, the composition of slag varies within a relatively narrow range, and thetotal number of g-mol of oxides per 100g of slag is within the range Σn = 1.6 ± 0.1. With this sim-plification, the mol fraction of the oxide in the slag is given by

(2.1.40)

2.1.3.1.1 Ideal Solutions – Raoult’s Law: The solutions are said to be ideal, if the activity is equal tothe mol or atom fraction of the component i in solution,

ai = Ni (2.1.41)

A thermodynamic consequence of Raoult’s law is that the enthalpy of mixing for an ideal solution,HM,id, is zero. Substituting a i = Ni and HM,id = 0 in the free energy equation gives for the entropyof formation of an ideal solution.

SM,id = R(N1 ln N1 + N2 ln N2 + N3 ln N3 +...) (2.1.42)

NiMi

i

= %.1 6

Ni

Mii

= ×%.0 5585

ni

Mii

= %

Nn

ni

i= Σ

log. .

aii iHRT

SR

= −2 303 2 303

ln aii iH

RTSR

= −

G H S Ti i i= −

Ironmaking Volume

Table 2.1 The Standard Free Energies of Formation of Selected Compounds from Com-piled Thermochemical Data

Notations: < > solid, liquid, ( ) gas, d decomposition, m melting, b boiling.

∆G° = ∆H° – ∆S°T–∆H° –∆S° ∆G° Temp.Range

kJ mol-1 J mol-1K-1 ±kJ °C<Al> = Al –10.8 11.5 0.2 660m2Al + 3/2(O2) = <Al2O3> 1683.2 325.6 8 660–1700Al + 1/2(N2) = <AlN> 328.3 115.5 4 660–1700

<C> + 2(H2) = (CH4) 91.0 110.7 2 25–2000<C> + 1/2(O2) = (CO) 114.4 –85.8 2 25–2000<C> + (O2) = (CO2) 395.3 –0.5 2 25–2000

<Ca> = Ca –8.5 7.7 0.5 842mCa = (Ca) 153.6 87.4 0.5 842–1500bCa + 1/2(O2) = <CaO> 900.3 275.1 6 842–1500bCa + 1/2(S2) = <CaS> 548.1 103.8 4 842–1500b<CaO> + <Al2O3> = <CaAl2O4> 19.1 – 17.2 8 25–1605m<CaO> + (CO2) = <CaCO3> 161.3 137.2 4 25–880d2<CaO> + <SiO2> = <Ca2SiO4> 118.8 – 11.3 10 25–1700<CaO> + <SiO2> = <CaSiO3> 92.5 2.5 12 25–1540m

<Cr> = Cr –16.9 7.9 – 1857m2<Cr> + 3/2(O2) = <Cr2O3> 1110.3 247.3 2 900–1650

<Fe> = Fe –13.8 7.6 1 1537m0.947<Fe> + 1/2(O2) = <Fe0.947O> 263.7 64.3 4 25–1371mFe + 1/2(O2) = FeO 225.5 41.3 4 1537–17003<Fe> + 2(O2) = <Fe3O4> 1102.2 307.4 4 25–1597m2<Fe> + 3/2(O2) = <Fe2O3) 814.1 250.7 4 25–1500<Fe> + 1/2(S2) = <FeS> 154.9 56.9 4 25–988mFe + 1/2(O2) + <Cr2O3>=<FeCr2O4> 330.5 80.3 2 1537–17002<FeO> + <SiO2> = <Fe2SiO4> 36.2 21.1 4 25–1220m

(H2) + 1/2(O2) = (H2O) 247.3 55.9 1 25–2000(H2) + 1/2(S2) = (H2S) 91.6 50.6 1 25–20003/2(H2) + 1/2(N2) = (NH3) 53.7 32.8 0.5 25–2000

K = (K) –84.5 82.0 0.5 63–759b(K) + <C> + 1/2(N2) = KCN 171.5 93.5 16 622–1132bKCN = 1/2(KCN)2 109.2 76.7 4 622–1132b

<Mg> = Mg –9.0 9.7 0.5 649mMg = (Mg) 129.6 95.1 2 649–1090b(Mg) + 1/2(O2) = <MgO> 759.4 202.6 10 1090–2000(Mg) + 1/2(S2) = <MgS> 539.7 193.0 8 1090–20002<MgO> + <SiO2> = <Mg2SiO4> 67.2 4.3 8 25–1898m<MgO> + <SiO2> = <MgSiO3> 41.1 6.1 8 25–1577m<MgO> + (CO2) = MgCO3) 116.3 173.4 8 25–402d

<Mn> = Mn –14.6 9.6 1 1244m<Mn> + 1/2(O2) = <MnO> 391.9 78.3 4 25–1244mMn + 1/2(O2) = <MnO> 406.5 87.9 4 1244–1700Mn + 1/2(O2) = MnO** 352.2 61.5 4 1500–1700** supercooled liquid below the melting point 1785°C<Mn> + 1/2(S2) = <MnS> 277.9 64.0 4 25–1244mMn + 1/2(S2) = <MnS> 292.5 73.6 4 1244–1530mMn + 1/2(S2) = MnS 265.0 66.1 4 1530–1700<MnO> + <SiO2) = <MnSiO3) 28.0 2.8 12 25–1291m

<Mo> = Mo –27.8 9.6 6 2620m<Mo> + (O2) = <MoO2> 578.2 166.5 12 25–2000<Mo> + 3/2(O2) = (MoO3) 359.8 59.4 20 25–2000

Fundamentals of Iron and Steelmaking

Table 2.1 (continued)

∆G° = ∆H° – ∆S°T–∆H° –∆S° ∆G° Temp.Range

kJ mol-1 J mol-1K-1 ±kJ °C1/2(N2) + 3/2(H2) = (NH3) 53.7 116.5 0.5 25–20001/2(N2) + 1/2(O2) + (NO) –90.4 –12.7 0.5 25–20001/2(N2) + (O2) + (NO2) –32.3 63.3 1 25–2000

Na = (Na) –101.3 87.9 1 98–883b(Na) + <C> + 1/2(N2) = NaCN 152.3 83.7 16 833–1530b2(Na) + 1/2(O2) = Na2O 518.8 234.7 12 1132–1950d

<Nb> = Nb –26.9 9.8 – 2477m2<Nb> + 1/2(N2) = <Nb2N> 251.0 83.3 16 25–2400m<Nb> + 1/2(N2) = <NbN> 230.1 77.8 16 25–2050m2<Nb> + 5/2(N2) = <Nb2O5> 1888.2 419.7 12 25–1512m

<Ni> = Ni –17.5 10.1 2 1453m<Ni> + 1/2(O2) = <NiO> 235.6 86.1 2 25–1984m<Ni> + 1/2(S2) = <NiS> 146.4 72.0 6 25–6003<Ni> + (S2) = <Ni3S2> 331.5 163.2 8 25–790m

1/2(S2) + (O2) = (SO2) 361.7 72.7 0.5 25–1700

<Si> = Si –49.3 30.0 2 1412mSi + 1/2(O2) = (SiO) 154.7 –52.5 12 1412–1700<Si> + (O2) = <SiO2> 902.3 172.9 12 400–1412mSi + (O2) = <SiO2> 952.5 202.8 12 1412–1723m

<Ti> = Ti –18.6 9.6 – 1660m<Ti> + 1/2(N2) = <TiN> 336.3 93.3 6 25–1660m<Ti> + (O2) = <TiO2> 941.0 177.6 2 25–1660m

<V> + V –22.8 10.4 – 1920m<V> + 1/2(N2) = <VN> 214.6 82.4 16 25–2346d2<V> + 3/2(O2) = <V2O3> 1202.9 237.5 8 25–2070m

Zn = (Zn) –118.1 100.2 1 420–907b(Zn) + 1/2(O2) = <ZnO> 460.2 198.3 10 907–1700Zn + 1/2(S2) = <ZnS> 277.8 107.9 10 420–907b(Zn) + 1/2(S2) = (ZnS) –5.0 30.5 10 1182–1700

<Zr> = Zr –20.9 9.8 – 1850m<Zr> + 1/2(N2) = <ZnN> 363.6 92.0 16 25–1850m<Zr> + (O2) = <ZrO2> 1092.0 183.7 16 25–1850m<Zr> + (S2) = <ZrS2> 698.7 178.2 20 25–1550m<ZrO2> + <SiO2> = <ZrSiO4> 26.8 12.6 20 25–1707m

* References to the compiled thermochemical data used in deriving ∆H° and ∆S° values are given in Ref. 27 cited inSection 2.2.2.4

Ironmaking Volume

2.1.3.1.2 Nonideal Solutions Almost all metallic solutions and slags exhibit nonideal behavior.Depending on the chemical nature of the elements constituting a solution, the activity vs com-position relation deviates from Raoult’s law to varying degrees, as demonstrated in Fig. 2.1 forliquid Fe–Si and Fe–Cu systems at 1600°C.

2.1.3.2 Activity Coefficient

The activity coefficient of solute i is defined by the ratio

(2.1.43)

If the activity is relative to the pure component i,it follows from Raoult’s law that as Ni→1, γ→1.

2.1.3.2.1 Henry’s Law for Dilute Solutions In infinitelydilute solutions, the activity is proportional to theconcentration

ai = γi°N

i(2.1.44)

The approach to Henry’s law at dilute solutions isdemonstrated in Fig. 2.2 for the activity of carbon(relative to graphite) in austenite at 1000°C. Theaustenite containing 1.65%C (NC = 0.072) is satu-rated with graphite at 1000°C for which the car-bon activity is one relative to graphite.

Since Henry’s Law is valid at infinite dilutiononly, the ration γi/γi

° is used as a measure of depar-ture from Henry’s Law for finite solute contents indilute solutions. For solute concentration in termsof mass percent, Henry’s activity coefficient isdefined by the ratio

γ ii

iN= a

0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0

Act

ivity

1.0

0.8

0.6

0.4

0.2

0

Silicon (atom fraction) Copper (atom fraction)

Raoult

's law

Raoult

's law

aSiaFe

aCu aFe

Fig. 2.1 Activities in liquid Fe–Si and Fe–Cu alloys at 1600°C showing strong negative and positive depar-tures from Raoult’s law.

0 0.02 0.04 0.06 0.08NC

1.0

0.8

0.6

0.4

0.2

0

Henry's law

a C

Fig. 2.2 Activity of carbon in austenite (relativeto graphite) at 1000°C, demonstrating deviationfrom Henry’s law.

Fundamentals of Iron and Steelmaking

(2.1.45)

such that fi→1 when %i→0.

2.1.3.2.2 Interaction Coefficients Over several mass percentages of the solute, the compositiondependence of activity coefficient fi of solute i in binary systems is represented by the followingrelation in terms of mass %i.

log fi = eii[%i] (2.1.46)

where e is called the solute interaction coefficient. For multi-component solutions, the followingsummation is used

log fi = eii[%i] + Σe

ij[%j] (2.1.47)

where eij is the effect of the alloying element j on the activity coefficient of solute i.

2.1.3.3 Conversion from One Standard State to Another

In steelmaking processes we are concerned with reactions involving dissolved elements at low con-centrations in liquid steel. Therefore, it is convenient to express the solute activity relative to Henry’slaw. The free energy change accompanying the isothermal transfer of solute from state A to state B is

(2.1.48)

Taking a pure component for state A, i.e. aA = 1 and Henry’s law for state B, i.e. aB = γi°Ni

∆G = RT ln(γi°Ni) (2.1.49)

For one mass percent solute in iron,

(2.1.50)

where Mi is the atomic mass (g) of the solute. Assuming that Henry’s law holds at 1 mass %, thestandard free energy of solution of pure component i in iron at 1 mass % is

(2.1.51)

Since Henry’s law is valid at infinite dilution only, appropriate correction must be made for non-ideal behavior when using the above equation.

2.1.4 Reaction Equilibrium Constant

Let us consider the following reaction equilibrium occurring at constant temperature and pressure.

mM + nN = uU + vV (2.1.52)

The state of equilibrium is defined by the following thermodynamic relation involving the activi-ties of reactants M and N and the activities of the products U and V.

(2.1.53)

where the equilibrium constant K can be derived from the standard free energy change accompa-nying the reaction thus,

∆G° = –RT ln K (2.1.54)

Κ = ( ) ( )( ) ( )

a a

a a

Uu

Vv

Mm

Nn

∆G RTMs

ii=

ln.0 5585 γ o

NMi

i

≈ 0 5585.

∆G RT B

A

=

lnaa

fii

i

= γγ o

Ironmaking Volume

Since ∆G° is a function of temperature only, the equilibrium constant is also a function of temper-ature only.

(2.1.55)

In terms of enthalpy and entropy changes

(2.1.56)

In exothermic reactions ∆H is negative, therefore the equilibrium constant K decreases with anincreasing temperature. The temperature effect on K is the opposite in endothermic reactions.

For ∆G° in J, R = 8.314 J mol–1K–1 and substituting log for ln,

(2.1.57)

As an example, let us consider the following reaction equilibrium between liquid slag and low alloysteel.

(MnO) + [C] = [Mn] + CO(g) (2.1.58)

where the parenthesis ( ) and [ ] represent respectively the oxides dissolved in slag and elementsdissolved in iron. From the free energy data in Table 2.1 and those in Table 2.8 in section 2.4 forthe dissolution of graphite and liquid manganese in liquid iron, the standard free energy changeaccompanying reaction 2.1.58 is

∆G° = 230,560 – 147.32TJ (2.1.59)

which gives for the equilibrium constant K

(2.1.60)

(2.1.61)

where pCO is in atm, the oxide activity is with respect to pure molten MnO and at low concentra-tions, the mass percentages of Mn and C in the steel are essentially equivalent to their activities,i.e. fMn and fC are close to unity.

For a steelmaking slag of basicity 3.0 containing 5% MnO, aMnO = 0.088; at 1600°C the equilib-rium constant is K = 18.42 for which equation 2.1.61 gives for the slag-metal equilibrium[%Mn]/[%C] = 1.62 at 1 atm pressure of CO.

2.2 Rate PhenomenaThere are many different facets of rate phenomena involving homogeneous or heterogeneouschemical reactions, mass transfer via atomic or molecular diffusional processes, viscous flow, ther-mal and electrical conduction and so on. The concepts of diffusion, mass transfer and chemicalkinetics presented briefly in this section of Chapter 2, are confined to cases which are relevant tothe study of the rates of reactions in the iron and steelmaking processes.

2.2.1 Diffusion

2.2.1.1 Fick’s Diffusion Laws

The first law is for the steady state diffusion.

Κ = ( )[ ][% ]

%Mn p

CCO

MnOa

log,

.Κ = − +12 0437 695

T

log.

Κ ∆= − GT

o

19 144

ln Κ ∆ ∆= − +HRT

SR

o o

ln Κ ∆= − GRT

o

Fundamentals of Iron and Steelmaking

The quantity of diffusing substance which passes per unit time through unit area of a plane per-pendicular to the direction of diffusion, known as the flux J, is proportional to the concentrationgradient of the diffusing substance

(2.2.1)

The coefficient D is the diffusivity of the substance in the medium; C is the concentration of thesubstance per unit volume and x the distance in the direction of diffusion.

The second law is for the nonsteady state diffusion.

The rate of accumulation of diffusing substance in a given volume element is the difference betweenthe inward and outward flux. In other words, what goes in and does not come out, stays there.

The rate of concentration change −dC/dt resulting from flux over a distance dx is

(2.2.2)

Hence, the change in flux with distance is

(2.2.3)

Invoking the first law and re-arranging gives the second law.

(2.2.4)

The solution of this equation depends on the geometry and on the boundary conditions of themedium in which the dissolved substance is diffusing.

2.2.1.2 Chemical and Self-Diffusivities

There are two kinds of diffusivities:

(i) The chemical diffusivity is the coefficient of diffusion defined by Fick’s lawDi = −Ji(∂C/∂x) for the single diffusing species i.

(ii) The self-diffusivity is the coefficient of diffusion measured in a homogeneousmedium with the radioactive or stable isotope (tracer) of the diffusing species. Theself-diffusion is a consequence of random movements of atoms or molecules.

For an ideal solution, or an infinitely dilute solution, we have the equality

Di = Di* (2.2.5)

For nonideal solutions in general (ionic or metallic), Onsager and Fuoss1 derived the followingrelation for the chemical diffusivity corrected for departure from ideal behavior.

(2.2.6)

where a i is the activity and γi the activity coefficient of the single diffusing species i.

2.2.1.3 Types of Diffusional Processes

There are various types of diffusional processes, depending on the medium in which the diffusion occurs.

2.2.1.3.1 Diffusion in Molten Slags and Glasses Because of the ionic nature of the medium, the diffu-sion in molten slags and glasses is by the ions. The ionic conduction is a purely random jump

D DC

DCi i

i

ii

i

i

=

= +

∗ ∗∂∂

∂ γ∂

lnln

lnln

a1

dJdx

ddx

DdCdx

dCdt

Dd Cdx

= −

=2

2

dJdx

dCdt

= −

JdCdt

dx= −

J DdCdx

= −

Ironmaking Volume

process. For the limiting case of purely free and random movements of ions, the self-diffusivity ofthe ionic species i is related to the electrical conductivity λi by the Nernst-Einstein2 equation

(2.2.7)

where Zi is the valence and Ci the concentration (mol cm-3) of the species i and F = 96,489 C mol–1

Reference may be made to a previous publication by Turkdogan3 on the review of interrelationsbetween ionic diffusion and conduction in molten slags.

2.2.1.3.2 Diffusion in Porous Media The rate of a heterogeneous reaction between a gas and a porousmedium is much affected by the counter-diffusive flow of gaseous reactants and products throughthe pores of the medium. There are two types of effective gas diffusivities, depending on the porestructure of the medium:

(i) Molecular diffusivity in large pores and at ordinary to high pressures.

(ii) Knudsen diffusivity in small pores and at low pressures.

The pore diffusion is discussed in more detail in Section 2.3.

2.2.1.3.3 Eddy Diffusivity The mass transfer occurring within a turbulent fluid flow ischaracterized by the diffusion coefficient called eddy diffusivity which is a function of thetime-averaged and fluctuating velocity components in turbulent flow. This subject is covered indetail in a text book on fluid phenomena by Szekely4.

2.2.2 Mass Transfer

In high temperature processes as in pyrometallurgy, the rates of interfacial chemical reactionsare in general much faster than the rates of transfer of the reactants and reaction products to andfrom the reaction site. The formulations of rate equations for transport controlled reactions varyconsiderably with the physical properties and type of fluid flow over the surface of the reactingcondensed phase. Then, there are formulations of rate equations for different regimes of gasbubbles in liquid metal and slag. For a comprehensive discussion of the transport controlledrate phenomena in metallurgical processes, reference may be made to textbooks by Szekely andThemelis5 and by Geiger.6

There are numerous computer software packages, as for example PHOENICS, FLUENT, CFDS-FLOWS3D, GENMIX, TEACH(2D, 3D), 2E/FIX, SOLA/VOF, METADEX(R) and FID, which areused in the steel industry in the process and design engineering of plant facilities and in the con-trol of steelmaking processes. References may also be made to the publications by Szekely et al.7-9

on the mathematical and physical modelling of metallurgical processes involving fluid flow, heattransfer, mass transfer and gas-slag-metal reactions.

There are of course many other publications on this subject which cannot all be cited here as thesubject matter is well outside the scope of this book.

The rate phenomena discussed in this chapter are on chosen subjects which are pertinent to vari-ous aspects of ferrous-pyrometallurgical processes, in addition to oxygen steelmaking, ladle refin-ing and degassing.

2.2.2.1 Parabolic Rate of Oxidation of Iron

The scale forming in the oxidation of iron, or low alloy steels, consists of three layers of oxides:wustite on the iron surface followed by magnetite then hematite on the outer surface of the scale.From several experimental studies it was found that the average wustite:magnetite:hematite thick-ness ratios were about 95:4:1. In iron oxides, the diffusivity of iron is greater than the oxygen

DRT

F Z Cii i

i∗ = 2 2 λ

Fundamentals of Iron and Steelmaking

diffusivity. The rate of oxidation is controlled primarily by diffusion of iron through the wustitelayer from the iron-wustite interface to the wustite-gas or wustite-magnetite interface, then throughthe thin layers of magnetite and hematite.

X2 = λt (2.2.8)

where λ is the parabolic rate constant, cm2 (scale) s–1

If the measurement of the rate of oxidation is made by the thermogravimetric method, then the par-abolic rate constant kp would be in units of (gO)2cm–4s–1. From the compositions and densitites ofthe oxides, with the relative thickness ratios of wustite:magnetite:hematite = 95:4:1, the values ofkp and λ are related as follows.

kp (gO)2 cm–4 s–1 = 1.877λ, cm2 (scale) s–1 (2.2.9)

Many experimental studies have been made of the rate of oxidation of iron in air and oxygen attemperatures 600 to 1300°C. The temperature dependence of the parabolic rate constant is shownin Fig. 2.3; the references to previous studies denoted by different symbols are given in a paper bySheasby et al.10

From theoretical considerations, Wagner11 derived the following equation for the parabolic rateconstant in terms of the activity of oxygen and self-diffusivities of the mobile species in the scale.For the case of wustite with D*Fe >> D*O Wagner’s equation is simplified to

(2.2.10)λ = ( )′

′′

∫ ∗2NN

D dO

FeFe O

O

O

a

a

aln

1300 1200 1100 1000 900 800 700 600

6 8 10 12

10–5

10–6

10–7

10–8

10–9

10–10

104

T(K–1)

Kp,

(g

O)2

cm

–4 s

–1

Temperature, °C

Fig. 2.3 Temperature dependence of the parabolic rate constant for oxidation of iron in air or oxygen with orwithout H2O. From Ref. 10.

Ironmaking Volume

where a′O and a″O are oxygen activities at the iron-wustite and wustite-magnetite interfaces, respec-tively. The diffusion of iron ions in the nonstoichiometric phase wustite FeXO, is via the cationvacant sites in the wustite lattice. It is for this reason that the self-diffusivity of iron increases withan increasing O/Fe atom ratio in wustite, i.e. with increasing iron deficiency, as shown in Fig. 2.4

The values of kp = 1.877λ calculated from the measured tracer diffusivity of iron using Wagner’sequation, are consistent with the average experimental values in Fig. 2.3 which is represented bythe following equation.

(2.2.11)

2.2.2.2 Oxidation of Carbon in CO2–CO Mixtures

Most forms of carbon are porous, therefore the rate of oxidation, i.e. gasification of carbon, is deci-sively affected by the pore structure, internal pore surface area, effective gas diffusivity in the poresand particle size.

In a critical review of the oxidation of carbon, Walker et al.14 gave a detailed and a comprehensiveaccount of (up to 1959) experimental and theoretical studies on this subject. In the late 1960s, Turk-dogan and co-workers15–17 pursued further experimental work on the oxidation of several types ofcarbon in CO2–CO mixtures at temperatures up to 1300°C and at pressures of 0.01 to 10 atm. Afew salient features of their findings are briefly given here.

Log kTp = − +8868

0 9777.

983°C

897°C

800°C

equilibriumwith Fe

equilibriumwithFe304

Himmel et al12

Hembree & Wagner13

1100°C

30

20

10

0 0.05 0.10 0.15

Sel

f diff

usiv

ity, D

* Fe

x 1

08 (c

m2 /s

ec.)

(1−NFe

/NO

)

Fig. 2.4 Self-diffusivity of iron as a function of (1 – NFe/NO) fraction of iron deficiency.

Fundamentals of Iron and Steelmaking

Depending on the particle size, pore structure, temperature and gas pressure, there is either com-plete internal burning or external burning of carbon. The rate equations are of the following formsfor these two limiting cases:

(i) For small porous carbon particles and at low temperatures and pressures, there is rapidcounter current pore diffusion of CO2 and CO, and the rate of oxidation is controlled bythe chemical kinetics on the pore walls of the carbon. For this limiting case of completeinternal burning, the rate equation is

ln(1 – F) = –φSCit (2.2.12)

where

F = the mass fraction of carbon oxidized,φ = specific isothermal rate constant of chemical reaction per unit area of the pore wall,S = connected internal pore surface area per unit mass cm2mol–1,

Ci = molar concentration of CO2 per cm3 in the gas stream,t = oxidation time

(ii) For large carbon particles and at high temperatures and pressures, the gas diffusion isconfined to the pore mouths on the surface of the carbon particle. For this limitingcase of external burning the rate equation is

(2.2.13)

where

De = effective CO2–CO pore diffusivity,ρ = molar bulk density of the carbon, ro = initial radius of carbon particle.

The effects of the particle size and gas pressure on the rate of oxidation of electrode graphite isshown in Fig. 2.5

A mathematical analysis was made by Tien and Turkdogan18 to formulate the pore diffusion effecton partial internal burning of relatively largecarbon particles. The experimentally determinedinitial rates of oxidation of coke and graphitespheres (≈ 2 cm dia.) in 1:1 CO2:CO mixture at1 atm pressure are compared in Fig. 2.6 with the

1 11

3

12

− −( ) = ( )F

SD

rC te

i

φρρ o

Particle diameter (mm)

R, r

ate

per

unit

mas

s of

carb

on (

min

–1 x

103

)

0 1 2 3

6

4

2

0

5

30

0.96

Atm. CO2

Fig. 2.5 Effect of particle size on the rate of oxidationof electrode graphite in pure carbon dioxide at1000°C. From Ref. 16.

900 1000 1100 1200Temperature (°C)

Graphite

Coke

ExperimentalCalculated

10–2

10–3

10–4

10–5

Rat

e, fr

actio

nal m

ass

loss

per

min

ute

Fig. 2.6 Effect of temperature on rate of oxidation ofcoke and graphite (1.9 and 2.2 cm dia. spheres,respectively) in 50:50 CO2:CO at 1 atm. From Ref. 18.

Ironmaking Volume

values calculated from the mathematical analysis, which is summarized in Fig. 2.7. In each dia-gram, the lower curve is for 80% internal burning; therefore, in the region below this curve thereis almost complete pore diffusion. The upper curve is for 20% internal burning; therefore, in theregion above this curve, the pore diffusion control predominates.

Reference should also be made to a paper by Aderibigbe and Szekely19 for a more detailed math-ematical formulation of the rate of pore-diffusion and reaction controlled gasification of metallur-gical coke in CO2–CO mixtures.

2.2.2.3 Reduction of Iron Oxides

In view of its practical importance to the understanding and control of ironmaking processes, agreat deal of research has been done on the gaseous reduction of iron oxides and iron ores.Because of the porous nature of iron oxides and the reduction products, the interpretation of thereduction rate data is inherently complex.

The formation of product layers during the gaseous reduction of dense sintered hematite and magnetitepellets or natural dense iron ore particles is a well-known phenomenon, as shown in Fig. 2.8.

In several studies made in the early 1960s20–22 it was found that the thickness of the reduced ironlayer, encasing the iron oxide core of the pellet, increased linearly with the reduction time. The mea-sured rates were interpreted in terms of the rate-controlling chemical reaction at the iron wustiteinterface; the diffusive fluxes of gases through the porous layers were assumed to be relatively fast.On the other hand, Warner23 and Spitzer et al.24 have expressed the view that the rate of gaseousreduction is much affected by the gaseous diffusional processes, e.g. the gas-film resistance at the

Tem

pera

ture

(°C

)1400

1200

1000

8001400

1200

1000

800

(a)

I

II

III

(b)

I

II

III

(c)

I

II

III

10–2 10–1 100 101 10–1 100

IReactioncontrol

IIMixedcontrol

IIIPore

diffusioncontrol

10110–2

Fig. 2.7 Critical radius and temperature for the limiting rate controlling processes at 1 atm pressure. (a) Coke,100% CO2; (b) Coke, 1:1 CO:CO2; (c) Graphite, 100% CO2; (d) Graphite, 1:1 CO:CO2. From Ref. 18.

Fundamentals of Iron and Steelmaking

pellet surface and particularly the resistance to dif-fusion in the porous product layers. The rate mea-surements made by Turkdogan and Vinters25 on thereduction of hematite pellets in H2–H2O andCO–CO2 mixtures have clearly demonstrated thatthe rate-controlling effects of gas diffusion into thepores of the oxide granules or pellets and throughthe porous iron layer dominate the reaction kinetics.

The sketch in Fig. 2.9 demonstrates three limitingrate controlling processes as outlined below.

(a) With fine granules there is internal reduc-tion producing rosettes or platelets ofmetallic iron within the oxide particle; therate in terms of mass fraction reduced, F, isindependent of particle size.

(b) With large and dense oxide particles andat high temperatures, the gas diffusion isslow and the reaction is confined essen-tially to pore mouths on the outer surfaceof the particle, bringing about the devel-opment of a porous iron layer around thepellet. Because of the layer formation, thismode of reduction is often called topo-chemical reduction. In the early stages of

reduction, the porous iron layer is sufficiently thin for rapid gas diffusion, therefore theinitial rate of reduction is controlled jointly by (i) gas diffusion into the pore mouths ofthe oxide and (ii) reaction on the pore walls of the wustite.

(2.2.14)

(c) When the porous iron layer becomes sufficiently thick, the rate of reduction will becontrolled essentially by the counter current gas diffusion (H2–H2O and CO–CO2)for which the limiting rate equation, for a given temperature is as follows.

(2.2.15)3 2 3 12

32− − −( )[ ] = =

− ( )

+F F Y

Dr

p p

RTt Ce i i eq

ρ

dFdt

SD

re∝

φ

a b c

Fig. 2.9 Schematic representation of (a) uniform internal reduction of wustite to iron, (b) limiting mixed con-trol (partial internal reduction) and (c) diffusion in porous iron as the rate-controlling step.

Fig. 2.8 Formation of reaction product layers inthe gaseous reduction of hematite pellets.

Iron

Wustite

Magnetite

Hematite

Ironmaking Volume

Fig. 2.10 Initial rate in hydrogenat 0.96 atm. as a function of par-ticle radius at indicated temper-atures. From Ref. 25.

where pi is the H2 or CO partial pressure in the gas stream and (pi)eq that for the iron-wustite equilibrium and C a constant (a negative number) that takes account of allearly time departures from the assumed boundary conditions for this limiting case.

(d) At high reduction temperatures, with large oxide pellets and low velocity gas flows,the rate of reduction is controlled primarily by mass transfer in the gas-film layer atthe pellet surface. In this limiting case the rate is inversely proportional to thesquare of the particle diameter.

The experimental data are given Fig. 2.10 showing the particle size effect on the initial rate ofreduction of hematite granules or pellets in hydrogen.

When the thickness of the reduced porous iron layer exceeds 1 mm, the subsequent rate of reduc-tion is controlled primarily by gas diffusion through the porous iron layer. The reduction data plot-ted in accord with equation 2.2.15 usually give elongated S-shaped curves as in Fig. 2.11 for 15mm diameter spheroidal hematite ore reduced in H2 at 1 atm. From about 50% to 95% or 99%reduction, data are well represented by straight lines. The effective H2–H2O diffusivities in thepores of the iron layer are derived from the slopes of the lines; details are given in Section 2.3.3.

The effect of reaction temperature on the pore surface area of iron and wustite formed by the reduc-tion of hematite is shown in Fig. 2.12. The higher the reduction temperature, the smaller the inter-nal pore surface area, i.e. the coarser the pore structure. The iron oxides reduced at temperaturesbelow 800°C are known to be pyrophoric, which is a consequence of a fine pore structure with alarge pore surface area as noted from the data in Fig. 2.12.

LimitingSlope –1

0.1 1

1100°C

1000°C

900°C

800°C

700°C

600°C

1200°C

Fra

ctio

nal o

xyge

n lo

ss p

er m

inut

e

dF dtO

,

0.01

0.1

1

10

frac

tiona

l oxy

gen

loss

per

min

ute

Fundamentals of Iron and Steelmaking

0 10 20 30 40

1200°C

1100°C

1000°C 900°C 800°C

1.0

0.8

0.6

0.4

0.2

0

100

98

95

90

75

50

25

% r

educ

tion

Time (min)

3 −

2F −

3(1

− F

)2/3

Fig. 2.11 Diffusion plot of reduc-tion data for 15 mm diameterspheroidal hematite ore. FromRef. 25.

Reduction temperature (°C)

100

10

1.0

0.1

0.01

S (

m2 g

-1)

(iron

or

wus

tite)

200 400 600 800 1000 1200

Fig. 2.12 Connected internal pore surface area of iron and wustite formed by reduction of hematite ores’ Aand B; (a) ore A reduced to iron in H2 (◊); (b) ore B reduced to iron in H2(∇ ) and reduced to wustite in anH2–H2O mixture (∆); (c) ore B reduced to iron in a CO–CO2 mixture () and reduced to wustite in anotherCO–CO2 mixture (). From Ref. 25.

Ironmaking Volume

2.2.2.4 Mass Transfer with Gas Bubbles in Oxygen Steelmaking

In most practical applications of gas injection into liquids, we are concerned mainly with rates ofreactions in the swarm of bubbles. Mass-transfer phenomena in the swarm of bubbles have beenstudied extensively with aqueous solutions; accumulated knowledge is well documented in areview paper by Calderbank.26 Also, several studies have been made of the bubble size and veloc-ity of rise of single bubbles in liquid metals. Szekely presented a comprehensive review of thesestudies in his book on Fluid Flow Phenomena in Metals Processing.4

In his recent book Fundamentals of Steelmaking, Turkdogan27 made an assessment of the sizerange of dispersed gas bubbles and the corresponding mass transfer in liquid steel for the condi-tions prevailing in the BOF and Q-BOP steelmaking processes. In this assessment, the bubbles areassumed to be generated from a multitude of points across the bottom of the vessel, as though theentire vessel bottom were in fact one big porous plug.

2.2.2.4.1 Gas Holdup and Superficial Gas Velocity The volume fraction of gas holdup (ε) is given bythe following ratio:

(2.2.16)

where

Vb = transitory bubble volume in the bath at any time,Vs = steel volume in the vessel,H = average bath depth,A = average bath cross sectional area.

The velocity of bubble rise, Ub, in a swarm of bubbles is given by the ratio

(2.2.17)

where

V.

= gas flow rate,Us = superficial gas velocity.

In the studies of Calderbank and co-workers26 with the air-water system, the gas was injected intothe column of water through a sieve plate on the bottom of the column. The fractional holdup ofgas was reported as shown in Fig. 2.13. The units in F factor are Us, m s–1 and ρg (the gas density),kg m–3.

The dot-dash curve is taken to represent the average values. It appears that at F ≥ 1, the gas holdupreaches an essentially constant value of ε = 0.6.

In the estimation of fractional gas holdup in the steel bath, during decarburization or argon stir-ring, the gas flow rates taken are for the melt temperature and average gas bubble pressure. Thevalues used are for 1600°C and 1.5 atm so that V

.T (m3s–1) = 4.57 × V

.o(Nm3s–1); for these condi-

tions the gas densities are 0.27 kg m-3 for N2 and CO and 0.39 kg m-3 for Ar; an average value isused, ρg = 0.33 kg m–3.

The average bath cross sectional area A in BOF or Q-BOP vessel increases with an increasinggas flow rate. Keeping in mind the inner dimensions of the BOF or Q-BOP vessel for 200-240ton heats, the area values used are: A = 22 m2 at V

.T = 60 m3s–1 decreasing to A = 16 m2 at V

.T = 1

m3s–1. On this basis, the following equation is obtained for the superficial gas velocity Us as afunction of V

.T.

(2.2.18)U m sV

VsT

T

−( ) =+

1

14 55 0 089

˙

. . ˙

UU V

Abs= =

ε ε

˙

ε =+

= −VV V

VHA

b

b s

s1

Fundamentals of Iron and Steelmaking

The volume fraction gas holdup and bubble velocity of rise calculated using equation 2.2.18 andFig. 2.13 are plotted in Fig. 2.14 as a function of the gas flow rate. The gas holdup in the slag layeris a more complex phenomenon, because of slag foaming and injection of large amounts of steeldroplets into the slag layer during decarburisation with oxygen blowing.

2.2.2.4.2 Estimation of Bubble Size for Uniformly Dispersed Bubbles in the Steel Bath Many estimateswere made in the past of gas bubble diameters in steelmaking processes, the estimates varying overa wide range from 1 to 8 cm or more. Bubbles with diameters >1cm acquire a spherical cap shapeas they rise in liquids. The apparent diameter is that of a sphere which has a volume equivalent tothat of the spherical cap shaped bubble.

Calderbank and co-workers26 and Leibson et al.28 have found that in aqueous solutions the bub-ble size becomes smaller with an increasing gas flow rate, ultimately reaching a minimum size ofabout 0.45 cm diameter at large gas flow rates. Relatively large gas bubbles in motion are subjectto deformation and ultimately to fragmentation into smaller bubbles. The drag force exerted bythe liquid on a moving bubble induces rotational and probably a turbulent motion of the gas withinthe bubble.

This motion creates a dynamic pressure on the bubble surface; when this force exceeds the surfacetension, bubble breakup occurs. Because of the large difference between the densitites of the gasand liquid, the energy associated with the drag force is much greater than the kinetic energy of thegas bubble. Therefore, the gas velocity in the bubble will be similar to the bubble velocity. On thebasis of this theoretical reasoning, Levich29 derived the following equation for the critical bubblesize as a function of bubble velocity.

1.0

0.8

0.6

0.4

0.2

00 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0

F=Us ρ (ms–1) (kg m–3)1/2√

ε, v

olum

e fr

actio

n ga

s ho

ldup

Average

Fig. 2.13 Experimental data of Calderbank26 on gas holdup in sieve plate columns for the air-water system.

F = Ïrw (ms–1) (kg m–3)1/2

Ironmaking Volume

0.6

0.5

0.4

0.3

0.2

0.1

0

6

5

4

3

2

1

0

Ub

(ms-

1 )

ε

ε

Ub

1 2 4 6 8 10 20 40 60 80 100

VT (m3 S–1)•

Fig. 2.14 Gas holdup and bubble velocity as a function of gas flow rate. From Ref. 27.

(2.2.19)

where σ is the surface tension and Cd the drag coefficient, which is close to unity. As the bubblesize decreases with increasing bubble velocity, the gas circulation within the bubble diminishes,thus becoming less effective in bubble fragmentation. Another view to be considered is that, as thegas holdup increases with increasing gas flow rate, the liquid layer separating the bubbles becomesthinner. Consequently, the dynamic gas pressure exerted on the bubble surface becomes nullifiedby similar forces exerted in the neighboring bubbles, hence the cessation of bubble fragmentationat high values of ε.

The bubble fragmentation with increasing ε, hence increasing Ub, is calculated for bubbles in waterwith σ = 0.072 Nm–1 and in liquid steel with (a) σ = 1.7 Nm–1 in the presence of O < 4 ppm and 40ppm S, and (b) σ = 1.3 Nm-1 in the presence of 600 ppm O and 120 ppm S. The results are shownin Fig. 2.15. As noted earlier, the limiting bubble size in air-water system is d = 0.45 cm which inter-sects the fragmentation curve at ε = 0.41, depicting the cessation of bubble fragmentation.

In an attempt to estimate the minimum bubble size in the swarm of bubbles in liquid steel, Turk-dogan proposed the following hypothesis: ‘the surface energy of bubbles per unit mass of liquidwhich the bubbles displace, are equal for all liquids.’ Thus, surface energy Eb of dispersed bubblesof uniform size per unit mass of liquid which they displace is given by:

(2.2.20)Ed

J kg liquidb =−

−61

1εε

σρ

dC Uc

d g b

=

3 2

2 2

13

ρ ρσ

l

Fundamentals of Iron and Steelmaking

This conjectured statement leads to the following similarity relation for non-foaming inviscid liquids.

(2.2.21)

With σ1 = 0.072 Jm-2 and d1 = 0.45 cm for gas-water system and σ2 = 1.3 Jm–2 and ρ2 = 6940 kg m–3,we obtain d2 = 1.16 cm for the limiting bubble diameter in liquid steel containing ≈ 600 ppm O and120 ppm S. For the melt containing O < 4 ppm and 40 ppm S, d2 = 1.52 cm. These limiting valuesintersect the fragmentation curves for liquid steel at about ε = 0.40, similar to that for water.

A uniform constant bubble size and essentially constant ε = 0.6 at high gas flow-rates, means a con-stant number of bubbles per unit volume of the emulsion. Noting that for the close-packed (fcc)arrangement of bubbles, the packing fraction (gas holdup) is ε = 0.74, the thickness of the liquid filmat the nearest approach of the bubbles is derived from the following equality of the bubble number.

(2.2.22)

Noting that for water the experimental data give d = 0.45 cm and that estimated for liquid steeld = 1.16 cm, equation 2.2.22 gives δ = 0.65 mm for bubbles in aqueous solutions and δ = 1.68 forbubbles in liquid steel at the limiting value of ε = 0.6for non-foaming inviscid liquids.

2.2.2.4.3 Rate Equation for Transport Controlled Gas Bubble Reactions in Liquid Steel For mass-transfercontrolled reactions of gas bubbles in liquid steel, the rate equation has the following form:

(2.2.23)

where Xo and X e are the initial and gas-metal equilibrium concentrations of the diffusing reactantin the melt, km the mass-transfer coefficient and So the bubble surface area which is in terms of ε.

ln% %% %

X XX X

S k te

em

−−

= −o

o

0 6 0 74

23 3

. .d d

=+( )δ

σρ

σρ

1

1 1

2

2 2

1

d dJ kg liquid= = −L

Equation 2.2.19

Uniform limitingbubble diameterLiquid steel

WaterEqu

ival

ent b

ubbl

e di

amet

er (

cm)

4

2

00 0.2 0.4 0.6ε

b a

Fig. 2.15 Calculated bubble diameter for bubble fragmentation mechanism equation 2.2.19, compared withuniform limited diameter at high values for water and liquid steel: (a) for O < 4 ppm and 40 ppm S (b) for 600ppm O and 120 ppm S. From Ref. 27.

Ironmaking Volume

(2.2.24)

Bubble surface area with respect to unit mass of liquid is:

(2.2.24a)

From many studies of gas bubble reactions in nonfoaming aqueous solutions, the following for-mulation have been derived for the liquid-phase mass-transfer coefficient for the regime of surface-renewal at the gas-liquid interface.26

(2.2.25)

where D is the diffusivity of the reactant in theliquid-film boundary layer.

In the presence of surface active solutes such asoxygen and sulphur in liquid steel, the bubble sur-face will be less mobile hence the rate constant kmwill be somewhat less than that given by equation2.2.25 for the mobile surface, which is a neces-sary condition for surface-renewal. On the otherhand, the surface active solutes decrease the bub-ble diameter, hence increase the bubble surfacearea for a given gas holdup. It appears that theproduct Sokm may not be too sensitive to the pres-ence of surface active solutes in the liquid.

The rate constant Sokm for the transport controlledreaction is obtained from the combination of equa-tions 2.2.17, 2.2.24 and 2.2.25 as given below foran average solute diffusivity D = 5 x 10–9 m2s–1.

(2.2.26)

The rate constant thus calculated is plotted in Fig.2.16 against the gas flow rate V

T at 1600°C andfor an average gas pressure of 1.5 atm in the steelbath for 220 + 20 ton heats.

2.2.2.4.4 Maximum Rate of Degassing of Liquid Steel with Argon Purging If the rates of diffusionalprocesses and chemical reactions are sufficiently fast, the argon bubbles traversing the melt will besaturated with N2 or H2 to the corresponding equilibrium values for the concentrations present in themelt. It is for this limiting case that the following rate equation is applicable.

Denoting N and H by X, and using molar contents in the gas bubbles,

(2.2.27)

(2.2.28)

where M is the molecular mass of X2 and V•

the argon blowing rate in Nm3 min–1t–1. In the X2-sat-urated argon bubbles for n⋅ Ar >> n⋅ X2

˙˙

.n

VAr =

× −22 414 10 3 g - mol Ar min ton

˙ minnd ppm X

dt MtonX 2

1010

66= ( ) ×

g - mol X2

S kU

dms

o =× ( )−5 43 10 4 1

2

32

. ε

kD U

dmb=

1 28

12

.

Sdm =

61

1εε ρ

,m / kg liquid2

Sd

m mo = 6 2 3ε, gas - melt emulsion

1 4 10 40 100

1.0

0.1

0.01

0.001

Sok

m (s

-1)

VT (m3 s-1) at 1600°C and 1.5 atm.

·

Fig. 2.16 Calculated rate constant for mass-trans-fer controlled reaction of gas bubbles in 220 + 20ton steel bath in the BOF or OBM (Q-BOP) vessel.From Ref. 27.

Fundamentals of Iron and Steelmaking

(2.2.29)

where P_

is the average bubble pressure in the melt.

Since the gas bubbles are in equilibrium with the melt

(2.2.30)

where K is the equilibrium constant. The integration of the above rate equation gives with Xo beingthe initial concentration,

(2.2.31)

For the average liquid steel temperature of 1650°C at turn down, the values of the equilibrium con-stants are as given below.

For an average gas bubble pressure of P_

= 1.5 atm in the melt, the following rate equations areobtained.

(2.2.32)

(2.2.33)

As discussed later in detail, the maximum rates are not observed in steelmaking processes; the ratesare limited by mass transfer and or chemical kenetics. Nevertheless equations 2.2.32 and 2.2.33indicate, even for the limiting case, large quantities of purging gas are required and the processesare normally not feasible.

2.2.3 Chemical KineticsThe theory of the absolute reaction rates isbased on the concept of the formation of anactivated complex as an intermediate transitionstate, which has an infinitesimally short lifetime of the order of 10–15 second. For anindepth study of the theory of reaction kinetics,to which outstanding contributions were madeby Eyring and co-workers, reference may bemade to the classical text books by Glasstone etal.30 and by Hinshelwood.31

As illustrated in Fig. 2.17, there is a change inenergy profile accompanying the reaction thatinvolves the formation and decomposition of anactivated complex. While the change in freeenergy accompanying reaction is ∆G° < 0, theactivation energy ∆G* > 0.

In almost all pyrometallurgical processes, weare concerned with heterogeneous reactions

1 10 0804

ppm H ppm HV t− =

o

. ˙

1 10 00395

ppm N ppm NV t− =

o

. ˙

For N : K = 459

For H : K = 27.2 with p in atm2

2X 2

1 122 414 10 3 2ppm X ppm X

M VP

t− =× −

o

˙

. Κ

pppm X d ppm X

dt MVPX 2

2

2

322 414 10= [ ] = ( ) × −

Κ.

˙

pn

nP

d ppm X

dt MVPX

X

Ar2

222 414 10 3

= = ( ) × −˙

˙.

˙

Activated complex

Reactants

Products

Reaction path

∆G°

∆G°

Ene

rgy

Fig. 2.17 Change in energy profile during the for-mation and decomposition of the activated complexinvolved in the reaction.

Ironmaking Volume

involving an interface between two reacting phases, e.g. solid-gas, solid-liquid, liquid-gas and twoimmiscible liquids (slag-liquid metal). For the case of a fast rate of transport of reactants and prod-ucts to and from the reaction site, the rate is controlled by a chemical reaction occurring in theadsorbed layer at the interface. The reaction between adsorbed species L and M on the surface pro-ducing product Q occurs via the formation of an activated complex (LM)*.

(2.2.34)

The theory of the absolute rates states that the activated complex is in equilibrium with the reac-tants for which the equilibrium constant K* for constant temperature is

(2.2.35)

where a’s are the thermodynamic activities.

Next to be considered is the specific rate of decomposition of the activated complex to the overallreaction product Q, represented by

(2.2.36)

where

dn/dt = the reaction rate, mol cm–2s–1,k = the Boltzmann constant, 1.380 × 10–23 J K–1,h = the Planck constant, 6.626 × 10–34 J s,T = temperature, K,Γ

°= total number of adsorption sites on the surface, 1015 mole cm–2,

θ* = fractional coverage by the activated complex.

For single site occupancy by the activated complex in the adsorbed layer, the activity of the com-plex is represented by

(2.2.37)

where θ is the total fractional occupancy of the sites by the adsorbed species and ϕ* is the activitycoefficient of the complex in the chemisorbed layer. Combining equations 2.2.35 - 2.2.37 gives therate of forward reaction in terms of the absolute reaction rate theory.

(2.2.38)

The thermodynamics of the chemisorbed layer at the interface, i.e. value of Γo, K* and ,ϕ are notknown, therefore the isothermal rate equation is given in a simplified general form thus

Rf = Φf (1 – θ)a L a M (2.2.39)

where Φf is the isothermal rate constant of the forward reaction.

As the reaction progresses, concentrations of the reactants L and M decrease while the concentra-tion of the product Q increases. Because of these composition changes and the influence of thereverse reaction Q→L + M, the rate decreases with an increasing reaction time. The rate of thereverse reaction is represented by

Rr = – Φr (1 – θ)a Q (2.2.40)

where Φr is the rate constant of the reverse reaction. Therefore, the net overall rate of reaction is

Rdndt

kThf L M= =

−( ) ∗

∗Γ Κo ϕ

θ1 a a

a∗ ∗∗

=−

ϕ θθ1

dndt

kTh

=

∗Γo θ

Κ∗∗

= aa aL M

L M LM Q+ = ( ) →

stage I

reactants

activated

complex

stage II

products

Fundamentals of Iron and Steelmaking

(2.2.41)

When the rates of forward and reverse reactions are the same, i.e. dn/dt = 0, the reaction is said tobe at an equilibrium state. It follows that the ratio of the rate constants Φf/ Φr is the equilibriumconstant of the reaction.

(2.2.42)

In terms of a single rate constant, the net reaction rate is formulated as

(2.2.43)

where (a La M)eq is the equilibrium value for the activity aQ in stage II at any given reaction time.

For a given surface coverage, the temperature dependence of the rate constant is represented by

(2.2.44)

where Φo is a pre-exponential constant and∆Η∗ is the apparent heat of activation for thereaction at a given site fillage θ.

Since the activation energy ∆G* is alwayspositive, the enthalpy of activation for thereaction is also positive. As shown in Fig.2.18 in the plot ln Φ vs 1/T the slope of theline gives ∆H*. It should be noted thatsince the thermodynamic quantities for theactivated complex (K*/ϕ*) in the chemi-sorbed layer are not known, the ∆H*derived from the rate measurements over asufficiently large temperature range, is theapparent heat of activation.

Another aspect of the kinetics of interfacialreactions is the rate of chemisorption or des-orption at the reaction surface as given bythe following theoretical equation for anuncontaminated surface.

(2.2.45)

where Mi is the molecular mass of the adsorbed species. This equation is transformed to the fol-lowing form for the maximum rate of vaporization, i.e. free vaporization, from an uncontaminatedsurface at low pressures

(2.2.46)

where pi is the vapor pressure in atm, for which the equation is reduced to the following form.

Ratemax (g-mol cm–2 s–1) = 44.3 pi (MT)–1⁄2 (2.2.47)

Ratemax = pM R T

i

i2 π

Φ ∆Ηf iM R T

R T= ( ) −

−∗

21

2π exp

Φ Φ ∆Η= −

o expRT

θ

dndt f L M L M eq

= −( ) ( ) Φ 1 θ a a a a-

K f

r

Q

L M eq

= =

ΦΦ

aa a

dndt f L M r Q= −( ) − −( ) Φ Φ1 1θ θa a a

In r

ate

cons

tant

(in

crea

sing

IT

(increasing

Slope = − ∆H*R

)

)

Fig. 2.18 Effect of temperature on rate constant forreaction involving an activated complex.

Ironmaking Volume

2.2.3.1 Examples of Experiments on Rates of Interfacial Reactions

2.2.3.1.1 Nitrogen Transfer Across Iron Surface The rate of reaction of gaseous nitrogen with liquidand solid iron, in the presence of surface active alloying elements, has been studied by many inves-tigators since the late 1950s. It was in the late 1960s32–34 that the rate controlling reaction mecha-nism was resolved, which was further confirmed in the subsequent experimental work done byFruehan and Martonik35, Byrne and Belton36, and Glaws and Fruehan37.

In particular the latter investigators used an isotope exchange technique which measured the rateof dissociation of the N2 molecule. They demonstrated the rate of dissociation was the same as therate of absorption of nitrogen, providing strong evidence that the absorption rate is controlled bydissociation.

When the rate of reaction is not hindered by slow nitrogen transport to and from the gas-metalinterface, the rate of nitrogenation

N2 (g) = N2* → 2[N] (2.2.48)

is controlled either by the rate of chemisorption or dissociation of N2 molecules on the metal sur-face. The rate of reverse reaction, i.e denitrogenation, is of course a second order type with respectto nitrogen dissolved in the metal. The equation below represents the rate of nitrogen transfer fromgas to liquid iron

(2.2.49)

where ρ is the density of liquid iron, A the surface area of the melt on which the nitrogen streamis impinging and V the volume of the melt. The rate constant Φf, in units of g N cm–2min–1atm–1N2,is for the forward reaction 2.2.48. The equilibrium partial pressure (pN2)eq corresponding to thenitrogen content of the melt at the reaction time t, is that given by the equilibrium constant K fornitrogen solubility.

(2.2.50)

With this substitution the isothermal rate equation is

(2.2.51)

For constant N2 pressure and temperature, the integration of equation 2.2.51 gives for %N = 0 att = 0,

(2.2.52)

Byrne and Belton made an accurate determination of the rate constant Φf for reaction of N2 withhigh purity iron and Fe-C alloys at 1550–1700°C, by measuring the rate of 15N→14N isotopeexchange that occurs on the iron surface, as represented by

(2.2.53)

where the rate constant Φf is in units of g N cm–2min–1atm–1. The apparent heat of activation =121.4 kJ mol–1 is much lower than the value expected for the rate of dissociation of N2. Aspointed out by Byrne and Belton, the rate of chemisorption of N2 is presumably controlling thereaction mechanism.

log . .Φf T= − ± ( ) + ±( )6340 710

1 85 0 38

ln%

%

ΚΚ

Φp N

p Np

AV

tN

NN f

2

2

22

1001

+ [ ]− [ ]

= −( )ρ

θ

d Ndt

AV

PN

f N% %[ ] = −( ) − [ ]

1001

2

2

ρθΦ

Κ

pNKN eq2

2

( ) = [ ]%

d Ndt

AV

P Pf N N eq

%[ ] = −( ) − ( ) 1001

2 2ρθΦ

Fundamentals of Iron and Steelmaking

The surface active elements dissolved in iron, e.g. O, S, Se, Te, are known to lower the rate ofnitrogen transfer across the iron surface. On the basis of the experimental rate data with liquidiron containing O and S, as given in various publications (Refs. 33–38) and the surface tensiondata, the effects of O and S on the fraction of vacant sites, 1−θ, in the chemisorbed layer maybe represented by

(2.2.54)

which is a slightly simplified form of the equation that was derived by Byrne and Belton.

For the chemical reaction-controlled nitrogen removal from liquid iron (or steel) in reduced pres-sures or in an inert gas stream with very low N2 pressure

2[N] → N2 (g) (2.2.55)

the integrated form of the rate equation is

(2.2.56)

where %No is the initial nitrogen content and Φr the rate constant = Φf /K.

The solubility of N2 in liquid iron or low alloy steel is given by

(2.2.57)

Combining this with equation 2.2.53 gives for the rate constant Φr in gN cm–2min–1%N–1

(2.2.58)

Now let us consider the chemical-reaction controlled rate of denitrogenation. It will be assumedthat the rate is controlled by only chemical kinetics. In actuality it is controlled by mass transferand chemical kinetics in series which is discussed later in detail. From equation 2.2.58 the rate for1600°C Φr = 0.233 g N cm-2s–1%N–1. For liquid steel containing 600 ppm O and 120 ppm S, (1 –θ) = 0.055 from equation 2.2.54. For the gas flow rate V

.T = 34 m3s–1, ε = 0.6 and the bubble sur-

face area is Sm = 1.11 cm2g-1 liquid steel. Inserting these numbers in equation 2.2.56 for the limit-ing case of %Ne ≈ 0, gives

(2.2.59)

In 60 seconds time of purging, 0.0030% No will be reduced only to 0.0024% N. In actual fact, theargon bubbles traversing the melt will contain some N2; for example, if the nitrogen partial pres-sure in gas bubbles were 0.001 atm N2, the equilibrium content in the melt would be 0.0015% Ne.Therefore, with %Ne > 0, the nitrogen removal will be much less than that calculated above for thechemical-reaction controlled rate for the hypothetical limiting case of %Ne ≈ 0.

The foregoing predication from the rate equation is in complete accord with the practical experience thateven at high rates of argon purging of the melt, as in OBM(Q-BOP), there is no perceptible nitrogenremoval primarily because of the presence of surface active solutes, oxygen and sulfur, in the steel bath.

2.2.3.1.2 CO2 and H2O Reaction with Fe–C Melts Another example of chemical kinetics con-trolling reaction rates is the decarburization of Fe–C melts.

C + CO2 = 2CO (2.2.60)

1 1100 1 11 0 233 0 055 1 42

% %. . . .

N Nt t

O

− = × × × =

log .Φ r T= − +5964

4 33

log%

.Κ = [ ]( )

= − −Np atm TN

2

2

3762 48

1 1 1001

% %N NA

Vtr− = −( )

o ρθΦ

11

1 2602

− =+ +

θ%

%O

S

Ironmaking Volume

Sain and Belton39 and later Mannion and Fruehan40 showed that the rate was affected by surfaceactive elements and was consistent with CO2 dissociation on the surface controlling the rate.

Nagasaka and Fruehan41 measured the rate of decarburization by H2O.

H2O + C = CO + H2 (2.2.61)

They also found that the rate was controlled by chemical kinetics and most likely dissociation of H2Oon the surface. For both the CO2 and H2O reaction, the rate constant could be expressed by the rela-tionship

(2.2.62)

where kC, kp and kr are the rate constants, kp is the rate constant for pure iron and kr is the residualrate at high sulfur contents respectively and Ks is the absorption coefficient for sulfur on liquid iron.The first term is based on the analysis by Belton42 and the residual rate which is relatively small isdiscussed by Nagasaka et al in detail.41 The overall rate constants are given as a function of sulfurcontent in Fig. 2.19.

kk

SkC

p

Sr=

+ [ ]+

1 Κ %

H2O

CO2

Fe-Csat. Melts

T=1873K

[mass % S]

100

10

1

0.10 0.005 0.01 0.015 0.02 0.025 0.03

k x

104

(mol

/cm

2 s

atm

)

Fig. 2.19 Rates of dissociationof CO2 and H2O on iron as afunction of sulfur content. FromRef. 41.

2.2.3.1.3 Chemical Kinetics of Carbon Oxidation in CO2–CO Mixtures Examples of the experimental dataon the initial rate of internal oxidation of granular (0.5 mm dia.) electrode graphite and metallur-gical coke are given in Figs. 2.20 and 2.21, reproduced from a previous publication.16

In a subsequent publication, Turkdogan27 re-assessed the interpretation of the rate data on theassumption that both CO and CO2 are chemisorbed on the pore walls of the carbon and the rate ofoxidation is due to the rate of dissociation of chemisorbed CO2. For the limiting case of completeinternal burning, the rate equation will be in the following form

(2.2.63)Ratep

k p k ptCO

CO CO

=′

+ +Φ

2

21 1 2

Fundamentals of Iron and Steelmaking

10–1

10–2

10–5

10–3

10–4

Rat

e, fr

actio

nal m

ass

loss

per

min

ute

0 20 40 60 80 100CO2 (%)

1200°C

1100°C

1000°C

Rat

e, fr

actio

nal m

ass

loss

per

min

ute

0 25 50 75 100CO2 (%)

100

10–1

10–2

10–6

10–5

10–4

10–3

900

800

700

°C140013001200

1100

1000

Fig. 2.20 Effects of temperature and gas composition on the rate of oxidation of electrode graphite granules(~0.5 mm dia.) in CO2–CO mixtures at 0.96 atm total pressure. From Ref. 16.

Fig. 2.21 Effect of temperature and gas composition on the rate of oxidation of granular metallurgical coke(~0.5 mm dia.) in CO2–CO mixtures at 0.96 atm total pressure. From Ref. 16.

Ironmaking Volume

where Φ′ is the rate constant (min–1atm–1CO2) for a given temperature and a particular type of car-bon; the constants k1 and k2 are associated with the chemisorption of CO and CO2. It should benoted that in compliance with the notation in equation 2.2.64 for the ideal monolayer, the constantsk1 and k2 are reciprocals of the respective activity coefficients of the absorbed species, i.e. k1 =1/ϕCO and k2 = 1/ϕCO2

; the fraction of vacant sites being (1 − θ ) = (1 − θCO − θCO2).

The fraction of surface sites θi covered by the adsorbed species is related to the solute activity asgiven in the following Langmuir adsorption isotherm.

(2.2.64)

From the cited experimental data for the oxidation of graphite and coke the following equations areobtained for the temperature dependence of Φ′, ϕ CO = 1/k1 and ϕCO2

= 1/k2.

For electrode graphite:

(2.2.65)

(2.2.66)

(2.2.67)

For metallurgical coke:

(2.2.68)

(2.2.69)

(2.2.70)

It should be noted that these equations fit the measured initial rates of oxidation within a factor ofabout 1.5 for temperatures 800 to 1200°C and for CO2 pressures 0.03 to 3 atm. For easy compari-son of the reactivities of electrode graphite and metallurgical coke, the numerical values are givenbelow from the above equations for 900 and 1200°C.

Electrode graphite Metallurgical cokeTemperature °C Φ′ ϕCO ϕCO2

Φ ′ ϕCO ϕCO2————————— —————————————————— —————————————————900 4.5 x 10–4 0.0025 0.27 1.9 x 10–3 0.029 0.67

1200 3.3 x 10–1 0.083 0.34 1.4 x 10° 0.068 0.14

After about 3 to 5 percent of initial oxidation, the pore surface area of the coke samples were foundto be four to five times greater than the graphite samples; this is consistent with the Φ′ values forcoke being greater than for graphite by a similar factor. The extent of CO adsorption on the porewalls of electrode graphite or coke is greater than the CO2 adsorption.

There are variations in the reported values of the apparent heat of activation for oxidation of theelectrode (or reactor grade) graphite in CO2. For example, Gulbransen et al.43 found ∆H* = 368 kJmol-1 while according to Blackwood’s work 44 ∆H* = 260 kJ mol–1; in the present case ∆H* = 317 kJmol-1. Reference should be made also to the papers of Ergun,45 Hedden and Lowe,46 and byGrabke47 for various other interpretations of the kinetics of oxidation of carbons.

Aderibigbe and Szekely48 also investigated the oxidation of metallurgical coke in CO2–CO mix-tures at 850 to 1000°C. Their rate constants K1 (≡ Φ′) are similar to those given by equation 2.2.68their estimate of the apparent heat of activation being ∆H* = 249±47 kJ mol–1.

log .ϕCO atmT2

38403 45( ) = −

log .ϕCO atmT

( ) = − +21170 27

log,

.′ ( ) = − +−Φ min-1 atm COT

12

16 54011 37

log .ϕCO atmT2

5900 072( ) = − −

log .ϕCO atmT

( ) = − +87194 84

log,

.′ ( ) = − +−Φ min-1 atm COT

12

16 54010 75

ai ii

i

=−

ϕ θθ1

Fundamentals of Iron and Steelmaking

Recently Story and Fruehan49 examined the oxidation of carbons in CO–CO2 gas mixtures at hightemperatures (>1300°C) under conditions of high external mass transfer. The gas mixture was jet-ted at high velocities, reducing the resistance to mass transfer at the surface. They were in limitingcase of external oxidation and determined the parameter (φρS De) from the data, and then usingpublished values of S and computed values of De, computed the rate constant. The results are com-pared to the rates measured at lower temperatures in Fig. 2.22.

1545 1393 1265 1155 1060 977

0.55 0.6 0.65 0.7 0.75 0.8

1/T x 103 (K–1)

10–6

10–7

10–8

10–9

10–10

10–11

Grabke(extrapolated)

Turkdogan et.al.(extrapolated)

Rat

e (m

ol/c

m2

s at

m)

This work

CP graphite UHP graphite

Guibrannsen et. al.

Temperature (°C)

Fig. 2.22 Arrhenius plotof graphite–CO2 data.

2.2.4 Mixed Control

In many metallurgical operations the rate is not controlled by a single reaction step such as masstransfer or chemical kinetics but rather two steps in series such as mass transfer followed by chem-ical kinetics. By equating the fluxes for each of the reaction steps it is possible to obtain expres-sions for the overall rate, or a series of expressions, which can be solved numerically.

2.2.4.1 Mixed Control for Gas Phase Mass Transfer and Chemical Kinetics

In general the temperature dependence of chemical kinetics is greater than for gas phase masstransfer. Consequently at low temperatures chemical kinetics is predominantly controlling the ratewhile at high temperatures mass transfer dominates. However for many reactions over a large rangeof conditions including temperature, fluid flow conditions and the concentration of surface activeelements which effect the chemical rate, the rate is controlled by both processes in series.

For example, the rate of dissociation of CO2 and H2O on liquid iron is controlled by both gas phasemass transfer and chemical kinetics in series over a large range of temperature and fluid flow con-ditions. In this case the pressure of the reacting gas at the surface is not the bulk composition. Theflux of the reacting gas and the rate of the reaction are given by 2.2.71 and 2.2.72 respectively,

(2.2.71)

R = k (pis – pi

e) (2.2.72)

JmR T

p piiB

is= −( )

Ironmaking Volume

where

mi = the gas phase mass transfer coefficient for i,

p iB = the pressure of i in the bulk phase,

pis = the pressure of i at the surface,

pie = the equilibrium pressure of i,

k = the chemical rate constant.

Equations 2.2.71 and 2.2.72 assume that the chemical rate is first order and the reaction is equil-molar in terms of the moles of reactant and product gases or the pressure of the reaction gas islow. As it is not possible to accumulate component i at the surface, the processes are assumed tobe at steady state and the flux and chemical rate are equated. It is then possible to calculate thepressure at the surface and the rate in terms of the bulk composition. Further simplification gives

(2.2.73)

Equation 2.2.73 is analogous to an electrical current with two resistances in series where k andmi/RT are analogous to conductivities. The first term in equation 2.2.73 is often referred to as theobserved or overall rate constant.

For example Nagasaka and Fruehan41 measured the rate of dissociation of H2O on liquid Fe-C-Salloys from 1673 to 1873°K for varying sulfur contents. At 1873K and 0.1% S the measured over-all rate constant was 2.5×10–4 mole/cm2 s atm for conditions where the mass transfer coefficientwas 100 cm/s. For this case the chemical rate was computed to be 3.9×10-4 mole/cm2 s atm.

Similarly the nitrogen and carbon dioxide reactions can be controlled by gas phase mass transferand chemical kinetics and equations 2.2.71 – 2.2.73 can be applied.

2.2.4.2 Mixed Control for Chemical Kinetics and Liquid Phase Mass Transfer

For many conditions in steelmaking and refining the rate of pick up or removal of nitrogen fromliquid iron is controlled by chemical kinetics and liquid phase mass transfer in series. Fruehan,Lally and Glaws50 developed a mixed control model and applied it to several metallurgicalprocesses. For nitrogen gas reacting with iron the flux of nitrogen for mass transfer and the chem-ical reaction are given by 2.2.74 and 2.2.75.

(2.2.74)

(2.2.75)

whereJN = flux of nitrogen (g/cm2 s),

m = mass transfer coefficient for nitrogen (cm/s),

k = chemical rate constant (g/cm2 s atm),

%Ns = nitrogen content at the surface,

K = equilibrium constant for nitrogen reaction with liquid iron,

ρ = density of iron (g/cm3).

J k pN

N N

s

= − [ ]

2

2%

Κ

Jm

N NNs= −[ ]ρ

100% %

R

kR Tm

p p

i

iB

ie=

+−( )1

1

Fundamentals of Iron and Steelmaking

Since no nitrogen can be accumulated at the surface it is possible to equate the two flux equa-tions, 2.2.74 and 2.2.75, and solve for the nitrogen content at the surface. The equation is a qua-dratic and is solved numerically for small time increments for specif ic conditions.. The surfacenitrogen content is then used to compute the rate of nitrogen absorption or removal. This tech-nique was applied to nitrogen absorption into liquid iron when bubbling nitrogen in the ladleand typical results are shown in Fig. 2.23. The rate of nitrogen pick up for low sulfur steel isconsiderably faster than for high sulfur steel, as sulfur decreases the chemical rate. Below0.005% S the rate does not increase further as liquid phase mass transfer then dominates and itis not affected by sulfur content.

0 4 8 12 16 20

0.010

0.009

0.008

0.007

0.006

0.005

0.004

0.005% S

0.03% S

Time (minutes)

Nitr

ogen

(%

)

Fig 2.23 Rate of nitrogen pick-up in 200 metric tons of steel containing 0.005 and 0.030% S, using 10 scfmof N2. From Ref. 50.

2.3 Properties of GasesOf importance to the iron and steelmaking and related pyrometallurgical processes, the selectedthermochemical and transport properties of gases are presented in this section.

2.3.1 Thermochemical Properties

2.3.1.1 Heat Content

The molar heat contents of simple selected gases of interest to pyrometallurgical processes areplotted in Fig. 2.24 over the temperature range 300–1900K.

SO2

CO2

H2S

H2O

O2

CO

N2

H2

Monatomic gases

300 700 1100 1500 1900Temperature (K)

∆HT

− ∆

H29

8 (k

J m

ol-1

)

80

0

20

40

60

Fig. 2.24 Heat contents of simple gases.

2.3.1.2 Equilibrium States in Gas Mixtures

When assessing the state of reactions involving gas mixtures, the partial pressures of the gaseousspecies should be evaluated from the reaction equilibrium data for all the pertinent gas reactions. Theprinciple of the computation is demonstrated by the following example for the gas mixtureCO–CO2–H2O–CH4.

This example is in relation to reheating a reformed gas in the direct iron ore reduction processes.If there is complete gas equilibrium at the reheating temperature and pressure, the activity of car-bon in the equilibrated gas mixture must satisfy the following three basic reaction equilibria:

(2.3.1)

(2.3.2)

(2.3.3)

(2.3.4)

(2.3.5)

(2.3.6)

For the predominant gaseous species the following equalities are derived from the mass balance for(ΣC), (ΣO) and (ΣH).

Κ3

22

4

=aC H

CH

p

p

CH C H4 22= +

Κ22

2

=aC H O

H CO

p

p p

H CO C H O2 2+ = +

Κ1 22=

aC CO

CO

p

p

2 2CO C CO= +

Ironmaking Volumme

Fundamentals of Iron and Steelmaking

(2.3.7)

(2.3.8)

where i and e indicate partial pressures in the ingoing and equilibrated gas mixtures, respectively.The equation below gives the total pressure P of the equilibrated gas mixture.

(pCO + pCO2+ pH2

+ pH2O +pCH4)

e= P (2.3.9)

The partial pressures of gaseous species and the activity of carbon in the equilibrated gas mixtureare computed by simultaneous solution of equations 2.3.1 to 2.3.9 with known values of the equi-librium constants K1, K2, and K3.

Examples are given in Fig. 2.25 showing the calculated carbon activities for 4 atm total pressureand for an initial gas mixture containing 73% H2, 18% CO, 8% CO2, 1% CH4 to which 0.2% to6.0% H2O has been added. The carbon deposition is imminent when its activity in the equilibratedgas exceeds unity, with respect to graphite. With the addition of 0.2% H2O to this gas mixture, thereshould be no carbon deposition in the equilibrated gas mixture at temperatures below 512°C andabove 720°C. In an earlier study of the reduction of iron oxides in a similar gas mixture, carbondeposition was observed at all temperatures below 1000°C (see Ref. 51), indicating lack of com-plete gas equilibrium even at 1000°C. These experimental findings suggest that carbon depositionmay occur during reheating of reformed natural gas in industrial operations, even when the calcu-lated carbon activity is less than unity in the gas mixture under equilibrium conditions.

ΣΣ

C

H

p p p

p p p

p p p

p p pCO CO CH

H O H CH i

CO CO CH

H O H CH e

=+ +

+ +

=

+ ++ +

2 4

2 2 4

2 4

2 2 42 2 4 2 2 4

ΣΣ

C

O

p p p

p p p

p p p

p p pCO CO CH

CO CO H O i

CO CO CH

CO CO H O e

=+ ++ +

=

+ ++ +

2 4

2 2

2 4

2 22 2

1.2

1.1

0.8

0.9

1.0

400 500 600 700 800

Act

ivity

of c

arbo

n

H2O (%)

0.2

2.0

3.0

4.0

6.0

Temperature (°C)

Fig. 2.25 Calculated activity of carbon for complete gas equilibrium at 4 atm and indicated temperatures forreformed natural gas containing 73% H2, 18% CO, 8% CO2 and 1% CH4 to which an indicated amount of H2Ois added. From Ref. 52.

Ironmaking Volume

The activity of carbon cannot be calculated for anonequilibrated gas mixture. However, for thepurpose of identifying the reactions that may beresponsible for carbon deposition, we may cal-culate carbon activities for individual reactionson the assumption that there is no change in thecomposition of the inlet gas upon heating. As isseen from the example given in Fig. 2.26 the car-bon activities for individual reactions differ con-siderably from those calculated for complete gasequilibrium. For complete gas equilibrium, thecarbon activity is below unity at temperaturesbelow 540 and above 700°C, while for the indi-vidual reactions the carbon activity is belowunity only within the temperature range880–1060°C. Therefore, in the nonequilibratedgas, there can be no carbon deposition onlywithin the temperature range 880–1060°C. Thetemperature at which carbon deposition maystart depends on the relative rates of reactions2.3.1 and 2.3.3: below 730°C if reaction 2.3.1 isfast, and below 880°C if reaction 2.3.3 is fast.

On the basis of the foregoing reasoning, we maycompute a diagram of % H2O in the inletreformed gas versus temperature, as in Fig. 2.27, to delineate the regions where (I) carbon will notdeposit, (II) carbon may deposit, and (III) carbon will deposit. With increasing pressure, regions II andIII move to higher temperatures and I to higher concentrations of H2O, and chances of carbon deposi-tion become greater. From the equilibrium constant for reaction 2.3.3, we can also compute the criti-cal pH2O/pCO ratio for possible carbon deposition at any temperature and partial pressure of H2 in theinlet gas. The possibility of carbon deposition in region II depends much on the catalytic behavior ofthe inner surface of the reheater tubes.

Temperature (°C)

600 700 800 900 1000

6

4

2

0

H2O

(vo

lum

e %

)

III

Carbonwill

deposit

II

Carbonmay

deposit

I

Carbonwill notdeposit

II

Carbonmay

deposit

For reactionH2 + CO = C + H2O

For completegas equilibrium

For reactionCH4 = C + 2H2

Fig. 2.27 Regions ofcarbon deposition atreheating temperaturesof reformed natural gasat 1 atm containingindicated amounts ofH2O. From Ref. 52.

400 500 600 700 800 900 1000

100

50

20

10

5

2

1

0.5

0.2

0.1

Act

ivity

of c

arbo

n

CO + H2 = C + H2O

2CO = C + CO2

For completegas equilibrium

CH4 = C + 2H2

Temperature (°C)

Fig 2.26 Calculated activity of carbon for completegas equilibrium at 4 atm. compared with the activityof carbon for individual reactions in a reformed inletgas containing 2% H2O. From Ref. 52.

Fundamentals of Iron and Steelmaking

77

0 20 40 60 80 100

Rat

e x

103

(mol

e C

min

-1)

6

4

2

0

0

2

4

H2 (volume %)

600°C

400°C

800°C

800°C

600°C

400°C

(a)

(b)

Fig. 2.28 Effect of gas composition (H2–CO) on rate of carbon deposition on 660-mg porous iron granules at1 atm(a) by reaction 2CO → C + CO2 and (b) by reaction CO + H2 → C + H2O. From Ref. 57.

2.3.1.3 Catalytic Decomposition of Carbon Monoxide

The catalytic decomposition of carbon monoxide has been the subject of much study, because of theoccurrence of carbon deposition in many processes, e.g., blast furnaces, the Stelling process, the Fis-cher-Tropsch process, nuclear reactors, and so on. References to early work on this subject are listedin an annotate bibliography by Donald53. The consensus is that iron, cobalt, and nickel are the mosteffective catalysts for the decomposition of carbon monoxide. Kehrer and Leidheiser54 reported vir-tually no catalytic effect of copper, silver, chromium, molybdenum, palladium, and rhenium.

In a comprehensive study of carbon deposition in CO–H2 mixtures at temperatures of 450–700°C,Walker et al.55 observed that the C/H atom ratio in the deposit increased from 10 to 50 with increas-ing reaction temperature and increasing CO/H2 ratio in the gas. They also found that the propertiesof carbon deposit were affected by the amount accumulated on the catalyst, e.g., with increasingthickness of the carbon layer, the crystallinity became poorer, the surface area increased, the elec-trical conductivity decreased, and the C/H2 ratio increased. Another important finding was that car-bon deposition ultimately ceased when most of the iron was converted to cementite. Uponhydrogen treatment, cementite decomposed to iron and graphite, but the regenerated iron lost mostof its reactivity as a catalyst. Similar observations were made by Turkdogan and Vinters51 in sub-sequent studies of the catalytic decomposition of carbon monoxide in the presence of porous iron.

It is generally agreed that iron, not cementite, catalyzes the decomposition of carbon monoxide. Thechemisorption of H2 and CO on the surface of iron is believed to approach equilibrium rapidly. Thecarbon formed by reactions 2.3.1 and 2.3.3 migrates across the surface to a nucleating center wherecementite and free carbon are deposited. Based on x-ray diffraction and electron microscopic stud-ies, Ruston et al.56 suggested that although the decomposition of carbon monoxide was catalyzed byiron, an iron carbide Fe7C3 formed as an intermediate step in the decomposition of the activatedreaction product to graphite.

Ironmaking Volume

78

As is seen from the experimental results of Olsson and Turkdogan57 in Fig. 2.28, the rate of car-bon deposition on an iron catalyst in CO–H2 mixtures is a complex function of temperature andgas composition. From the measured rate of carbon deposition and the measured CO2/H2O inthe exhaust gas, the rates of reactions 2.3.1 and 2.3.3 were determined. These measured ratesare shown in Fig. 2.29 as a function of gas composition at 400, 600 and 800°C. The hydrogenappears to have a dual role: at low concentrations the hydrogen catalyzes reaction 2.3.1, and athigh concentrations of hydrogen reaction 2.3.3 contributes directly to carbon deposition.

0 20 40 60 80 100

Rat

e x

103

(mol

e C

min

-1)

6

4

2

0

600°C

400°C

800°C

H2 (volume %)Fig. 2.29 Effect of gas composition (H2–CO) on rate of carbon deposition on 660–mg porous iron granulesat atmospheric pressure and indicated temperatures. From Ref. 57.

Although H2O is expected to retard or inhibit carbon deposition by virtue of reverse reaction2.3.4, it has been found57 that an addition of 0.5%–2% H2O to CO–CO2 mixtures enhances therate of carbon deposition at 400–600°C. A similar catalytic effect of H2O has been observed forcarbon deposition from methane in the presence of nickel58. We might mention in passing thatthe rate of carbon formation by the disproportionation of carbon monoxide is much faster thanthe pyrolysis of methane under similar conditions.59 Ever since the first observations made byByrom60 and soon after by Carpenter and Smith61, it has become generally recognized that sul-fur in the gas retards or inhibits the catalytic action of iron in the decomposition of carbonmonoxide. This is due to the coating of iron surface with cementite, which does not decomposereadily in the presence of sulfur. In fact, in the Stelling process62 the iron ore is reduced tocementite in a CO–CO2 atmosphere without the formation of free carbon, probably because ofthe presence of sulfur in the system.

The nitrogen-bearing gaseous species such as NH3 and (CN)2 are also known to retard the decom-position of carbon monoxide.62–63 Again, this may be attributed to extended metastability of cemen-tite in the presence of nitrogen. The retarding effect of sulfur and nitrogen on carbon deposition issimilar to sluggish graphitization of steel (by decomposition of cementite) in the presence of sul-fur and nitrogen in solution in steel.

Fundamentals of Iron and Steelmaking

The carburization of iron in gas mixtures containing H2 and CO following reactions similar to 2.3.1and 2.3.3 occurs on iron surfaces. These reactions are relevant to the early stages of metal dustingand were studied by Fruehan and Martonik.64 They also found that the rate of reaction 2.3.3 isfaster than 2.3.1 and contributes significantly to the carburization of iron64 as shown in Fig.2.30.When CO is replaced by H2 the rate increases significantly. The H2–CO reaction rate constant isapproximately tenfold greater than that for CO for carburization.

2.3.2 Transport Properties

The molecular transfer of mass, momentum and energy are interrelated transport processes of dif-fusion under a concentration gradient, viscous flow in a velocity gradient and heat conduction in athermal gradient.

The derivation of the transport properties from the rigorous kinetic theory of gases, described indepth by Chapman and Cowling65 and Hirschfelder et al.66 is based on the evaluation of the inter-molecular energy of attraction, the collision diameter and the collision integral involving thedynamics of a molecular encounter, hence the intermolecular force law.

For a brief description of the theoretical equations for the calculation of the transport properties ofgases, reference may be made to a previous publication.52 For the present purpose, it is sufficientto give selected numerical data on the transport properties of a few gases, relevant to ironmakingand steelmaking processes.

3

2

1

0

1273 K

1188 K

Vol % CO

0 20 40 60 80 100

x 10

4

i

gCcm

2 m

indC dt

Fig. 2.30 Initial rates of carburization or iron in H2–CO mixtures (pT = 0.965 atm). From Ref. 64.

Ironmaking Volume

2.3.2.1 Interrelations Between Transport Properties

2.3.2.1.1 Viscosity/Thermal Conductivity

For monatomic gases,

(2.3.10)

whereR = 8.314 J mol–1K–1 (molar gas constant),M = molecular mass, kg mol–1,η = viscosity, Nsm–2 ≡ Jm–3s.

κ η= 154

RM

Table 2.2 Diffusivity D at 1 atm Pressure: cm 2s–1 ≡ 10–4m2s–1

Temperature, K

Gas 300 1000 1500 2000

H2 1.46 10.82 21.07 33.90Ar 0.18 1.46 2.88 4.56N2 0.20 1.59 3.05 4.98O2 0.22 1.67 3.27 5.30CO 0.20 1.63 3.20 5.19CO2 0.11 0.93 1.87 3.00H2O 0.28 2.83 5.79 9.57

Table 2.3 Viscosity η (poise) ≡ g cm –1 s–1 ≡ 0.1N s m–2 ≡ 0.1J m–3s

Temperature, K

Gas 300 1000 1500 2000

H2 0.89 1.95 2.53 3.06Ar 2.50 5.34 6.98 8.27N2 1.77 4.07 5.11 6.30O2 2.07 4.82 6.20 7.64CO 1.79 4.15 5.34 6.53CO2 1.49 3.85 5.01 6.05H2O 1.57 4.77 6.44 7.84

Table 2.4 Thermal Conductivity κ 3 104, J cm –1s–1K–1 ≡ 3 102, kg m s –3K–1 ≡ 3 102,Wm–1K–1

Temperature, K

Gas 300 1000 1500 2000

H2 17.45 39.96 53.87 67.64Ar 1.97 4.18 5.44 6.44N2 2.50 6.18 8.15 10.53O2 2.57 6.68 9.02 11.62CO 2.53 6.35 8.57 10.96CO2 1.62 5.49 7.71 9.95H2O 3.84 13.55 20.20 26.93

Fundamentals of Iron and Steelmaking

For polyatomic gases,

(2.3.11)

where CV is the molar heat capacity at constant volume and

is the Eucken67 correction factor for thermal conductivity of polyatomic gases.

For monatomic gases CV = 3R/2; with this substitution, equation 2.3.11 is reduced to equation2.3.10. In terms of the molar heat capacity at constant pressure, CV = Cp − R, equation 2.3.11 istransformed to the following form.

(2.3.12)

2.3.2.1.2 Thermal Diffusivity/Thermal Conductivity The thermal diffusivity, DT, is analogous to massdiffusivity and is given by the ratio

(2.3.13)

where ρ is the molar density of the gas.

2.3.2.1.3 Temperature and Pressure Effects: The diffusivity, viscosity and thermal conductivityincrease with an increasing temperature, thus

D ∝ T3⁄2 (2.3.14)

η ∝ T1⁄2 (2.3.15)

κ ∝ T1⁄2 (2.3.16)

The viscosity and thermal conductivity are independent of pressure; however, the diffusivity isinversely proportional to pressure.

2.3.2.1.4 Molecular Mass Effect

D ∝ M–1⁄2 (2.3.17)

η ∝ M1⁄2 (2.3.18)

κ ∝ M–1 (2.3.19)

2.3.3 Pore DiffusionWhen the pores are small enough such that the mean free path of the molecules is comparable tothe dimensions of the pore, diffusion occurs via the collision of molecules with the pore walls.Knudsen68 showed that the flux involving collision of molecules with reflection from the surfaceof the capillary wall is represented by the equation

(2.3.20)

where v– is the mean thermal molecular velocity = (8kT/πm)1/2, r the radius of capillary tube anddC/dx the concentration gradient along the capillary. For r in cm and the Knudsen diffusivity DKin cm2s-1

(2.3.21)D rTMK = ×

9 7 103

12

.

J vrdCdx

= − 23

DC

T

P

= κρ

κ η= +

C

RMP

54

415

35

CR

V +

κ η= +

154

415

35

RM

CR

V

Ironmaking Volume

The Knudsen diffusivity being independent of pressure but molecular diffusivity inversely propor-tional to pressure, it follows that in any porous medium, the Knudsen diffusion predominates at lowpressures where the mean free path is larger than the dimensions of the pore.

For the mixed region of molecular and Knudsen diffusion in capillaries, Bosanquet69 derived thefollowing expression based on the random walk model in which the successive movements of mol-ecules are terminated by collision with the capillary wall or with other molecules:

(2.3.22)

where Dii is the molecular self-diffusivity. For a porous medium of uniform pore structure withpores of equal size, the Bosanquet interpretation formula gives for the effective diffusivity of com-ponent i

(2.3.23)

where ε is the volume fraction of connected pores, τ the tortuosity factor, D12 the molecular diffu-sivity for a binary mixture 1–2 and Dki the Knudsen diffusivity of component i for a given uniformpore radius r.

2.3.3.1 Examples of Experimental Data

The experimental data are shown in Fig. 2.31 for effective diffusivity He–CO2 at 20°C. As dis-cussed in Section 2.2.2.3 the pore structure of iron becomes finer at a lower reduction temperature.It is for this reason that the Knudsen diffusion effect at lower pressures becomes more pronouncedfor porous iron reduced at 800°C as compared to that reduced at 1000°C. More detailed informa-tion is given in the previous publications on the subject of gas diffusion in porous media.51, 70

DD D

D DeiKi

Ki

=+

ετ

12

12

1 1 1D D DKi ii

= −

1.0

0.1

0.01

Experimental

Calculated

Limiting slope -1

0.1 1.0 10 0.1 1.0 10

Pressure (atm.)

De

(cm

2 /s)

800°C 1000°C

Fig. 2.31 Pressure dependence of effective diffusivity He–CO2 at 20°C in iron reduced from hematite ore inhydrogen at indicated temperature. From Ref. 70.

It is seen from the data in Fig. 2.32 that the effective diffusivities for H2–H2O measured directly orcalculated from the pore structure considerations, agree well with those derived from the rate mea-surements within the regime of pore-diffusion control, i.e. from the slopes of the lines in Fig. 2.11.The temperature has a small effect on gas diffusivities. A marked effect of temperature on the effec-tive diffusivity seen in Fig. 2.32 is due mainly to the coarseness of the pore structure of iron whenthe oxide is reduced at higher temperatures.

Fundamentals of Iron and Steelmaking

In the case of internal burning of carbon, the pore structure becomes coarser as the gasification pro-gresses, resulting in an increase in the effective gas diffusivity. A few examples of the measuredCO–CO2 effective diffusivities for electrode graphite are given in Table 2.5, reproduced from Ref. 17.

400 600 800 1000 1200

Direct measurements

Calculated from pore structure

Derived from reduction data

4

3

2

1

0

Reduction temperature (°C)

De

(cm

2 /s)

Fig. 2.32 H2–H2O effective diffusivity derived from data for rate of reduction of hematite to iron is comparedwith that obtained by direct measurements and calculated from pore structure. From Ref. 70.

Table 2.5 Measured CO–CO 2 Effective Diffusivities for Electrode Graphite

Temperature % oxidized De(CO–CO2), cm2 s–1

500 0 0.006500 3.8 0.016500 7.8 0.020500 14.6 0.045700 0 0.009700 3.8 0.023700 7.8 0.029700 14.6 0.067800 0 0.012900 0 0.014

Ironmaking Volume

Recently Story and Fruehan49 demonstrated the effect of Knudsen diffusion in the oxidation of car-bon in CO2–Ar and CO2–He gas mixtures. Normally one would expect the rate to be significantlyfaster in CO2–He and CO2–Ar due to their higher molecular diffusivities. In general the diffusiv-ity is given by 2.3.22. Knudsen diffusion is important when the pore diameter is smaller than themean free path of the molecules, where the molecules strike the pore walls and diffusivity does notdepend on the molecule size. For ultra pure graphite the overall rate constant for external oxida-tion, (SDe) as discussed in Section 2.2.2.2, was the same for CO2–He and CO2–Ar gas mixtures.For this particular material the pore size was small and Knudsen diffusion predominates. On theother hand for coke with large pores the rate is significantly faster with He as the dilution gas asthe pores are large and molecular diffusion dominates.

2.4 Properties of Molten Steel

2.4.1 Selected Thermodynamic DataThe thermodynamic properties of liquid iron alloys have been studied extensively, both experi-mentally and theoretically. Most of these studies were made over a period from 1950 through 1970.For the present purpose, only a selected set of activity data need to be considered, in relation to thestudy and understanding of the chemistry of iron and steelmaking reactions.

2.4.1.1 Solute Activity Coefficients

For low solute contents, as in low-alloy steels, the activity is defined with respect to Henry’s lawand mass percent of the solute

a i = fix[%i] (2.4.1)

such that fi→1.0 as [%i]→0.

Up to several percent of the solute content, log f i increases or decreases linearly with an increas-ing solute concentration.

log fi = ei[%i] (2.4.2)

The proportionality factor ei is known as the interaction coefficient.

The binary interaction coefficients eii for dilute solutions in liquid iron are listed in Table 2.6, taken

from the data compiled by Sigworth and Elliott.71

Table 2.6 Values of e ii for Dilute Solutions in Liquid Iron at 1600°C. From Ref. 71

Element i eii Element i ei

i

Al 0.045 O –0.10C 0.18 P 0.062Cu 0.023 S –0.028Cr 0.0 Si 0.11Mn 0.0 Ti 0.013Ni 0.0 V 0.015

In multicomponent melts, as in alloy steels, the activity coefficient of solute i is affected by thealloying elements for which the formulation is

log fi = eii[%i] + Σ ei

j[%j] (2.4.3)

where eij is the interaction coefficient of i as affected by the alloying element j.

(2.4.4)ed fd ji

j i= [ ]log%

Fundamentals of Iron and Steelmaking

Selected interaction coefficients in dilute solutions of ternary iron base alloys for C, H, N, O andS at 1600°C are given in Table 2.7.

Table 2.7 Selected Interaction Coefficients in Dilute Solutions of Ternary Iron BaseAlloys for C, H, N, O and S at 1600°C. From Ref. 71.

Element j eCj e

Hj e

Nj e

Oj e

Sj

__________________________________________________________________________________________Al 0.043 0.013 –0.028 –3.9 0.035C 0.14 0.06 0.13 –0.13 0.11Cr –0.024 –0.002 –0.047 –0.04 –0.011Mn –0.012 –0.001 –0.02 –0.021 –0.026N 0.13 0 0 0.057 0.007O –0.34 –0.19 0.05 –0.20 –0.27P 0.051 0.011 0.045 0.07 0.029S 0.046 0.008 0.007 –0.133 –0.028Si 0.08 0.027 0.047 –0.131 0.063

For the mass concentrations of carbon and silicon above 1%, as in the blast furnace and foundryirons, the following values of fs

j should be used.

Mass % C or Si:2.0 2.5 3.0 3.5 4.0 4.5 5.0

f SC: 1.79 2.14 2.53 3.05 3.74 4.56 5.75

f SSi: 1.37 1.50 1.64 1.78 1.95 2.10 2.32

2.4.1.2 Free Energies of Solution in Liquid Iron

For the solution of element Xi in liquid iron at mass % X i,

Xi (pure) = [X i] (1 mass %)

the free energy of solution is

(2.4.5)

where Mi is the atomic mass (g-atom) and γ iº the activity coefficient (with respect to pure element)at infinite dilution (%Xi→ 0).

For ∆GS in J mol-1 and substituting log for ln,

(2.4.6)

The free energies of solution of various elements in liquid iron are listed in Table 2.8.

2.4.2 Solubility of Gases in Liquid IronDiatomic gases such as O2, S2, N2 and H2 dissolve in liquid and solid metals in the atomic form

1/2 X2(g) = [X] (2.4.7)

for which the isothermal equilibrium constant is

(2.4.8)Κ = [ ]( )

%X

pX 2

12

∆G TMS

ii=

19 1440 5585

. log. γ o

∆G RTMS

ii=

ln.0 5585 γ o

Ironmaking Volume

For ideal solutions, the concentration of X is directly proportional to the square root of the equi-librium gas partial pressure; this is known as the Sievert’s law.

2.4.2.1 Solubilities of H2, N2 and O2

For the solute content in ppm (by mass) and the gas pressure in atm., the temperature dependenceof the equilibrium constants for H2, N2 and O2 solubilities are given in Table 2.9 from the compileddata cited in Ref. 27.

Table 2.8 Free Energies of Solution in Liquid Iron for 1 mass %: (g) gas, (l) liquid,(s) solid. From Ref. 71.

Element i γ iº ∆Gs, Jmol-1

Al(l) 0.029 – 63,178 – 27.91TC(gr) 0.57 22,594 – 42.26TCo(l) 1.07 1,004 – 38.74TCr(s) 1.14 19,246 – 46.86TCu(l) 8.60 33,472 – 39.37T1/2H2(g) – 36,377 + 30.19TMg(g) – –78,690 + 70.80TMn(l) 1.30 4,084 – 38.16T1/2N2(g) – 3,599 + 23.74TNi(l) 0.66 – 20,920 – 31.05T1/2O2(g) – – 115,750 – 4.63T1/2P2(g) – – 122,173 – 19.25T1/2S2(g) – – 135,060 + 23.43TSi(l) 0.0013 – 131,500 – 17.24TTi(s) 0.038 – 31,129 – 44.98TV(s) 0.10 – 20,710 – 45.61TW(s) 1.20 31,380 – 63.60TZr(s) 0.043 – 34,727 – 50.00T

Table 2.9 Equilibrium Constants of Solubilities of H 2, N2 and O2 in Liquid Iron.

(2.4.9)

(2.4.10)

(2.4.11)log .ppm O

p TO

[ ]( )

= +2

12

60464 242

log .ppm N

p TN

[ ]( )

= − +2

12

1882 760

log .ppm H

p TH

[ ]( )

= − +2

12

19002 423

2.4.2.2 Solubility of Gaseous Oxides

2.4.2.2.1 Solubility of CO Carbon monoxide dissolves in liquid iron (steel) by dissociating intoatomic carbon and oxygen

CO(g) = [C] + [O] (2.4.12)

for which the equilibrium constant (which is not too sensitive to temperature) is given by the fol-lowing equation for low alloy steels containing less than 1% C.

Fundamentals of Iron and Steelmaking

(2.4.13)

At higher carbon contents, a correction should be made to K regarding the activity coefficients f O

C (log f OC = − 0.13[%C]) and f C

C(log f CC= 0.18[%C]).

For the reactionCO2 (g) = CO(g) + [O] (2.4.14)

(2.4.15)

For 800 ppm O in low carbon steel at tap, the equilibrium ratio pCO/pCO2is 13.75. For this state of

equilibrium, the gas mixture contains 6.8% CO2 and 93.2% CO.

2.4.2.2.2 Solubility of H2O From the free energy of formation of water vapor and the solubilitites ofhydrogen and oxygen in liquid iron, the following equilibrium constant is obtained for the reactionof water vapor with liquid iron for 1600°C.

H2O(g) = 2[H] + [O] (2.4.16)

(2.4.17)

The hydrogen and oxygen contents of low alloy liquid steel in equilibrium with H2–H2O mixturesat 1 atm pressure and 1600°C are shown in Fig. 2.33.

Κ = [ ] [ ]( )

= ×ppm H ppm O

p atmH O

26

2

1 77 10. at 1600 Co

Κ = [ ] = ×pp

ppm OCO

CO2

1 1 104. at 1600 Co

Κ = [ ][ ]( )

=%C ppm O

p atmCO

20

H2 + H2O = 1 atm.

Oxygen (wt. %)

Hyd

roge

n (p

pm)

PH2O atm. 0.003

0.01

0.050.1

0.2

0.001 0.004 0.01 0.04 0.1 0.2

10080

60

40

20

108

4

2

1

6

Fig. 2.33 Concentrations of hydrogen and oxygen in liquid iron at 1600°C in equilibrium with indicated com-positions of H2–H2O mixtures.

Ironmaking Volume

2.4.2.2.3 Solubility of SO2 From the free energy of formation of SO2 and the solubilities of gaseoussulfur and oxygen in liquid iron, the following equilibrium constant is obtained for the reaction ofSO2 with liquid iron at 1600°C.

SO2(g) = [S] + 2[O] (2.4.18)

(2.4.19)

For the concentrations of sulfur and oxygen present in liquid steel, it is seen that the correspond-ing equilibrium pressure of SO2 is infinitesimally small. It is for this reason that no sulfur can beoxidized to SO2 during steelmaking with oxygen blowing.

2.4.3 Iron-Carbon Alloys

2.4.3.1 Fe-C Phase Equilibrium Diagram

Since carbon is one of the most important ingredients of steel, the study of the iron-carbon phaseequilibrium diagram has received much attention during the past several decades. The phase dia-gram is given in Fig. 2.34.

Κ = [ ][ ]( )

=% %S Op atmSO

2

2

1558 at 1600 Co

0 1 2 3 4 5

0.020%

0.10%

1600

1400

1200

1000

800

600

Tem

pera

ture

(°C

)

Carbon (wt. %)

0.021%

0.76% 727°C

738°C

0.68%

910°C

α + γ

α + graphite

α + cementite

γ + graphite (stable phase)

γ + cementite (metastable phase)

2.01%

2.04% 1146°C

1152°C

4.27%γ

γ + liquid

1392°C

0.16%1499°C

Liquid

Graphite+

liquid

0.52%

1537°C δ + liquid

δ

Fig. 2.34 Iron-carbon phase equilibrium diagram. Dashed lines represent phase boundary for metastableequilibrium with cementite.

Fundamentals of Iron and Steelmaking

There are three invariants in this system; peritectic at 1499°C, eutectic at 1152°C and eutectoid at738°C. The phase boundaries shown by broken lines are for the metastable equilibrium of cementite,Fe3C, with austenite. During heat treatment of steel if sufficient time is allowed, iron-carbon alloyscontaining austenite and cementite decompose to austentite and graphite. The solubilitites of graphiteand of cementite in α-iron below the eutectoid temperature are given by the following equations

(2.4.20)

(2.4.21)

The solubility of graphite in pure liquid iron is well established through many independent stud-ies; the experimental data are summarized by the equation

[%C] = 1.30 + 2.57 x 10–3T(°C) (2.4.22)

If atom fraction NC is used, the same set of data can be represented by the following equation interms of log NC and the reciprocal of the absolute temperature.

(2.4.23)

The effect of silicon, phosphorus, sulfur, manganese, cobalt and nickel on the solubility ofgraphite in molten iron was determined by Turkdogan et al.72, 73 and graphite solubility in iron-silicon and iron-manganese melts by Chipman et at.74, 75 Similar measurements with iron-chromium melts were made by Griffing and co-workers.76 The experimental data are givengraphically in Fig. 2.35 for 1500°C; the solubility at other temperatures can be estimated fromthis plot by using the temperature coefficient given in equation 2.4.22 for binary iron-carbonmelts. In the iron-sulfur-carbon system there is a large miscibility gap. For example, at 1500°Cthe melt separates into two liquids containingphase (I) 1.8% S and 4.24% C and phase (II)26.5% S and 0.90% C.

2.4.3.2 Activity Coefficient of Carbon

The activity of carbon in liquid iron was mea-sured in many independent studies. The datacompiled and re-assessed by Elliott et al.77 aregiven in Figs. 2.36 and 2.37 as activity coeffi-cients γC and f C for two different standardstates.

2.4.3.3 Peritectic Reaction

The peritectic reaction occurring in the earlystages of solidification of low carbon steels isof particular importance in the continuouscasting of steel. The peritectic region of theFe–C system is shown on a larger scale in Fig.2.38. As the temperature decreases within thetwo phase region, δ+liquid, the carbon con-tents of δ-iron and residual liquid ironincrease. At the peritectic temperature 1499°C,δ-iron containing 0.10% C reacts with liquidiron containing 0.52% C to form γ-iron with0.16% C.

log .NTC = − −560

0 375

log % .C cementiteT

( ) = − +32001 50

log % .C graphiteT

( ) = − +52503 53

0 5 10 15Alloying element (wt.%)

Car

bon

(wt.%

)

CrMn

Co

Ni

Al

Si

P

S

Miscibilitygap

6

5

4

3

2

Fig. 2.35 Solubility of graphite in alloyed iron meltsat 1500°C.

Ironmaking Volume

0 0.04 0.08 0.12 0.16 0.20 0.24NC

0 1 2 3 4 5 6C(%)

0.8

0.6

0.4

0.2

0

–0.1

–0.2

–0.3

log

γ C

Austenite saturation

Graphite saturation1360°C

1260°C

1460°C

1560°C

1660°C

1760°C

Standard state:ac = 1 for pure graphite

0 1 2 3 4 5 6C (mass%)

1.0

0.8

0.6

0.4

0.2

0

log

f C

0 0.04 0.08 0.12 0.16 0.20

NC

Reference state:fC = 1 when %C→0

Austenite saturation

Graphite

Eutectic

1560°C

1660°C

1260°C1360°C

1460°C

1760°C

Fig. 2.36 Activity coefficient (γC) of carbon in liquid iron.

Fig. 2.37 Activity coefficient (fC) of carbon in liquid iron.

Fundamentals of Iron and Steelmaking

The X-ray diffraction data give for the densities of iron-carbon alloys: 7.89 g cm-3 for δ–Fe with0.10% C and 8.26 g cm-3 for γ–Fe with 0.16% C. Hence, the δ to γ phase transformation is accom-panied by 4.7% volume shrinkage. Because of this shrinkage, the thin solidified shell in the mouldof the caster will contract, producing a gap between the shell surface and mould wall. This situationleads to an uneven surface which is in partial contact with the mould wall, hence resulting in reducedheat flux at contracted areas. A reduced solidification growth rate and a nonuniform shell with thinspots, lowers the resistance of the steel to cracking which may cause a breakout in the mould. Thisphenomenon was well demonstrated experimentally by Singh and Blazek78 using a bench scalecaster; this subject is discussed furtherin a paper by Wolf and Kurz.79

In low alloy steels containing 0.10 to0.16% C, the solid/liquid ratio at theperitectic invariant is higher than forsteels containing more than 0.16% C.Therefore, due to the peritectic reac-tion, low alloy steels with 0.10 to 0.16%C are more susceptible to the develop-ment of surface cracks in continuouscasting than steels with higher carboncontents.

2.4.3.3.1 Effect of Alloying Elements onPeritectic Invariant As shown schemat-ically in Fig. 2.39 for the ternaryFe–C–X, or multicomponent alloy steels,the peritectic reaction occurs over atemperature and composition range.From the experimental data on the liq-uidus and solidus temperatures of alloysteels, the carbon and temperatureequivalents of alloying elements havebeen evaluated in three independentinvestigations.80–82

0 0.2 0.4 0.6Mass (%C)

1550

1500

1450

Tem

pera

ture

(°C

)

Liquid

δ + liquidδ

+ γ

δ

γ

γ + liquid

0.520.160.10 Fig. 2.38 Peritectic region of

binary iron-carbon system.

0 %C

Liquid

δ + liquid

δ

δ + γ

γ

δ + γ + liquid

γ + liquid

Tem

pera

ture

Fig. 2.39 Schematic representation of phase boundaries inlow alloy steels as pseudo binary Fe–C system.

Ironmaking Volume

The carbon equivalents of the alloying elements for the peritectic reaction

C(δ – Fe) + C (l – Fe) = C (γ–Fe) (2.4.24)

are usually formulated as follows

(2.4.25)

(2.4.26)

The changes in peritectic temperatures are formulated as

(2.4.27)

(2.4.28)

The coefficients ∆CPX and ∆TP

X can be positive or negative, depending on the alloying element X. Theperitectic temperature and carbon coefficients determined by Yamada et al.81 are listed in Table 2.10with minor numerical adjustments to some of the parameters in accord with the empirical correlationsgiven in Fig. 2.40, reproduced from Ref. 27.

Delta phase: T = 1499 C + TPX∆ ∆Σoδ %X[ ]

Liquid phase: T = 1499 C + TPX∆ ∆Σol %X[ ]

Delta phase: %C = 0.10 + CPX∆ ∆Σ δ %X[ ]

Liquid phase: %C = 0.52 + CPX∆ ∆Σ l %X[ ]

−60 −50 −40 −30 −20 −10 0 10

−0.10 −0.08 −0.06 −0.04 −0.02 0 0.02 0.04

∆TPδ (°C/%X)

10

0

−10

−20

−30

∆TP

l (°C

/%X

)

Si

MoV

Cr

Ni

Mn

PS

∆CPδ (%C/%X)

0.1

0

−0.1

−0.2

−0.3

−0.4

−0.5

∆CP

l (%

C/%

X)

Cr

VMoSi

Mn

P

S

Ni

Fig. 2.40 Interrelations between peritectic temperature and composition changes. From Ref. 27.

Fundamentals of Iron and Steelmaking

The phase boundaries in the peritectic region of the Fe–C–X alloys, projected on the Fe–C–X com-position diagram, are shown schematically in Fig. 2.41 for alloys where X is: (a) ferrite stabiliserand (b) austenite stabiliser. In the Fe–C–Mn (or Ni) system, the peritectic reaction occurs at all com-positons between the peritectic regions of the binaries Fe–C and Fe–Mn (Ni) systems. In the Fe–Calloys with ferrite stabilisers, the peritectic reaction will not occur beyond a certain concentration ofthe alloying element X as shown in Fig. 2.41. This limiting case applies only to high alloy steels.

2.4.4 Liquidus Temperatures of Low Alloy SteelsThe liquidus temperatures of low alloy steels are derived from the binary Fe–X systems on theassumption that the coefficients α = ∆T/%X are additive in their effects on the melting point of iron.

Below 0.5% C, where the solidification begins with the formation of delta (δ) iron, the followingequation would apply

Liquidus T (°C) = 1537 – 73.1[%C] + Σα[%X] (2.4.29)

For the carbon contents within the range 0.5 to 1.0% C, where the solidification begins with theformation of gamma (γ) iron, the following equation is recommended.

Liquidus T (°C) = 1531 – 61.5[%C] + Σα[%X] (2.4.30)

The same coefficients α are used in both equations.

Alloying element X Coefficient α, °C/%X_________________ ___________________Al –2.5Cr –1.5Mn –4.0Mo –5.0Ni –3.5P –30.0Si –14.0S –45.0V –4.0

2.4.5 Solubility of Iron Oxide in Liquid IronSubsequent to earlier studies by various investigators, Taylor and Chipman83 made the most reli-able measurement of the oxygen solubility in liquid iron in equilibrium with essentially pure liq-uid iron oxide at temperatures of 1530–1700°C. In a later study, Distin et al.84 extended thesolubility measurements up to 1960°C. The solubility data are represented by the equation

(2.4.31)log % ..

OTsat[ ] = − +6380

2 765

Table 2.10 Peritectic Temperature and Composition Parameters in Accord with theCurves in Fig. 2.40.

Alloying Composition ∆°C/%X ∆%C/%X______________________ ______________________Element range, wt.% ∆ΤPl ∆ΤPδ ∆CPl ∆CPδ

Cr <1.5 –3 –5 +0.022 +0.006Mn <1.5 +3 +7 –0.085 –0.029Mo <1.5 –10 –18 +0.055 +0.012Ni <3.5 +4 +9 –0.082 –0.027P <0.05 –24 –56 –0.250 –0.080S <0.03 –28 –64 –0.500 –0.105Si <0.6 –16 –32 –0.035 –0.010V <1.0 –6 –11 +0.045 +0.010

Ironmaking Volume

The oxygen content of liquid iron oxide in equilibrium with liquid iron decreases with an increas-ing temperature as given below and reaches the stoichiometric composition (22.27%) at about2000°C.

Temperature °C %O in iron %O in liquid iron oxide___________________ __________ ____________________1527 (eutectic) 0.16 22.601785 0.46 22.401880 0.63 22.371960 0.81 22.32

2.4.6 Elements of Low Solubility in Liquid Iron

A few elements of low solubility in liquid iron play some role in the steelmaking technology; abrief comment on the chemistry of such elements in liquid iron is considered desirable.

The break out of the furnace lining is often blamedon the presence of lead in the melt. Small amountsof metal trapped in the crevices of the lining arelikely to get oxidized subsequent to tapping. Thelead oxide together with iron oxide will readilyflux the furnace lining, hence widening the crackswhich ultimately leads to failure of the lining. Thesolubility of lead in liquid iron is sufficiently highthat in normal steelmaking practice there shouldbe no accumulation of lead at the bottom of themelt, except perhaps in the early stages of themelting of lead-containing scrap.

At steelmaking temperatures the vapor pressureof lead is about 0.5 atm and the solubility85 inliquid iron is about 0.24% Pb at 1500°C increas-ing to about 0.4% Pb at 1700°C. The free-machining leaded steels contain 0.15 to 0.35%Pb. Evidently lead added to such steels is in solu-tion in the metal prior to casting and precipitatesas small lead spheroids during the early stages offreezing.

2.4.6.2 Calcium

The boiling point of calcium is 1500°C and itssolubility in liquid iron is very low. Sponsellerand Flinn86 measured the solubility of calcium iniron at 1607°C for which the calcium vapor pres-sure is 1.69 atm. Under these conditions at1607°C, 0.032% Ca is in solution. That is, the sol-ubility at 1 atm pressure is 189 ppm Ca. They alsoinvestigated the effect of some alloying elementson the solubility; as seen from the data in Fig.2.42, C, Si, Ni and Al increase markedly the cal-cium solubility in liquid iron. In melts saturatedwith CaC2 the solubility of calcium of coursedecreases with an increasing carbon content.

%X

%X

(a) X: Ferrite stabilizer

(b) X: Austenite stabilizer

Liquid

Liquid

δ + liquid

δ

δ + γ

δ + γ

δ

δ + γ + liquid

γ + liquid

δ + γ+ liquid

γ + liquid

0 %C

0 %C

Fig. 2.41 Phase boundaries in the peritectic region ofthe Fe-C-X alloys projected on the composition diagram.

Fundamentals of Iron and Steelmaking

2.4.6.3 Magnesium

The solubility of magnesium in iron-carbon alloys determined by Trojan and Flinn87, is shown isFig. 2.43 as functions of temperature and carbon content. Subsequently, Guichelaar et al.88, madesimilar measurements with liquid Fe-Si-Mg alloys. Their data have been used in numerous studiesto derive the equilibrium relations for the solubility of magnesium in liquid iron. However, thereare some variations in the interpretation of the above mentioned experimental data. A reassessmentof these experimental data is considered desirable.

The equilibrium relation for the solubility of Mg (in units of mass % atm-1) is represented by

(2.4.32)

where fMg is the activity coefficient affected by the alloying elements. In the experiments with theFe–C–Mg melts coexistent with liquid Mg, the latter contained less than 2 percent Fe, therefore,the Mg vapor pressure prevailing in the reactor would be essentially the same as that for pure Mgfor which the following is obtained from the data of Guichelaar, et al.

(2.4.33)log .P atmTMg

o ( ) = − +67304 94

Mg g Mg

Mg f

PMgMg

Mg

( ) = [ ]

=[ ]

Κ%

0 2.5 5.0 7.5 10.0

Alloying elements (wt.%)

Ca

(wt.%

)

0

C

CaC2 − saturated

Si

Al

Ni

0.3

0.2

0.1

Fig. 2.42 Effect of alloying elements on the solubility of liquid calcium in liquid iron at 1607°C, correspond-ing to 1.69 atm pressure of calcium vapor. From Ref. 87.

Ironmaking Volume

2.4.7 Surface Tension

The experimental data for the surface tension of liquid iron and its binary alloys have been com-piled recently by Keene.89 For purified liquid iron, the average value of the surface tension at tem-perature T(°C) is represented by

σFe = (2367 ± 500) – 0.34(°C), mNm–1 (2.4.34)

Keene derived the following weighted average limiting values of (mNm-1) for dilute solutions of Xin Fe-X binary alloys.

Fe–C: Virtually no effect of C on σFeFe–Ce: σ = σFe − 700[%Ce]

Fe–Mn: σ = σFe − 51[%Mn]; ∂σ/∂T = − 0.22Fe–N: σ = σFe − 5585[%N]Fe–P: σ = σFe − 25[%P]Fe–S: (Discussed later)

Fe–Si: σ = σFe − 30[%Si]; ∂σ/∂T = − 0.25

3

2

1

02 3 4 5

Carbon (wt. %)

Mag

nesi

um (

wt.

%)

atm. Mg vapor

Carbon saturation

8.7 5.5 3.2

1426°C

1343°C

1260°C

Fig. 2.43 Solubility of magnesium in liquid iron–carbon alloys at indicated temperatures and pressures ofmagnesium vapor. From Ref. 88.

Fundamentals of Iron and Steelmaking

Gibbs’ exact treatment of surface thermodynamics gives, for fixed unit surface area and constanttemperature and pressure,

(2.4.35)

where Γi is the surface excess concentration of the ith component and ai its activity. For a ternarysystem, equation 2.4.35 is reduced to

dσ = –RT(Γ2d(ln a2) + Γ3d(ln a3)) (2.4.36)

Since carbon dissolved in iron has virtually no effect on the surface tension of liquid iron, for theternary system Fe–C–S, equation 2.4.36 is simplified to

dσ = –RTΓsd(ln as) (2.4.37)

As is seen from the compiled data in Fig. 2.44, the experimental results of various investigators forthe Fe–S melts are in close agreement. References to these data are given in an earlier publication.90

d RT di

k

i iσ = − ( )ΣΓ ln a

2000

1800

1600

1400

1200

1000

800

600

0 0.2 0.4 0.6 0.8 1.0S (mass %)

Sur

face

tens

ion

(mN

m–1

)

Fig. 2.44 Surface tension of Fe–S alloys at 1550-1600°C. From Ref. 90.

Ironmaking Volume

The classical work of Kozakevitch91 on the surface tension of Fe–C–S melts at 1450°C are repro-duced in Fig. 2.45

The points read off from the curves in Figs. 2.44 and 2.45 are plotted in Fig. 2.46 as σ versus logaS. It is seen that for aS (%S x fS) > 0.01, σ is a linear function of log aS, a limiting case for almostcomplete surface coverage with chemisorbed S. The shaded area represents the data of Selcuk andKirkwood92 for 1200°C.

0 0.4 0.8 1.2 1.6 2.0 2.4Sulfur activity

1300

1100

900

700

500

Sur

face

tens

ion

(mN

m–1

)

Fig. 2.45 Surface tension of liquid Fe–C–S alloys at 1450°C. From Ref. 91.

(Fe–S) 1575°C

(Fe–C–Si–S) 1200°C

Sur

fact

tens

ion

(mN

m–1

)

–3 –2 –1 0

2000

1800

1600

1400

1200

1000

800

600

Log aS

(Fe–C–S) 1450°C

Fig. 2.46 Surface tension of Fe–S,Fe–C–S and Fe–C–Si–S alloys related tosulfur activity; aS→%S when %C and%Si→0. From Ref. 90.

Fundamentals of Iron and Steelmaking

Numerous studies have been made of the surface tension of the Fe–O melts. The more recent exper-imental data93,94 are reproduced in Fig. 2.47. At oxygen activities aO (%O x fO) > 0.1, there is essen-tially complete surface coverage with the chemisorbed oxygen.

2200

2000

1800

1600

1400

1200

1000

800–9 –8 –7 –6 –5 –4 –3 –2 –1

Jimbo and Cramb93

Kasama et al94

Sur

face

tens

ion

(mN

m–1

)

Γ ° O ≈ 1.1 x 1019 mol m–2

In a O

Fig. 2.47 Effect of oxygen on surface tension of liquid iron at 1550°C.

2.4.8 DensityThe temperature dependence of the densities of liquid iron, nickel, cobalt, copper, chromium, man-ganese, vanadium and titanium are given by the following equations as a linear function of tem-perature in °C in g cm–3:

Iron: 8.30 – 8.36 × 10–4TNickel: 9.60 – 12.00 × 10–4TCobalt: 9.57 – 10.17 × 10–4TCopper: 9.11 – 9.44 × 10–4TChromium: 7.83 – 7.23 × 10–4TManganese: 7.17 – 9.30 × 10–4TVanadium: 6.06 – 3.20 × 10–4TTitanium: 4.58 – 2.26 × 10–4T

The specific volume and density of liquid iron-carbon alloys are given in Fig. 2.48 for various tem-peratures. It should be noted that the density of the liquid in equilibrium with austenite does notchange much over the entire liquidus range.

2.4.9 ViscosityThe viscosity is a measure of resistance of the fluid to flow when subjected to an external force. Asconceived by Newton, the shear stress ε, i.e. force per unit area, causing a relative motion of two adja-cent layers in a fluid is proportional to the velocity gradient du/dz, normal to the direction of theapplied force

(2.4.38)

where the proportionality factor η is viscosity of the fluid (liquid or gas).

ε η= dudz

Ironmaking Volume

Viscosity unit: poise (g cm-1s–1) ≡ 0.1N s m–2.

The viscosities of Fe–C alloys determined by Barfield and Kitchener96 are given in Fig. 2.49. In theiron-carbon melts the coefficient of viscosity is essentially independent of composition within therange 0.8 to 2.5% C; above 2.5% C, the viscosity decreases continously with an increasing carboncontent.

2.4.10 Diffusivity, Electrical and Thermal Conductivity, and Thermal Diffusivity

The diffusivity is an exponential function of temperature,

(2.4.39)

where Do is a constant for a given solute and E the activation energy (enthalpy) for the diffusionprocess.

D DE

RT= −

o exp

Carbon concentrations / atom %

Spe

cific

vol

ume

(cm

3 /g)

Austenite liquidus

0 2 4 6 8 10 12 14 16 18 20

wt. (%)0 1 2 3 4 5

6.5

6.6

6.7

6.8

6.9

7.0

7.1

7.2

Den

sity

(g/

cm3 )

1600°C1500°C

1400°C1300°C

0.155

0.150

0.145

0.140

Fig. 2.48 Density of iron-carbonalloys. From Ref. 95.

5.0 5.5 6.0 6.5Carbon wt % 1/T x 104 (K-1)

0.08

0.07

0.06

0.05

Vis

cosi

ty 0

.1N

s m

-2

1500°C

1550°C

1600°C

1400°C

1450°C

0 1.0 2.0 3.0 4.0

log

η (0

.1N

s m

-2)

4.40

3.43

2.10

2.53

X

X

X

-1.0

-1.1

-1.2

-1.3

-1.4

0.75

Fig. 2.49 Composition and temperature dependence of the viscosity coefficient of iron-carbon melts. FromRef. 96.

Fundamentals of Iron and Steelmaking

The general trend in the temperature dependence of solute diffusivity in solid iron is shown in Fig.2.50. The interstitial elements, e.g. O, N, C, B, H have diffusivities much greater than the substitu-tional elements. Because of larger interatomic spacing, the diffusivities of interstitials in bcc-ironare greater and the heats of activations (∼ 85 kJ) are smaller than those in the fcc-iron with E ~ 170kJ. With the substitutional elements, the heat of activation is within 210 to 250 kJ for bcc-iron andwithin 250 to 290 kJ for fcc-iron.

In liquid iron alloys, diffusivities of elements are within 10–5 to 10–4 cm2s-1 with E within 15 to 50 kJ.

Some solute diffusivity data for liquid iron and iron-carbon alloys are given in Table 2.11.

Table 2.11 Selected Solute Diffusivities in Liquid Fe-C Alloys

Diffusing Concentration Temp. D Do Eelement mass % Medium range °C cm2sec–1 cm2sec–1 kJC 0.03 Fe 1550 7.9x10–5 – –C 2.1 Fe 1550 7.8x10–5 – –C 3.5 Fe 1550 6.7x10–5 – –Co Dilute sol. Fe 1568 4.7x10–5 – –Co Dilute sol. Fe 1638 5.3x10–5 – –Fe – Fe–4.6%C 1240–1360 – 4.3x10–3 51Fe Fe–2.5%C 1340–1400 – 1.0x10–2 66H Dilute sol. Fe 1565–1679 – 3.2x10–3 14Mn 2.5 gr.satu.Fe 1300–1600 – 1.93x10–4 24N Dilute sol. Fe 1600 1.1x10–4 – –N Dilute sol. Fe–0.15%C 1600 5.6x10–5 – –O Dilute sol. Fe 1600 5.0x10–5 – –P Dilute sol. Fe 1550 4.7x10–5 – –S <0.64 gr.satu.Fe 1390–1560 – 2.8x10–4 31S ~1 Fe 1560–1670 – 4.9x10–4 36Si <2.5 Fe 1480 2.4x10–5 – –Si <1.3 Fe 1540 3.8x10–5 – –Si 1.5 gr.satu.Fe 1400–1600 – 2.4x10–4 34

The electrical conductivity λ in the units of Ω–1cm–1 is the reciprocal of the electrical resistivity. Theelectrical conductivity of liquid low alloy steel is about λ = 7140 Ω–1cm–1 at steelmaking temperatures.

From Fick’s law, the thermal conductivity is defined by

(2.4.40)

where Q is heat flux, energy per unit per unit time, ∂T/∂x the temperature gradient normal to thedirection of heat flow and κ the thermal conductivity.

Units of κ: J cm–1s–1K–1 ≡ 10–2 kg m s–3K–1 ≡ 10–2 Wm–1K–1

The effect of temperature on the thermal conductivities of iron, carbon steels and high alloy steelsare shown in Fig. 2.51.

Analogous to mass diffusivity, the thermal diffusivity is defined as

(2.4.41)

where ρ is density and Cp molar heat capacity. In metals, the electrons migrate at much faster ratesthan the atoms; therefore the thermal diffusivity is much greater than the mass diffusivity.

For low–alloy steels at 1000°C:

α ≈ 0.04 cm2s–1

D ≈ 3 × 10–12 cm2s–1 (substitutional)D ≈ 3 × 10–7 cm2s–1 (interstitial)

α κρ

= −

Ccm s

p

2 1

κ∂ ∂

= − QT x

Ironmaking Volume

1600 1400 1200 1000 800 600°C

5 6 7 8 9 10 11104/T (K–1)

10–4

10–5

10–6

10–7

10–10

10–11

10–12

Diff

usiv

ity (

cm2 /s

ec.)

Interstitials in bcc-Fe

Interstitials in fcc-Fe

Substitutional in bcc-Fe

Substitutional in fcc-Fe

Temperature (°C)

The

rmal

con

duct

ivity

(W

m–1

K–1

)

80

64

48

32

160 200 400 600 800 1000

Purified iron

High alloy steels

Carbon steels

Fig. 2.50 Range of diffusivities ofinterstitial and substitutional ele-ments in bcc and fcc iron.

Fig. 2.51 Temperaturedependence of thermalconductivity of purifiediron and iron alloys.

Fundamentals of Iron and Steelmaking

2.5 Properties of Molten Slags

2.5.1 Structural Aspects

Molten slags are ionic in nature consisting of positively charged ions known as cations, and nega-tively charged complex silicate, aluminate and phosphate ions known as anions.

The fundamental building unit in solid silica and molten silicates is the silicate tetrahedron SiO44–.

Each silicon atom is tetrahedrally surrounded by four oxygen atoms and each oxygen atom isbonded to two silicon atoms. The valency of silicon is +4 and that of oxygen is –2, therefore thesilicate tetrahedron has 4 negative charges.

The addition of metal oxides such as FeO, CaO, MgO, . . . to molten silica brings about a break-down of the silicate network, represented in a general form by the reaction

(2.5.1)

The cations are dispersed within the broken silicate network. In MO–SiO2 melts the atom ratioO/Si > 2, therefore part of the oxygen atoms are bonded between two silicon atoms and part to onlyone silicon atom. Partial depolymerization of the silicate network with the addition of a metal oxideMO is illustrated in Fig. 2.52.

Si Si + MO 2 Si O| | |

|| |O M

+

−+2

Fig. 2.52 Schematic representationof depolymerization of the silicatenetwork with the dissolution of metaloxides in silicate melts.

In highly basic slags with molar ratio MO/SiO2 > 2, the silicate network completely breaks downto individual SiO4 tetrahedra intermixed with cations M2+ and some oxygen ions O2–.

At low concentrations, Al2O3 behaves like a network-modifying oxide and forms aluminum cationsAl3+. At high concentrations, the aluminum enters the tetrahedral structure isomorphous with silicon.

This process may be schematically represented by the reaction

(2.5.2)

The cation M+ is located in the vicinity of Al–O bonding to preserve the local charge balance. At lowconcentrations of phosphorus in steelmaking slags, the phosphate ions PO4

3– are incorporated in thesilicate network. In steelmaking slags, the sulfur exists as a sulfide ion S2–. The sulfate ions SO4

2– existin slags only under highly oxidizing conditions and in the absence of iron or any other oxidizable metal.

Si O Si + MAlO O Al

O

O Si + M|

|

|

|

2|

|+

Si|

|

|

|

Ironmaking Volume

Although molten slags are ionized, the slag composition can be represented in terms of the con-stituent oxides, e.g. CaO, FeO, SiO2, P2O5. The thermodynamic activity of an ion in the slag can-not be determined. However, the activity of an oxide dissolved in molten slag, forming M2+ andO2– ions, can be determined experimentally and the following equality can be written

MO → M2+ + O2– (2.5.3)

(2.5.4)

where the superscript ° refers to the standard state which is usually pure solid or liquid oxide.

2.5.2 Slag BasicityFor steelmaking slags of low phosphorus content, the slag basicity has traditionally been repre-sented by the mass concentration ratio

(2.5.5)

For slags containing high concentrations of MgO and P2O5, as in some laboratory experiments, thebasicity may be defined by the following mass concentration ratio, with the assumption that on amolar basis the concentrations of CaO and MgO are equivalent. Similarly, on a molar basis 1/2P2O5, i.e. PO2.5, is equivalent to SiO2.

(2.5.6)

For slags containing MgO < 8% and P2O5 < 5%, the basicity B is essentially directly proportionalto V.

B = 1.17V (2.5.7)

Another measure of slag basicity is the difference between the sum of the concentrations of basicoxides and acidic oxides.

(%CaO + %MgO + %MnO) – (%SiO2 + P2O5 + TiO2) (2.5.8)

This formulation of slag basicity is not used very often.

For the calcium aluminate type of slags used in steel refining in the ladle furnace, the slag basic-ity used in some German and Japanese publications, is defined by the ratio

(2.5.9)

However, such a ratio becomes meaningless at low concentrations of either SiO2 or Al2O3. For theladle furnace slag the basicity may be defined by the following mass concentration ratio, on theassumption that on a molar basis Al2O3 is equivalent to SiO2.

(2.5.10)

The slag basicities as defined above are for the compositions of molten slags. In practice, the steel-making slags often contain undissolved CaO and MgO. The chemical analyses of such slag sam-ples without correction for undissolved CaO and MgO, will give unrealistic basicities which aremuch higher than those in the molten part of the slag.

There has been a trend in recent years to relate some physiochemical properties of slags, such assulfide capacity, phosphate capacity, carbide capacity, etc., to optical slag basicity. The opticalbasicity is discussed briefly in Section 2.5.12.

BCaO MgO

SiO Al OLF = + ×+ ×

% . %% . %

1 40 62 2 3

%% %

CaOSiO Al O2 2 3×

BCaO MgO

SiO P O= + ×

+ ×% . %

% . %1 40 842 2 5

VCaOSiO

= %% 2

a

a

a a

a a

MO

MO

M O

M O( )

=( )( )

+ −

+ −

o o

2 2

2 2

Fundamentals of Iron and Steelmaking

2.5.3 Iron Oxide in SlagsIron oxide dissolves in slags in two valency states: divalent iron cations Fe2+ and trivalent ironcations Fe3+. The ratio Fe3+/ Fe2+ depends on temperature, oxygen potential and slag composition;this is discussed later in this section. In the formulation of the equilibrium constants of slag-metalreactions and the thermodynamic activities of oxides in slags, the total iron dissolved in the slag asoxides is usually converted to the stoichiometric formula FeO and denoted by FetO, thus

%FetO = %FeO (analyzed) + 0.9 x %Fe2O3 (analyzed) (2.5.11)or

%FetO = 1.286 x %Fe (total as oxides) (2.5.12)

For the ease of understanding, the subscript t will be omitted in all the subsequent equations anddiagrams.

2.5.4 Selected Ternary and Quaternary Oxide SystemsMost steelmaking slags consist primarily of CaO, MgO, SiO2 and FeO. In low-phosphorus steel-making practices, the total concentration of these oxides in liquid slags is in the range 88 to 92%.Therefore, the simplest type of steelmaking slag to be considered is the quaternary systemCaO–MgO–SiO2–FeO.

First let us consider the ternary system CaO·SiO2–FeO; the liquidus isotherms of this system isshown in Fig. 2.53. The isothermal section of the composition diagram in Fig. 2.54 shows the phaseequilibria at 1600°C.

90 10

60 20

40 60

30 70

20 80

10 90

2000

SiO2

Cristobalite

TroymitePseudowollastonite

OlivineCaO.FeO.SiO2O

Ca2SiO4

Lime

Rankinite

Weight %

CaO 10 20 30 40 50 60 70 80 90 FeO

FeO.SiO2

2FeO.SiO2

CaO.SiO2

3CaO.2SiO2

2CaO.SiO2

3CaO.SiO2

50

40

70

1700

1700

1600150014001300

1200Wollastonite 1150

1500

1400

13001250

12001150

1100

1150

1200

12001250

1300

2500

2400

23002200 2100

1900 1800 1700 1600 1500

2100

2000

1900

1800

1700

1600

15001400

1300

Wustite

II-Ca2SiO4

Ca3 SiO

5

Fig. 2.53 Liquidus isotherms of CaO–SiO2–FeO system.

Ironmaking Volume

There are four two-phase regions where, as depicted by dotted lines, the melt is saturated withSiO2, 2CaO·SiO2, 3CaO·SiO2 or CaO; two three-phase regions (2CaO·SiO2 + 3CaO·SiO2 + liquid)and (3CaO·SiO2 + CaO + liquid); and one liquid phase region.

Magnesia is another important ingredient of steelmaking slags, which are invariably saturated withMgO to minimize slag attack on the magnesia refractory lining of the furnace.

The effect of MgO on the solubility of calcium silicates and calcium oxide is shown in Fig 2.55 for the system (CaO + MgO)–SiO2–FeO, in equilibrium with liquid iron at 1600°C.

80 20

60 40

40 60

20 80

CaO

(wt%

) SiO2 (w

t%)

2CaO-SiO2

3CaO-SiO2

20 40 60 80

FeO (wt%)

liquid

SiO2

FeOCaO

Fig. 2.54 Phase equilibrium inthe system CaO–SiO2–FeO inequilibrium with liquid iron at1600°C.

40 60

60 40

80 20

20 80

SiO2 + liquid

CaO

+ M

gO (w

t%)

SiO2 (w

t%)Liquid

Silicate + liquid

0% MgO

Silicate + Ca(Mg)O +Mg(Fe)O→ liquid

Ca(Mg)O + Mg(Fe)O → liquid

FeO (wt%)20 40 60 80

108

64

2

SiO2

FeOCao + MgO

Fig. 2.55 Effect of MgO (wt.%) onthe solubility isotherms at 1600°Cin the system (CaO + MgO)–SiO2–FeO in equilibrium with liq-uid iron.

Fundamentals of Iron and Steelmaking

The broken-line curve delineates the region of saturation of molten slag with solid calcium (magne-sium) silicates and solid magnesio-wustite (MgO–FeO solid solution). Effects of the concentrationsof MgO and FeO on the solubility of CaO in 2CaO·SiO2-saturated slags are shown in Fig. 2.56.

Tromel et al.97 have made a detailed study of the solubility of MgO in iron–calcium silicate meltsin equilibrium with liquid iron at 1600°C. Below the dotted curve BACD in Fig. 2.57 for doublesaturations, the curves for 10 to 60% FeO are the MgO solubilities in the slag.

MgO (%)

FeO (mass %)

60

55

50

45

40

2

8CaO

(m

ass

%)

0 10 20 30

Fig. 2.56 Solubility of CaO in(CaO–MgO–SiO2–FeO) slagssaturated with 2CaO·SiO2 at1600°C.

0 1 2 3 4 5

olivine + 2MgO SiO2

Mg(Fe)O + Mg(Ca)O

10% FeO

A

20

30

40

B C

Mg(Fe)O + 2Ca(Mg)O SiO2

60

D

Mg(Fe)O + Ca(Mg)O

olivine+

Mg(Fe)O

MgO

(w

t %)

32

24

16

8

%CaO%SiO2

Fig. 2.57 Solubility of MgO, as magnesio–wustite, in the system CaO–MgO–SiO2–FeO at 1600°C as a func-tion of slag basicity and FeO concentration. From Ref. 97.

Ironmaking Volume

Pertinent to the compositions of neutral ladle slags, the phase equilibria in part of the systemCaO–Al2O3–SiO2 at 1600°C is shown in Fig. 2.58.

2.5.5 Oxide Activities in Slags

In this section the activity data are given for a few ternary and multicomponent systems which areclosely related to the iron and steelmaking slags.

2.5.5.1 Activities in CaO – FeO–SiO2 System

The oxide activities in the CaO–FeO–SiO2 melts relevant to oxygen steelmaking in equilibriumwith liquid iron at about 1550°C are given in Fig. 2.59. The iso-activity curves in the left dia-gram represent the experimentally determined activities of iron oxide with respect to liquidFeO.98–99 The activities of CaO and SiO2 with respect to solid oxides were calculated from theFeO activities by Gibbs-Duhem integration.99

CaO 10 20 30 40 50 60 70 80 90 Al2O3

liquid

Mass (%) CaO•2Al2O3 CaO•6Al2O3

2CaO•SiO2

3CaO•SiO23Al2O3•2SiO2

70

80

90

SiO2

30

20

10

Fig. 2.58 Phase equilibria in the system CaO–Al2O3–SiO2 at 1600°C.

0.4 0.6

CaO 0.2 0.4 0.6 0.8 FeO

(0.9)(0.7)

(0.6)

(0.4)

(0.2)

(0.1)(0.05)

(0.001)(0.0005)

0.6 0.4

0.8 0.2

0.2 0.8SiO2♦ liq .

0.10.2

0.3

0.4

0.50.6

0.7

0.8

0.9

C2S ♦ liq.

aFeO(1)

0.4 0.6

CaO 0.2 0.4 0.6 0.8 FeO

N CaO

NSiO

2

NFeO

0.6 0.4

aSiO2(s)

aCaO(s)

0.8 0.2

NFeO

N CaO

NSiO

2

0.0020.006

0.01

0.1

0.2

0.4

Fig. 2.59 Activities of FeO(l) (experimental), CaO(s) and SiO2(s) (by Gibbs-Duhem integration) inCaO–FeO–SiO2 melts in equilibrium with liquid iron at 1550°C. From Refs. 98, 99.

Fundamentals of Iron and Steelmaking

Recently new iron smelting processes have been developed and are briefly discussed here. Theslags are CaO–SiO2–FeO–A12O3–MgO (saturated) with low FeO contents (<5%). Knowledgeof the activity of FeO in these slags is critical and has been recently measured by Liu et al.100

The activity coefficient of FeO in these slags is given in Fig. 2.60 and is approximately 3.5. Itincreases slightly with basicity as shown in Fig. 2.61 but is nearly constant with a value of 3.5.

0.00 0.01 0.02 0.03 0.04 0.05

· Liu et al

Temperature: 1550°CBasicity (wt% CaO/ wt%SiO2): 0.79 – 1.23

Al2O3 Content (wt%): 6.31 – 8.04

FeO

act

ivity

coe

ffici

ent

FeO mole fraction

10.00

8.00

6.00

4.00

2.00

0.00

Fig. 2.60 The activity of FeO in CaO–SiO2–Al2O3–FeO–MgO (saturated) slags relevant to iron smelting. FromRef. 100.

1.50 2.00 2.50 3.00

10.00

8.00

6.00

4.00

2.00

0.00

FeO

act

ivity

coe

ffici

ent

Liu et al

Temperature: 1550°CFeO content: 0.7 – 4.7

Al2O3 content: 6.3 – 8.0

(CaO+MgO)SiO2

Slag basicity,

Fig. 2.61 The effect of slag basicity on the activity coefficient of FeO in CaO–SiO2–Al2O3–FeO–MgO(saturated) slags relevant to iron smelting. From Ref. 100.

Ironmaking Volume

2.5.5.2 Activities in CaO–Al2O3–SiO2 System

Rein and Chipman101 measured the activity of silica in the CaO–Al2O3–SiO2 system; from theseexperimental data they calculated the activities of CaO and Al2O3 by Gibbs-Duhem integration.The salient features of these oxide activities at 1600°C, with respect to solid oxides, are shown inFig. 2.62 for the mass ratios of CaO/Al2O3 = 2/3 and 3/2; the compositions of ladle slags are wellwithin the range given in Fig. 2.62.

Rein and Chipman also measured the activity of silica in the quaternary melts CaO–MgO–Al2O3–SiO2.The activity coefficients of SiO2 derived from these data are given in Fig. 2.63 for melts contain-ing 10% MgO and 0, 10 or 20% Al2O3.

SiO

2 ac

tivity

CaOAl2O3

2/3

3/2

Mass % SiO20 10 20 30

Al 2

O3

activ

ity

CaOAl2O3

2/3

3/2

0.5

0.4

0.3

0.2

0.1

00 10 20 30

Mass % SiO2

10–1

10–2

10–3

10–4

Fig. 2.62 Silica and alu-mina activities, with re-spect to solid oxides, inCaO–Al2O3–SiO2 meltsat 1600°C, derived fromexperimental data ofRein and Chipman.101

0.4 0.8 1.2 1.6

1.6

1.2

0.8

0.4

0

Act

ivity

coe

ffici

ent o

f SiO

2

0

20

10

% CaO + % MgO% SiO2

Fig. 2.63 Activity coefficient of SiO2 withrespect to pure solid oxide, in CaO–MgO–Al2O3–SiO2 melts at 1600°C, con-taining 10% MgO and 0, 10 or 20%Al2O3, derived from experimental data ofRein and Chipman101.

Fundamentals of Iron and Steelmaking

The ratio of the activities (aAl2O3)1/3/aCaO within the entire liquid composition range up to 30% SiO2

is shown in Fig. 2.64 reproduced from Ref. 27.

2.5.5.3 Activities in MnO–Al2O3–SiO2 System

In the deoxidation of steel with the ladle addition of silicomanganese and aluminum together, thedeoxidation product is molten manganese aluminosilicate with the mass ratio MnO/SiO2 at about1:1 and containing 10 to 45% Al2O3. The activities of oxides in the MnO–Al2O3–SiO2 melts at1550 and 1650°C were computed by Fujisawa and Sakao102 from the available thermochemical dataon the system. They also determined experimentally the activities of MnO and SiO2 by the selectedslag-metal equilibrium measurements and found a close agreement with the computed data.

The activities of Al2O3 and SiO2, with respect to solid oxides, are plotted in Fig. 2.65 for melts withmass ratio of MnO/SiO2 = 1. For melts containing up to 30% Al2O3 the activity of MnO remainsessentially unchanged at about 0.1 then decreases to about 0.05 at 40% Al2O3.

2.5.5.4 Activity Coefficient of FeO in Slags

With hypothetical pure liquid FeO as the standard state, the activity of iron oxide is derived fromthe concentration of dissolved oxygen in liquid iron that is in equilibrium with the slag. For thereaction equilibrium

FeO(l) = Fe + [O] (2.5.13)

(2.5.14)

where aO = [%O]fO, using log fO = – 0.1×[%O]. The temperature dependence of the equilibriumconstant KO is given below.

(2.5.15)log .ΚO T= − +5370

2 397

ΚOO

FeO

= [ ]a

a

Silica (mass%)

Saturated with

CaO

Ca2SiO4

Ca3SiO5

Saturated with

CaO/Al2O3 = 1.0

0 5 10 15 20 25 30

Molten aluminosilicate

CaAl4O7

CaAl12O19

(a A

l 2O

3)1 /

3(a

CaO

)

40

10

4

1.0

0.4

0.1

100

Fig. 2.64 Effect of slag compositionon the activity ratio (aAl2O3

)1/3/aCaOfor the system CaO–Al2O3–SiO2 at1600°C. From Ref. 27.

In the past a wide variety of formulations were generated to represent the composition dependenceof the iron oxide activity or activity coefficient in complex slag. On a recent reassessment of thisproperty of the slag, Turkdogan103 came to the conclusion that, within the limits of uncertainty ofthe experimental data on slag-metal reaction equi-librium, there is a decisive correlation between theactivity coefficient of FeO and the slag basicity asshown in Fig. 2.66. The γFeO reaches a peak at abasicity of about B = 1.8. It should be pointed outonce again that the concentration of iron oxide isfor total iron as oxides in the slag represented bythe stoichiometric formula FeO.

As discussed in Ref. 103, the experimental dataused in deriving the relation in Fig. 2.66 are forsimple and complex slags which differ consider-ably in their compositions thus: in mass percent,CaO 0–60, MgO 0–20, SiO2 0–35, P2O5 0–20,FeO 5–40, MnO 0–15.

2.5.5.5 Activity of MnO in Slags

The activity coefficient ratio γ FeO/γ Mno, derivedfrom the slag-metal equilibrium data cited in Ref.103, varies with slag basicity as shown in Fig.2.67. There is a sharp decrease in the ratio of theactivity coefficients as the basicity B increasesfrom 1.5 to 2.0. At basicities above 2.5, the ratioγFeO/γMnO is essentially constant at about 0.63. Thecurve for γMnO in Fig. 2.66 is that derived from thecombination of the curve for γFeO with the ratio inFig. 2.67.

0 5 10 15 20 25 30 35 40 45Mass % Al2O3

1550°C

1650°C

Al 2

O3

and

SiO

2 ac

tiviti

es

a SiO21650°C1550°C

a Al2O3

1.0

0.8

0.6

0.4

0.2

0

Fig. 2.65 Al2O3 and SiO2 activities in MnO–Al2O3–SiO2 system for mass ratio MnO/SiO2 = 1, derived fromdata compiled by Fujisawa & Sakao102.

4

3

2

1

0

B0 2 4 6

γ F

eO a

nd γ

MnO

γ MnOγ FeO

Fig. 2.66 Effect of slag basicity B on the activitycoefficients of FeO and MnO, with respect to pureliquid oxides, in simple and complex slags at tem-peratures of 1550 to 1700°C. From compiled datain Ref. 103.

Ironmaking Volume

2.5.6 Gas Solubility in Slags

2.5.6.1 Solubility of H2O

In acidic melts, H2O vapor reacts with doublebonded oxygen and depolymerizes the melt, thus

In basic melts, H2O reacts with free oxygen ions

(O2–) + H2O = 2(OH)– (2.5.16)

Both for acidic and basic melts the overall reaction isrepresented by

(O*) + H2O = 2(OH*) (2.5.17)

where O* represents double or single bonded oxygen,or O2–, and OH* is single bonded to silicon or as a freeion. The equilibrium constant for a given melt compo-sition is

(2.5.18)

where PH2O is the vapor partial pressure.

The solubilities of H2O (in units of mass ppm H2O) at1 atm pressure of H2O vapor in CaO–FeO–SiO2 at 1550°C, measured by Iguchi et al.104 are given inFig. 2.68.

Cppm H O

pOH

H O

= ( )( )

21 2

2

/

Si O Si OH|

|

|

|

|

|

+ =

H O Si2 2

5

4

3

2

1

00 2 4 6

B

γ FeO

γ MnO

Fig. 2.67 Variation of activity coefficient ratiowith basicity. From Ref. 103.

Al2O3 (wt%)

SiO2

Al2O3

Mullite

SilicateCorondum

Cris

toba

lite

liquid

500

600

650

800 750

1000

2000

2500

1400

CaO 10 20 30 40 50 60 70

Al2O3

10 90

20 80

30 70

40 60

50 50

60

70

80

90

Fig. 2.68 Hydroxyl capacity, COH ofCaO–FeO–SiO2 and CaO–Al2O3–SiO2melts at 1500°C. From Ref.104.

30

40

50

60

701300 1050

650

600

650

SiO2

FeO (wt%)

30

40

50

60

70

CaO FeO10 20 30 40 50 60

Fundamentals of Iron and Steelmaking

Ironmaking Volume

2.5.6.2 Solubility of N2

Nitrogen dissolves in molten slags as a nitride ion N3– only under reducing conditions1/2N2(g) + 3/2(O2–) = (N3–) + 3/4O2(g) (2.5.19)

for which the equilibrium constant (known as nitride capacity) is

(2.5.20)

Many studies have been made of the solubility of nitrogen in CaO–Al2O3 and CaO–Al2O3–SiO2 meltsin the 1970s. These were reviewed in a previous publication3. Reference should be made also to a sub-sequent work done by Ito and Fruehan105 on the nitrogen solubility in the CaO– Al2O3–SiO2 melts. Theyshowed that the nitride capacity of the aluminosilicate melts increases with a decreasing activity of CaO.

2.5.6.2.1 Nitrogen Dissolution into Slags The nitride capacity in certain slag systems increases and inothers decreases with basicity. According to equation 2.5.19 one would expect it to increase withincreasing slag basicity, i.e. increasing concentration of free oxygen ion O2–. The reason for thisapparent contradiction is that nitrogen can enter the slag by replacing single bonded oxygen ionsin the SiO2 network. This phenomena is explained in detail by Ito and Fruehan.105

Briefly, spectroscopic research indicates that the nitrogen is combined with the network former insilicate melts which can be represented by

(2O–) + 1/2N2 =(N–) + 1/2 (O2–) + 3/4 O2 (2.5.21)

where O– is a nonbridging system in the network. If SiO2 is the network former equation 2.5.21corresponds to

(2.5.22)

In this case the nitride capacity is given by

(2.5.23)

where K is an equilibrium constant for reaction 2.5.21, fi is an activity coefficient for species i. In thiscase N3– does not mean a freenitride ion but the nitrogen analyzedas a nitride which is associated withthe network former. Similar reac-tions can be written for bridgingoxygen, but then reactions are lesslikely. In either case the nitridecapacity decreases with oxygen ionactivity, i.e. increasing slag basicity.

For the CaO–SiO2, CaO–Al2O3,and CaO–SiO2–Al2O3 systems CaOis the basic component. Thereforethe equations predict that a plot ofthe logarithm of nitride capacityversus the logarithm of the activityof CaO should yield a straight linewith a slope of –1⁄2 as shown in Fig.2.69.

CN p

p fN

O

N

O

N O

32

34

2

12

2

12

3

− −

=( )( )

( )=

( )−%

Κa

a

O Si O =- -

|

|

|

|

+ =

+ ( ) +− −1

2 21

22 3

4 2N Si N O O

C Np

pNO

N

= ( )% 2

34

2

12

–12

–13

–14 –3 –2 –1 0log a

CaO

log

CN

3–

CaO – SiO2 – Al2O3

CaO – SiO2

CaO – Al2O3

1823 K

1

2

Fig. 2.69 The relation between the nitride capacity and the activ-ity of lime for CaO–SiO2–Al2O3 slag at 1823 K. Ref. 105.

Fundamentals of Iron and Steelmaking

For highly basic oxide systems the nitrogen enters as a free nitride ion and the simple relationshipgiven by 2.5.19 is valid. In this case the free nitride concentration and the nitride capacity is pro-portional to the oxygen ion activity to the 3/2 power (aO2–)3/2. Min and Fruehan106 have shown thatthe nitride capacity does increase with basicity for highly basic slags, particularly when there is nostrong network former such as SiO2 present. In theory the nitride capacity should decrease withbasicity when the nitrogen is primarily in the network and increase when it is a free nitride. Thiswas observed for the BaO–B2O3 and CaO–B2O3 system as shown in Fig. 2.70.

–12

–13

–14

: CaO–B2O3, 1773 K

log

CN

3–

1

2

3

2: BaO–B2O3, 1698 K

log a MO

–4 –3 –2 –1 0

Fig. 2.70 Nitride capacity of the slagsas a function of the activity of CaO orBaO. From Ref. 106.

2.5.6.2.2 Nitrogen Removal by Slags For Al-killed steels the corresponding equilibrium partial pres-sure of oxygen is

(2.5.24)

From the solubility data for nitrogen we have

(2.5.25)

Substituting these in the equation for CN gives

In lime-rich aluminate ladle slags of low SiO2 content, the lime activity is aCaO = 0.5 for which CN = 10–13. These give the following equilibrium relation

Dissolved [%Al] (%N) / [%N]______________ ___________0.005 0.00950.02 0.0380.06 0.1140.10 0.190

%%

. %NN

Al( )[ ]

= × [ ]1 9

CN

N AlN = ( )[ ][ ]

× × −%% %

.5 3 10 14

p NN 2

12 1

2 21 9( ) = [ ] (atm) at 1600 C. % o

pAlO 2

43

1 22 10 16

(atm) at 1600 C= ×[ ]

−.

%o

Ironmaking Volume

The equilibrium nitrogen distribution ratio between slag and steel is very low even at high alu-minum contents, well above the practical range. The slag/steel mass ratio in the ladle is also low,about 1/100. For these reasons, liquid steel in the ladle cannot be de-nitrogenized by the slag thatis usable in industry in steel refining.

As noted from the recent experimental studies of Fruehan and co-workers,106–108 that even with fluxesof high nitride capacities (as with alkaline earth borates) it is not practically possible to remove nitro-gen from the aluminum-killed steel in the ladle. The highest nitride capacity was for a slag containingabout 22% CaO – 27% BaO – 48% Al2O3 – 3% TiO2 and was about 5 × 10–12. For this case for a steelcontaining 0.06% Al the nitrogen distribution ratio is about 5.5 which is still not high enough for effec-tive nitrogen removal.

2.5.6.3 Solubility of S2

Sulfur-bearing gases dissolve in molten slags as sulfide ions (S2–) under reducing conditions, andas sulfate ions (SO4

2–) under highly oxidizing conditions. In steelmaking the oxygen potential isnot high enough for the solution of sulfur as sulfate ions, therefore we need to consider only thesulfide reaction.

Whether the sulfur-bearing species is primarily H2S or SO2, there is a corresponding equilibriumvalue of pS2

depending on the temperature and gas composition. It is convenient to consider thereaction in a general form as

1/2S2(g) + (O2–) = (S2–) + 1/2O2(g) (2.5.26)

For a given slag composition the equilibrium relation is represented by

(2.5.27)

where p’s are equilibrium gas partial pressures. The equilibrium constant CS is known as the sul-fide capacity of the slag. The value of CS depends on slag composition and temperature.

Experimentally determined sulfide capacities of binary oxide melts are shown in Fig. 2.71. Refer-ences to experimental data are given in Ref. 3.

For the slag-metal system, the sulfur reaction is formulated in terms of the activities

(≅ concentrations) of sulfur and oxygen dissolved in the steel.

[S] + (O2–) = (S2–) + [O] (2.5.28)

For low-alloy steels

(2.5.29)

where the equilibrium constant kS depends on slag composition and temperature.

2.5.6.3.1 Conversion of pO2/ pS2

to [%O]/[%S] The free energies of solution of O2 and S2 in liquid lowalloy steel are given below; see Table 2.1 in section 2.1.2.4.2.

1/2S2 = [S]; ∆Gs = –135,060 + 23.43TJ (2.5.30)

1/2O2 = [O]; ∆Go = –115,750 – 4.63TJ (2.5.31)

For the reaction equilibrium

1/2S2 = [O] = 1/2O2 + [S]

the standard free energy change is

∆G° = ∆Gs – ∆Go = –19,310 + 28.06TJ (2.5.32)

kSS

OS = ( )[ ] [ ]%%

%

C Sp

pSO

S

= ( )

% 2

2

12

Fundamentals of Iron and Steelmaking

(2.5.33)

For steelmaking temperatures an average value of K is 0.133; with this conversion factor the fol-lowing is obtained.

(2.5.34)

With this substitution the values of CS are converted to kS.

(2.5.35)7 5.%%

%× = = ( )[ ] [ ]C k

SS

OS S

p

pOS

O

S

2

2

12

0 133

= [ ]

[ ].

%%

log%%

.p

pSO T

O

S

2

2

12

10091 466

[ ][ ]

= −

0 20 40 60 80 100

CS

(wt %

)

10–1

10–2

10–3

10–4

10–5

1350°C

1500°C

1650°C

1622°C

CaO–FeOx

'FeO'

MnO–Al2O3

CaO–Al2O3

MnO–SiO2

Na2O–SiO2

CaO–P2O5

CaO(cryst.)

1650°CMgO–SiO2

CaO–SiO2

Al2O3–SiO2

Basic oxide (mol. %)

Fig. 2.71 Sulfide capacities ofbinary oxide melts. From Ref. 3.

Ironmaking Volume

A slag of high kS value and steel deoxidation to low levels of [O] are necessary conditions for steeldesulfurization. The subject is discussed in more detail later.

2.5.6.4 Solubility of O2

Oxygen dissolves in molten slags by oxidizing the divalent iron ions to the trivalent state.

Gas–slag reaction: 1/2O2(g) + 2(Fe2+) = 2(Fe3+) + (O2–) (2.5.36)

Slag–metal reaction: Fe° + 4(Fe3+) + (O2–) = 5(Fe2+) + [O] (2.5.37)

These reactions provide the mechanism for oxygen transfer from gas to metal through the over-laying slag layer. Partly for this reason, the steel reoxidation will be minimized by maintaining alow concentration of iron oxide in the ladle slag, tundish and mold fluxes.

Examples are given in Fig. 2.72 of variations of the ratio Fe3+/Fe2+ with slag composition of meltsco-existing with liquid iron, reproduced from a paper by Ban-ya and Shim109.

100 80 60 40 20

0 10 20 30 40

0.20

0.15

0.10

0.05

0

1600°C 40%50%

60%

70%

(a)

20%10%

1 2 3 4 5 6Molar ratio (CaO + MgO)/SiO2

Fe3

+/F

e2+

0

0.10

0.06

0.04

0.02

0.08

0.12

(b)

liq. Fe-saturated1600°C

δ-Fe-saturated1400°C

FeO (mol. %)

Fe3

+/F

e2+

1600°C

Al2O3

CaO

TiO2

P2O5 SiO2

MxOy (mol. %)

(c)

0.2

0

0.1

0.3

Fig. 2.72 Effect of slag composition on the ratio Fe3+/Fe2+ in melts saturated with metallic iron at 1600°C: (a)CaO–MgO–SiO2–FeO melts at indicated molar concentrations of total iron oxide FeO; (b) MgO–SiO2–FeOmelts; (c) pseudobinary FeO–MxOy melts. From Ref. 109.

Fundamentals of Iron and Steelmaking

2.5.7 Surface Tension

Surface tensions measured by Kozakevitch110 are given in Fig. 2.73 for binary melts with ironoxide, and in Fig. 2.74 for FeO–MnO–SiO2 and FeO–CaO–SiO2 melts at 1400°C. For additionaldata on surface tension of a wide variety of slags and mold fluxes, reference may be made to areview paper by Mills and Keene111.

Sur

face

tens

ion

(mN

m–1

)

Al2O3

MnO

P2O5Na2O(1480°C)

TiO2

CaO

SiO2

Additions to FeO at 1400°C (mol.%)0 4 8 12 16 20 24 28 32

600

550

500

450

400

0.6

0.4

0.2

MnO

390410

430450

470490

510530

550

FeO 0.2 0.4 0.6 0.8NMnO

mN

m–1

(a)

SiO2

xSiO

2

410430

450470

490510

530550

570FeO

0.6

0.4

0.2

CaO

(b)

SiO2

xSiO

2

mN

m–1

NCaO0.2 0.4 0.6 0.8

Fig. 2.73 Surface tensions ofbinary iron oxide melts at 1400°C.From Ref. 110.

Fig. 2.74 Isosurface tensioncurves in (a) FeO-MnO-SiO2 and(b) FeO-CaO-SiO2 melts saturatedwith iron at 1400°C. From Ref. 110.

Ironmaking Volume

2.5.7.1 Interfacial Tension

The slag-metal interfacial tensions have values between those for the gas-slag and gas-metal surface tensions. Consequently, the addition of surface active elements to liquid ironlowers the slag-metal interfacial tension.

Effects of sulfur and oxygen dissolved in iron on the interfacial tension between liquid iron andCaO–Al2O3–SiO2 melts at 1600°C, determined by Gaye et al.112, are shown in Figs. 2.75 and 2.76;compared to the surface tensions of Fe–S and Fe–O melts. The effect of oxygen on the interfacial ten-sion is greater than sulfur, e.g. σi = 600 mN m–1 with aO = 0.05 (0.05%) while at aS = 0.05 (0.05%),σi = 1000 mN m–1.

1300

1100

900

700

500

Inte

rfac

ial t

ensi

on (

mN

m–1

)

Oxygen activity in iron

Interfacial tension

Surface tension Fe–O

0 0.02 0.04 0.06 0.08

Surface tension Fe–S

Interfacial tension

Inte

rfac

ial t

ensi

on (m

Nm

–1)

1200

1100

1000

900

800

700

Sulfur activity in iron0.1 0.3 0.5 0.7

Fig. 2.75 Effect of oxygen in iron on the interfacialtension between liquid iron and CaO–Al2O3–SiO2melts, determined by Gaye et al.112 is compared tothe surface tension of Fe–O melt at 1600°C.

Fig. 2.76 Effect of sulfur in iron on the interfacial ten-sion between liquid iron and CaO–Al2O3–SiO2 melts,determined by Gaye et al.112 is compared to the sur-face tension of Fe–S melts at 1600°C.

Fundamentals of Iron and Steelmaking

As shown by Ogino et al.113 Fig. 2.77, a single curve describes adequately the effect of oxygen iniron on the interfacial tension between liquid iron and a wide variety of simple and complex slags,including those containing Na2O and CaF2. In the case of slags containing iron oxide, a decreasein interfacial tension with an increasing iron oxide content is due entirely to the correspondingincrease in the oxygen content of the iron.

Recently Jimbo and Cramb114 accurately measured the interfacial tension between liquid iron andCaO–Al2O2–SiO2 slags. As shown in Fig. 2.78 their results are slightly higher than those of Gaye et al.

Mass % oxygen in iron0.0010 0.0032 0.0100 0.0316 0.1000 0.2512

1800

1400

1000

600

200

Inte

rfac

ial t

ensi

on (

mN

m–1

)

−3.0 −2.5 −2.0 −1.5 −1.0 −0.6Log [%O]

Fig. 2.77 General relation between theoxygen content of iron and the interfacialtension between the metal and variousslag systems at 1580°C. From Ref. 113.

0 20 40 60 80SiO2 content [wt %]

Data from Gaye et al.

Inte

rfac

ial t

ensi

on (

mN

m–1

) CaO/Al203 (1:1)CaO/Al203 (3:5)

2200

1800

1400

1000

600

Fig. 2.78 Interfacial tension between CaO–Al2O3–SiO2 and Fe at 1600°C. From Ref. 114.

Ironmaking Volume

2.5.8 Density

Many repetitive measurements of slag densities have been made. Only selected references aregiven on the density data cited here for steelmaking type of slags. Since the density of silica(2.15 g cm–3 at 1700°C) is much lower than the densities of other metal oxide components ofslags, densities of slags will decrease with an increasing silica content.

The density data for binary silicates are given in Fig. 2.79. The data in Fig. 2.80 are forCaO–MgO–Al2O3–SiO2 melts, relevant to neutral slags for steel refining in the ladle.

0 20 40 60 80

Mass % SiO2

CaO–SiO21700°C, (119)

MgO–SiO21700°C, (119)

MnO–SiO2 1475°C, (117, 118)

FeO–SiO2 1400°C, (115, 116)

Den

sity

(g

cm−3

)

2

3

4

5

Fig. 2.79 Densities ofbinary silicate melt. FromRefs. 115–119.

0 10 20 30 40 50 60

a b c

Mass % SiO2

Den

sity

(g

cm–3

)

2.8

2.6

2.4

Fig. 2.80 Densities ofCaO–MgO–Al2O3–SiO2melt at 1550°C, usingdata in Refs; 120–122.(a) 0% MgO, CaO/Al2O3= 1; (b) 0% MgO, 5%Al2O3; (c) 5% MgO,5%Al2O3.

Fundamentals of Iron and Steelmaking

The density data in Fig. 2.81 compiled by Mills and Keene111 are for simple and complex slagscontaining FeO, CaO, MgO, SiO2 and P2O5. Since the densities of FeO–SiO2 and MnO–SiO2 areessentially the same, the average of the data in Fig. 2.81 is represented by the following equationin terms of (%FeO + %MnO).

ρ,gcm–3 = 2.46 + 0.018 x (%FeO + %MnO) (2.5.38)

0 10 20 30 40 50 60 70 80 90 100

Total mass % iron oxides

4.5

4.4

4.3

4.2

4.1

4.0

3.9

3.8

3.7

3.6

3.5

3.4

3.3

3.2

3.1

3.0

2.9

2.8

2.7

2.6

2.5

Den

sity

, ρ (

g cm

-3)

+5%

−5%

Fig. 2.81 Densities ofsimple and complex slagscontaining iron oxide atabout 1400°C. From Ref.111.

Ironmaking Volume

2.5.9 Viscosity

The size of the silicate and aluminosilicate network in molten slags becomes larger with increas-ing SiO2 and Al2O3 contents, hence their mobility decreases resulting in a higher viscosity. Theaddition of metal oxides or an increase in temperature leads to the breakdown of the Si(Al)O4 net-work, resulting in lower melt viscosity.

Machin and Yee123 made an extensive study of the viscosity of CaO–MgO–Al2O3–SiO2 melts attemperatures of 1350 to 1500°C. The data in Fig. 2.82 are for the ternary system at 1500°C. Theisokoms are approximately parallel to the binary side Al2O3–SiO2, indicating that Al2O3–SiO2 areisomorphous in their effect on the slag viscosity. The isokoms in Fig. 2.83 are for the quaternarysystem with 35% and 50% SiO2. In this case, the isokoms are approximately parallel to the binaryside CaO–MgO, indicating that Ca2+ and Mg2+ cations have similar effects on the breakdown of thealuminosilicate network.

30 60

40 50

50 40

60 30

10 80

20 70

CaO

(wt%

)

Al2O3 (wt%)

Al2O3

SiO2 (w

t%)

SiO2

0 90

2000

CaO10 20 30 40 50 60 70

3.03.5

4

5 6 7 8 910 12 1416

18 2030

4060

80

100200

400600

1000

2.5

35% SiO2

Al2O

3

MgO

Mass % CaO

1500°C

3 poise 2.5 24

56789

12

10

1416

18

20 30 40 50 60

25

35

45 0

10

2015 5

1500°C

89

10

1214

16

18

242628

30

3540

45

7 65 4

3.53

20 30

30 20

40 10

10 20 30 40 50Mass % CaO

Al2O 3

MgO

50% SiO2

0

2022

Fig. 2.83 Isokoms (0.l N s m–2) for CaO–MgO–Al2O3–SiO2 system at 1500°C for melts containing 35% and50% SiO2. From Ref. 123.

Fig. 2.82 Isokoms (0.l N s m–2)for CaO–Al2O3–SiO2 system at1500°C. From Ref. 123.

Fundamentals of Iron and Steelmaking

Viscosities of steelmaking slags are well represented by the experimental data of Kozakevitch110

given in Fig. 2.84

In the study of viscosities of mold fluxes for continuous casting, the experimental results have beenrepresented as a function of temperature using the relation.

η = AT exp (B/T) (2.5.39)

where A and B are functions of slag composition. For the composition range (wt %) 33–56% SiO2,12–45% CaO, 0–11% Al2O3, 0–20% Na2O and 0–20% CaF2, an interpolation formula has been derivedfor the parameters A and B as a function of the mole fractions of the constituents as given below.

lnA = –17.51 – 35.76(Al2O3) + 1.73(CaO) + 5.82(CaF2) + 7.02(Na2O) (2.5.40)

B = 31,1140 – 68,833(Al2O3) – 23,896(CaO) – 46,351(CaF2) – 39,519(Na2O) (2.5.41)

where A is in units of 0.1 N s m–2 K–1 ( poise/deg.) and B in degrees Kelvin.

2.5.10 Mass Diffusivity, Electrical Conductivity and Thermal Conductivity

2.5.10.1 Mass Diffusivity

Because of the ionic nature of molten slags, the diffusive mass transfer is by ions. The ionic diffu-sivities are measured using the radioactive tracer elements dissolved in an oxidized form in themelt. Typical examples of ionic diffusivities in slags at 1600°C are given below.

Ion Di*, cm2/s_____________ _______________

Si4+, O2– 4 x 10–7 – 1 × 10–6

Al3+ ≈1 × 10–6

Ca2+, Mg2+, Fe2+ 6 x 10–6 – 1 × 10–5

S2– ≈ 4 × 10–6

Since the electroneutrality has to be maintained, diffusion of a cation is accompanied by diffusionof the oxygen ion. The diffusion that occurs in the dissolution of a solid oxide in the slag is con-trolled by the mobility of the O2– ion which is smaller than the divalent cations.

CaO (mass%)

SiO 2

(mas

s%)

FeO (m

ass%)

90 10

80 20

70 30

60 40

50 50

40 60

30 70

20 80

10 90

90 80 70 60 50 40 30 20 10

0.40.2

0.150.1

0.05

Fig. 2.84 Viscosity (N s m–2) ofCaO–FeO–SiO2 melts in 1400°C.From Ref. 110.

Ironmaking Volume

2.5.10.2 Electrical Conductivity

The electrical current in molten slags is carried by the cations. However, in slags containing high con-centrations of FeO or MnO (> 70%) the electronic conduction becomes the dominant mechanism.

The ionic conductivity λi is theoretically related to the self diffusivity of the ionic species i by theNernst-Einstein equation

(2.5.42)

where F = Faraday constant; 96,489 C mol–1,Zi = valency of ion i,Ci = concentration of ion i, mol cm–3,λi = specific conductivity, Ω–1cm–1.

For steelmaking slags: λ = 0.5–1.5 Ω–1cm–1.For ladle slags: λ = 0.4–0.7 Ω–1cm–1.

The electrical conductivity increases with an increasing slag basicity and increasing temperature.

2.5.10.3 Thermal Conductivity

Because of the presence of iron oxide, the metallurgical slags are opaque to infrared radiation,therefore the heat conduction is primarily thermal.

Thermal conductivity of slags and mold fluxes are in the range 0.5 to 1.2 Wm–1K–1. From experi-mental data the following approximate empirical relation has been found

κ(Wm–1 K–1) = 1.8 × 10–5 V–1 (2.5.43)

where V is the molar volume = M/ρ, m3mol–1.

2.5.11 Slag FoamingSlag foaming plays an important role in many steelmaking processes. In oxygen steelmakingexcessive foaming can lead to slopping. On the other hand controlled foaming in the electric arcfurnace is desirable to protect the refractories from the electrical arc radiation. In the direct iron-making processes such as DIOS and AISI Direct Steelmaking, excessive foaming can cause oper-ational problems. However some foam is desirable to help capture the energy from postcombustion. Slag foaming should not be confused with simple gas bubbling or hold up. Whenevergas passes through a liquid, the liquid expands due to the presence of the gas. However in some liq-uids a stable foam develops which consists of foam bubbles on the top of an unfoamed liquid.

Early work on foaming was limited to a qualitative understanding of this complex phenomenon.Due to the added importance of foaming in the EAF and iron bath systems Ito and Fruehan124,125

and other researchers developed a quantitative measure of foaming and measured the foamingcharacteristics of many important slag systems. The foam index (Σ) was defined by

(2.5.44)

(2.5.45)

where ∆ = the increase in the height of the slag,

Vgs = the superficial gas velocity,

Q = the gas flow rate,A = the area of the vessel.

It follows that the volume of foam is approximately given by

Vf = QΣ (2.5.46)

VQAg

s =

Σ ∆= hVg

s

DRT

F Z Cii i

i∗ = 2 2 λ

Fundamentals of Iron and Steelmaking

The foam index has the units of time and represents the average traveling time of the gas throughthe foam.

The foam can also be characterized by the time for the foam to decay. The average foam life (τ) isdefined by the first order decay

(2.5.47)

where h and ho are the foam height and the foam height when the gas flow stops, respectively. Itcan be shown that for an ideal foam, in which the gas fraction of the foam is constant, that the foamindex (Σ) and foam life (τ) are equal.

The foam index for CaO–SiO2–FeO–Al2O3 system is shown in Fig. 2.85. The foam index decreasesinitially with increasing basicity because the viscosity is decreasing. However when the solubilitylimit is reached the foam index increases with basicity because the second phase particles increasethe bulk viscosity of the slag.

Zhang and Fruehan126 later demonstrated that the foam index on stability increased with decreas-ing bubble size and developed a general correlation demonstrated in Fig. 2.86 from which the foamindex for many complex systems would be desired.

(2.5.48)

whereη = slag viscosity,σ = surface tension,ρ = slag density,

DB = foam bubble diameter.

Takumetsu et al127 showed that in bath smelting processes char could reduce foaming significantly.Zhang and Fruehan128 examined the fundamentals of slag control by carbonaceous materials. Dueto surface tension phenomenon the slag foam bubbles collapse and form longer bubbles resulting ina less stable foam. Carbonaceous materials will cause the foam to collapse while others such as alu-mina particles or iron oxide pellets do not due to the different wetting characteristics with the slag.

The fundamentals of slag foaming have been applied to a variety of processes such as oxygen andEAF steelmaking, bath smelting and ladle processing. The fundamental principles allow for rea-sonable predictions of foaming in these processes.

Σ = ησ ρ

1 2

0 2 0 9

.

. .DB

lnhh

t

o

= −τ

0 0.5 1.0 1.5 2.0

1673 K

CaO-SiO2–FeO–(Al2O3)FeO=30%, Al2O3 = 3~5%

20

10

5

2

1

1573 K

Σ (s

)

(wt %)CaOSiO2 + Al2O3

100

10

1

0.1

Pre

dict

ed fo

am in

dex

(sec

)

Measured foam index (sec)0.1 1 10 100

Fig. 2.85 The foam index of CaO–SiO2–FeO–Al2O3 slags illustrating the effect of second phaseparticles. From Ref. 126.

Fig. 2.86 Comparison between the measuredfoam index and that predicted by the correlationequation 2.5.48. From Ref 126.

Ironmaking Volume

2.5.12 Slag Models and Empirical Correlations for Thermodynamic Properties

There have been several attempts to develop models and correlations for slags, from which thermo-dynamic properties such as activities and capacities can be predicted. Simple models such as a regu-lar solution have been used.129 However because of the ionic nature and structure of slags they aregenerally inadequate. Recently Gaye and Lehmann reviewed the current status of structural models.130

The most successful models have been developed by Gaye and coworkers131 at IRSID and Blanderet al.132 In the IRSID model the slag is represented using an oxygen sublattice and a cationic sub-lattice. The structure is defined in terms of cells composed of a central oxygen surrounded by twocations. Two parameters are used to calculate the energy of the system; the energies of formationof asymmetric cells and the interaction energies limited to one parameter per couple of cations.These parameters are computed from the known thermodynamics of the binary systems. It isbeyond the scope of this chapter to describe the model in greater detail. The model has been usedsuccessfully to estimate the phase diagrams and thermodynamic activities in multi-component sys-tems as well as sulfide capacities. Whereas this model is complex and requires binary data, to dateit is the best model available for estimating thermodynamic properties of slags.

In recent years various capacities such as the sulfide and phosphate capacities have been correlatedto a term called the optical basicity. This concept has been recently reviewed by Summerville etal.133 Briefly each oxide is assigned a value for its optical basicity which is related to the Paulingelectronegativity. By definition the optical basicity of CaO is taken as unity. Components such asNa2O have optical basicities greater than one while acidic oxides such as SiO2 have values less thanone. The optical basicity of a slag is then computed from a weighted average of the components inthe slag. The optical basicity has been used to correlate a large number of studies on sulfide andother capacities.133, 134 Whereas the optical basicity is an interesting concept, the correlations arenot sufficiently accurate to predict capacities for industrial purposes. For example the deviationsbetween the correlation and actual data is 25–50% in some cases. This is not accurate enough forcomputing sulfur equilibrium in industrial applications. However the optical basicity correlationmaybe useful for making crude estimates of capacities for which no data exists or to predict trendswhen changing slag compositions slightly.

2.6 Fundamentals of Ironmaking ReactionsReference may be made to a book entitled “The Iron Blast Furnace”, authored by Peacey and Daven-port.135 In this book, the theoretical, experimental and operational data have been put together about theblast furnace with particular emphasis on the interrelations between countercurrent heat and masstransfer between gases and solids in the blast furnace stack. Reference may also be made to the earlierstudies of Rist and co-workers136–140 on the heat and mass transfer and reduction reactions in the stack.

In this section, the following aspects of the blast furnace reactions are considered: oxygen poten-tial diagram, role of vapor species in blast furnace reactions, slag-metal equilibrium, reactionmechanisms and operational slag-metal data.

2.6.1 Oxygen Potential DiagramThe reducibility of a metal oxide relative to other oxides, or the oxidisability of a metal relative toother metals, can readily be assessed from the free energy data.

For the oxidation reaction involving pure metals and metal oxides in their standard states, i.e. aM = 1, aMO = 1

2M + O2 = 2MO (2.6.1)the isothermal equilibrium constant is

(2.6.2)Κ = 1

2pO

Fundamentals of Iron and Steelmaking

where pO2is the equilibrium oxygen partial pressure for which the standard state is 1 atm at the

temperature under consideration. The standard free energy change is

∆G° = –RT ln K = RT 1n pO2(2.6.3)

which is also called the oxygen potential.

In an earlier study, Richardson and Jeffes141 compiled the free energy data on metal oxides whichwere then available, and presented the data, Fig. 2.87, as an oxygen potential diagram.

The oxides for which the oxygen potential lines are above that of CO may be reduced by carbon.As the affinity of the metals for oxygen increases, i.e. ∆G° decreases, the temperature of reductionof the oxides by carbon increases.

For easy conversion of oxygen potentials to the corresponding values of pO2or to the equilibrium

ratios of H2/ H2O and CO/CO2, appropriate scales are included in the enclosed oxygen potentialdiagram for various oxides of metallurgical interest.

Scale for pO2:

Lines drawn from the point O on the ordinate for the absolute zero temperature throughthe points marked on the right hand side of the diagram give the isobars. For example, forthe Fe–FeO equilibrium the oxygen potential is –82 kcal (–343 kJ) at 1200°C. By drawinga line passing through this point and the point O, the oxygen partial pressure of about 7 ×10–13 atm is read off the log pO2

scale.

Scale for CO/CO2:

Draw the line from point C to a point on the oxygen potential; the extension of this linegives the corresponding equilibrium log CO/CO2 ratio.

Scale for H2/H2O:

Same as above by using point H.

These diagrams can be used to predict CO/CO2 or H2/H2O ratios as well as the pressure of oxygenin equilibrium with numerous metals and their oxides. They are particularly useful for predictingthe CO/CO2 ratio in a blast furnace or the H2/H2O ratio in direct reduction with natural gas. It alsogives an indication of the relative reduceability of the oxides. It should be remembered that the dia-grams are for unit activity of the metal. If the metal is in solution, it is easier to reduce. For exam-ple, if the activity of Si is 10–3 relative to pure Si in liquid iron, the equilibrium oxygen pressure is103 times higher. Similarly, if the activity of SiO2 is lowered in a slag it is more difficult to reduce.

2.6.2 Role of Vapor Species in Blast Furnace Reactions

Because of the high temperatures involved, vaporization plays a significant role in pyrometallurgi-cal reactions. In a reactor such as a blast furnace, the formation and condensation of various vaporspecies is responsible for the recycle of some of the elements between the high and low tempera-ture regions of the furnace.

The countercurrent flow in the blast furnace of solids from low- to high-temperature zones and ofgases from high- to low-temperature zones brings about a cyclic process of vaporization and con-densation which has a decisive influence on the overall operation of the furnace.

2.6.2.1 Vapor Species SiO, SiS and CS

It is now well established that the silicon and sulfur in the coke are transferred to the slag and ironin the blast furnace via the vapor species SiO, SiS, CS, and other minor sulfur-bearing species. Theearlier and recent studies of quenched blast furnaces have revealed that while the sulfur content ofthe slag increases with the descent of the burden in the bosh, the sulfur and silicon contents of themetal droplets reach maxima and then decrease as they pass through the slag layer. This phenom-enon of vapor-phase mass transfer has been substantiated by the experimental work of Tsuchiya et

Ironmaking Volume

al,142 Turkdogan et al 143 and Ozturk and Fruehan144 under conditions partly simulating the boshregion of the blast furnace.

In the presence of carbon and depending on temperature and activity of silica in the slag or coke,the SiO vapor is generated by one of the following reactions

SiO2 (in coke ash or slag) + C → SiO + CO (2.6.4)

SiC + CO → SiO + 2C (2.6.5)

13 12 11

–8 –7 –6 –5 –4 –3

Temperature (°C)

log CO/CO2

Absolute zero0 200 400 600 800 1000 1200 1400 1600 1800 2000 2200 2400

RT

log

PO

2 (kc

al)

0

–20

–40

–60

–80

–100

–120

–140

–160

–180

–200

–220

–240

–260

–280

–300

Suggested accuracies(A) ± 1 kcal(B) ± 3 kcal(C) ± 10 kcal(D) ± 10 kcal

Changes of state Element Oxide

Melting point M M

Boiling Point B B

Sublimation pt. S S

Transition pt. T T

log H2/H2O

O

H

C

log pO2

0

–1

–2

–3

–4

–6

–8

–10

–12

–14

–16

–18

–20

–22

–24

–200 –150 –100–90 –80 –70 –60 –50 –44 –38 –34 –30 –28 –26

–2

–1

0

1

2

3

4

5

6

7

8

9

10

–8 –7 –6 –5 –4 –3 –2

–1

0

1

2

3

4

5

6

7

8

9

10

11

14 13 12

4Cu + O2 = 2Cu2O (A)

4 Fe3O4 +

O2 = 6Fe2O

3 (B)

2Pb + O2 = 2PbO (B

)

•S2 + O2 = SO2 (B)

2Ni + O2 = 2NiO (B

)

C + O2 = CO2

2Co + O2 = 2CoO (C)

6FeO + O2 = 2Fe3O4

2CO + O2 = 2CO2 (A

)

2H2 + O2 = 2H2O (A)

2 Fe + O2 = 2FeO (A)

2SnO + O2 = 2SnO2

3Fe + 2O2 = Fe3O4 (A

)Sn + O2 = SnO2 (B

)

2P2 + 5O2 =

2P2O5 (C)

4K + O2 = 2K2O

(D) 2Zn + O2 =

2ZnO (B)

4Na + O 2 = 2Na 2

O (B)

4Cr + 3O2 = 2Cr2O3 (B

)

2Mn + O2 = 2MnO (B)

4V + 3O2 = 2V2O3 (C

)

Si + O2 = SiO2 (B

)

Ti + O2 = TiO2 (B

) 2SiO

+ O

2 =

2SiO

2 (B

)

2C + O2 = 2CO (A)

4Al + 3O2 = 2Al2O3 (

B)

U + O2 = UO2

4Li + O2 = 2Li 2O

(C)

2Mg + O2 = 2MgO (C

)

2Ca + O2 = 2CaO (C)

B

M

M

M

B

M

M

M

M

M

M

M

M

MM

M

M

MM

M

B B

B

S

B

B

B

M

M

M

BM

T

M

M

M

B

Fig. 2.87 Oxygen potential diagram. From Ref. 141.

Fundamentals of Iron and Steelmaking

At 1 bar pressure of CO, aSiO2= 1 and above about 1500°C, SiO2 is converted to SiC and SiO is gen-

erated by reaction 2.6.5; for aSiO2= 0.1, reaction 2.6.5 applies only at temperatures above about

1610°C. In the experiments cited,143 the SiO generated by passage of CO through a coke bed at tem-peratures of 1600 to 1900°C, were found to be close to the equilibrium values for reaction 2.6.5.Volatile SiS is generated by reactions of the type with the coke ash:

CaS (in coke ash) + SiO → SiS + CaO (2.6.6)

FeS (in coke ash) + SiO + C → SiS + CO + Fe (2.6.7)

The reaction of these vapor species with metal and slag may be represented by the equations:

(2.6.8)

(2.6.9)

Ozturk and Fruehan,144 in carefully controlled experiments, demonstrated that the rate of the SiOreactions with metal and slag are controlled by gas phase mass transfer and are rapid.

Coke samples taken from the tuyere zone of the blast furnace usually contain 12 to 16% ash whichhas a basicity (CaO + MgO)/SiO2 of about 0.6; for a typical blast furnace slag, the basicity is about1.5. Therefore, the partial pressures of SiO and sulfur-bearing species in the gas near the coke sur-face are expected to differ from those interacting with the slag. For the purpose of comparison, cal-culations are made for assumed local equilibrium at 1500°C for the systems gas-slag and gas-cokeash; the results are given in Table 2.12. The amount of ash in the tuyere coke and its compositionsuggests that, although most of the silica and sulfur in the coke ash are removed from the furnaceby the slag and liquid iron, there is significant recycle of silicon and sulfur in the bosh region bythe vaporization and condensation of these species on the coke particles.

Slag

SiO + Si O

Si O

12

|

|-

|

|-

O C CO

SiS O C S CO

2 12

12

32

2 12

2 12

− −

+ =

+

+ + =

+ ( ) +

Metal SiO + C[ ] = [ ] +

= [ ] + [ ]

Si CO

SiS Si S

Table 2.12 Calculated Equilibrium Vapor Pressures in bar for the Systems Gas–Slagand Gas–Coke Ash at 1500°C and 1 bar Pressure of CO.

B = 1.5, aSiO2= 0.05 B = 0.6, aSiO2

= 0.32%(S), CS = 3 x 10–4, 5%(S), CS = 10–5,

Vapor (wt%) * (wt%)* SiO 2.6 × 10–4 1.5 × 10–3

SiS 3.9 × 10–5 1.7 × 10–2

S2 8.6 × 10–9 4.9 × 10–5

CS 5.5 × 10–5 4.3 × 10–3

COS 5.5 × 10–6 1.2 × 10–4

* CS(wt%) is the sulfide capacity of the slag.

2.6.2.2 Alkali Recycle and Removal by Slag

The alkalies constitute another dominant vapor species in the bosh and stack regions of the blast fur-nace. Many studies have been made of the alkali recycle in the blast furnace via the process of vapor-ization and condensation; the subject is well covered in the references cited.145–147 Generalconsensus evolved from elementary thermodynamic calculations is that the alkali silicates in the ore

Ironmaking Volume

and coke ash decompose at elevated temperatures in the lower part of the bosh and the combustionzone. In part the alkali vapors carried away with the ascending gas react with the slag and can there-fore be removed from the furnace; part are converted to alkali cyanides and carbonates anddeposited on the burden and the refractory lining of the furnace stack. Some new thoughts are pre-sented in the following discussion on the sequence of reactions and vapor species that may governthe alkali recycle in the blast furnace.

As an example, let us calculate the equilibrium vapor pressure of potassium for the reduction reaction:

(K2O) + C = 2K(g) + CO(g) (2.6.10)

The computed equilibrium values in Table 2.13 are for a blast furnace slag containing 0.5% K2Oand having a basicity of B = 1.5: K is the equilibrium constant for reaction 2.6.10 from the ther-mochemical data and aK2O is the activity of K2O in the slag, relative to the hypothetical solid K2O,from the experimental data of Steiler.148

If the potassium input with the blast furnace burden is 4 kg K/t–HM and 80% of it is removed bythe slag, about 0.8 kg K/t–HM will be in the vapor phase carried away by the furnace gas. For atypical total gas volume of 2300 nm3/t–HM, the partial pressure of the total potassium vaporspecies would be 7.2 x 10–4 bar (for a total gas pressure of 3.6 bar in the bosh region). Compari-son of this total potassium pressure in the gas with those in Table 2.13 for the gas-slag equilibriumindicates that the slag particles will pick up potassium from the gas only at temperatures below1200°C. The ash in the coke samples taken from the tuyere zone contains 2 to 4% (Na2O + K2O)which is several fold of that in the original coke ash. Because of the low basicity of coke ash, theamount of alkali therein is expected to be 5 to 10 times greater than that found in the slag. In theupper part of the bosh, the slag and coke will pick up alkalies from the gas. As the temperature ofthe slag and coke increases during descent in the bosh, they will emit alkali vapors to the gas phase.However, the partial pressure of potassium vapor in the gas would probably be below that given inTable 2.13 for the gas-slag equilibrium. Nevertheless, the numerical examples cited suggest thatmuch of the alkalies accumulated in the bosh and hearth zone of the blast furnace, via recycling,are in the gas phase.

Table 2.13 Equilibrium Vapor Pressure of Potassium for Reaction 2.6.10 with Slaghaving 0.5% K 2O and B = 1.5.

Temperature (°C) K, bar aK2O pK, bar

1200 3.10 × 105 2.1 × 10–12 7.1 × 10–4

1300 2.69 × 106 5.5 × 10–12 3.4 × 10–3

1400 1.81 × 107 1.4 × 10–11 1.4 × 10–2

1500 9.78 × 107 3.5 × 10–11 2.6 × 10–1

According to a mass spectrometric study of vaporization of potassium cyanide by Simmons et.al,149 the equilibrium pressures of vapor species are in the order p(KCN)2

> p(KCN) > p(KCN)3. For

atmospheric pressure of nitrogen and at graphite saturation, the following are the equilibrium ratiosof the vapor species: at the melting point of KCN (635°C), (KCN)2: KCN : K = 2 : l : 0.76 and atthe boiling point (1132°C), (KCN)2: KCN : K = 4.6: l : 0.19. It is all too clear that (KCN)2 is thedominant alkali-bearing species in the blast furnace. The sodium in the burden undergoes cyclicreactions similarly to potassium; however, the concentration of sodium-bearing species are aboutone-tenth of the potassium-bearing species.

One method of minimizing the ascent of alkali vapors to the stack, hence reducing the alkali recy-cle, is by operating the furnace with a slag of low basicity, particularly when the alkali input is high.The slag of low basicity, however, will have an adverse effect on the composition of the hot metalproduced; it will result in low manganese, high silicon and high sulfur in the metal. For a givenpreferred basicity, the slag mass per ton of hot metal may have to be increased when there is anincrease in the alkali input to the furnace. An increase in amount of slag will increase the coke rate,

Fundamentals of Iron and Steelmaking

hence will increase the alkali input. Obviously, with a burden of high alkali input, a compromisehas to be made in adjusting slag basicity and slag mass so that the alkali recycle would be low.

Even with a low alkali input some alkali buildup will occur. To prevent excessive accumulation ofalkalies, which lead to scaffolding, gas channeling, furnace upsets and so on, periodic additions ofgravel (silica) or olivine (magnesium silicate) are made to the blast furnace charge. The silica reactswith alkali carbonates and cyanides, thus facilitates the discharge of the accumulated alkalies fromthe furnace by the slag. Practical experience also shows that periodic addition of calcium chlorideto the burden also facilitates the removal of alkalies by the slag.

2.6.2.3 Ammonia and Hydrogen Cyanide in Blast Furnace Stack

The contaminants in the wash water for the iron blast-furnace off-gas are in the ranges 10–300 mgNH3/l, 1–30 mg CNt (total)/l, and 0.3–15 mg phenols/l. In terms of ppm by volume in the stackgas, the concentrations are usually in the ranges 3000–4000 ppm NH3 and 150–250 ppm CNt. Asobserved by Pociecha and Biczysko,150 for example, most of the cyanide in the de-dusted furnaceoff gas is in the form of hydrogen cyanide. They also found that the blast furnace dust contains onlya small amount of solid cyanides (presumably alkali cyanides) in comparison with the amount ofhydrogen cyanide present in the de-dusted top gas. The same contaminants in the ferromanganeseblast furnace off gas are about an order of magnitude greater than those in the iron blast furnace.

The experimental work of Turkdogan and Josephic,151 under conditions partly simulating the blastfurnace stack, substantiated the validity of this mechanism of generation of ammonia and hydro-gen cyanide in the stack, by the following reactions.

2K(Na)CN + 3H2O = (K, Na)2CO3 + 2NH3 + C (2.6.11)

NH3 + CO = HCN + H2O (2.6.12)

The amounts of ammonia and hydrogen cyanide generated will increase with an increase in theconcentration of water vapor in the stack gas. Other reactions will occur with these volatile speciesgenerating some amino-nitro phenols, e.g. NH2(NO2)C6H3OH. The equilibrium concentrations ofthese volatile organic species become greater at lower temperatures.

2.6.3 Slag-Metal Reactions in the Blast FurnaceSlag-metal reactions in the hearth of the blast furnace control the chemistry of the hot metal. Inparticular, the silicon, sulfur and manganese contents depend upon these reactions. In this sectionthe equilibrium and reaction mechanisms are presented.

2.6.3.1 Slag-Metal Equilibrium for Blast Furnace Reactions

From the thermodynamics of the slag systems and of the various solutes in iron such as sulfur, sil-icon and manganese, it is possible to predict the equilibrium relationship for blast furnace reactions.

The three-phase reactions to be considered are for graphite-saturated melts at 1 atm pressure of car-bon monoxide, which is close to the partial pressure of CO in the blast furnace bosh and hearth zones.

2.6.3.1.1 Silicon Reaction The reaction equilibrium to be considered is

(SiO2) + 2[C] = [Si] + 2CO(g) (2.6.13)

(2.6.14)

where the SiO2 and C activities are with respect to pure solid silica and graphite, respectively.

The temperature dependence of the equilibrium constant is from the free energy data

(2.6.15)log,

.ΚSi T= − +30 935

20 455

ΚSiSi

SiO

CO

C

Si f p= [ ]( )

%

a a2

2

Ironmaking Volume

Substituting aSiO2= (%SiO2)γSiO2

/60 × 1.65 and for theactivity coefficient fSi = 15 in graphite-saturated ironcontaining Si < 2%, the equilibrium metal/slag silicondistribution ratio is represented by

(2.6.16)

The equilibrium silicon distribution ratios computedpreviously, using the γSiO2

values for the blast furnacetype slags (CaO, 10% MgO, 10% Al2O3, SiO2), aregiven in Fig. 2.88. The dotted curves are derived fromother data discussed later. For the blast furnace typeslags, the basicity is usually defined by the mass ratio(%CaO + %Mg)/%SiO2.

2.6.3.1.2 Manganese Reaction For the reaction

(MnO) + [C] = [Mn] + CO(g) (2.6.17)

(2.6.18)

(2.6.19)

For the graphite-saturated iron, the activity coefficientfMn = 0.8, and inserting aMnO = (%MnO) γMnO/71 ×1.65, the equilibrium manganese distribution ratio isrepresented by

(2.6.20)

Abraham et al.152 measured the MnO activity in CaO–Al2O3–SiO2– MnO melts containing Al2O3< 20% and MnO < 8%. The values of γMnO derived from their data are seen in Fig. 2.89 toincrease with an increasing slag basicity. The equilibrium manganese distribution ratio forgraphite saturated melts thus evaluated are given in Fig. 2.90.

%%

.Mn

MnOpCO MnO Mn

[ ]( )

= × −1 07 10 2 γ Κ

log,

.KTMn = − +15 090

10 970

ΚMnMn

MnO

CO

C

Mn f p= [ ]( )

%a a

%%

.Si

SiOpCO SiO Si

[ ]( ) = × −

2

2 46 73 102

γ Κ

1600°C

1500°C

1400°C

0.8 1.0 1.2 1.4 1.6% CaO + %MgO

% SiO2

10

1

0.1

0.01

0.001[%

Si]

(%S

iO2)

ρ2 co

(atm

2 )

Fig. 2.88 Silicon distribution ratio forgraphite–saturated melts for blast furnacetype slags containing about 10% MgO and10% Al2O3. Lines – – – are derived fromthe data in Fig. 2.90 and equation (2.6.23).

0.4 0.8 1.2 1.6 2.0

2.4

1.6

0.8

0

γ M

nO

%Al2O320

100

%CaO %SiO2

Fig. 2.89 Activity coefficient of MnO, rela-tive to pure solid oxide, in CaO–Al2O3–SiO2–MnO slags, with MnO < 8%, at 1500to 1650°C, derived from the data of Abra-ham, Davies and Richardson152.

Fundamentals of Iron and Steelmaking

2.6.3.1.3 Si–Mn Coupled Reaction

The silicon-manganese coupled reaction

2(MnO) + [Si] = (SiO2) + 2[Mn] (2.6.21)

between graphite-saturated iron and blast furnace type slags has been investigated by several exper-imental studies.143,153,154

(2.6.22)

The combination of equations 2.6.16 and 2.6.20 gives the following equilibrium constant for reac-tion (2.6.21)

The variation of the equilibrium relation KMnSi with slag basicity is shown in Fig. 2.91. The dotted

line for 1400 to 1600°C is calculated from the thermochemical data, i.e. from the computed equi-librium data in Figs. 2.88 and 2.90. The difference of the calculated equilibrium dotted line fromthe average experimental values by a factor of 2.7 (≡ ~15 kJ) is due to the accumulated uncertain-ties in the free energy data on MnO and SiO2 as well as ∆Gs for solutions of Mn and Si ingraphite-saturated iron.

The experimental data in Fig. 2.91 for graphite saturated melts at 1400 – 1600°C may be repre-sented by the following equation.

(2.6.23)

To be consistent with the experimental data in Fig. 2.91, the dotted curves are derived from the reli-able equilibrium data in Fig. 2.90 and the experimental data represented by equation (2.6.23) forthe Si–Mn coupled reaction in graphite saturated melts.

In a study of slag-metal equilibria between CaO–MnO–SiO2 slags and graphite-saturated man-ganese-base alloys, Turkdogan and Hancock155 found that the ratios Si/SiO2 and Mn/MnO variedwith slag basicity in a manner similar to that for iron base alloys. Their results for 1400°C areshown in Fig. 2.92; the dot-dash line is for the iron-base alloys, reproduced from Fig. 2.91.

log .% %

%.ΚMnSi

CaO MgOSiO

= +

−2 8 1 162

Κ ΚΚ

= [ ]( )

( )[ ]

=%%

%

%.

MnMnO

SiO

SiMn

Si

MnO

SiO

2

22 2

0 172

γγ

%CaO + %MgO%SiO2

16

12

8

4

0

[%M

n](%

Mn)

ρ co

(atm

)

0.4 0.8 1.2 1.6

1400°C

1500°C

1600°CFig. 2.90 Manganese distribution ratio for graphite-saturated melts derived for blast furnace type slagscontaining about 10% MgO and 10% Al2O3.

Ironmaking Volume

0.6 1.0 1.4 1.8

k MnS

i

0.5 0.7 0.9 1.1 1.3 1.5 1.7

2000

1000800600

400

200

1008060

40

20

1086

4

Thermodynamic data

(a) (b)

104

103

102

10

1

14001550140015001600

Temp°C

calculated

CaO-SiO2-10% Al2O310% MgO

CaO-SiO2-10% Al2O3

%CaO + %MgO%SiO2

Fig. 2.91 Experimental data showing the equilibrium relation KMnSi with basicity of the blast furnace type slagsat graphite saturation: (a) reproduced from Ref. 143 and (b) from Ref. 154; lines---derived from equation2.6.23 and Fig. 2.90.

2.6.3.1.4 Si–S and Mn–S Coupled Reactions The silicon-sulfur coupled reaction is represented by

[S] + 1/2[Si] + (CaO) = (CaS) + 1/2(SiO2) (2.6.24)

for which the isothermal equilibrium constant is

(2.6.25)

From an analysis of the most available experimental data, Turkdogan et al.143 developed a relationfor KSiS shown in Fig. 2.93. For the range 1400 to 1600°C, the temperature dependence of KSiS isrepresented by the equation

(2.6.26)

From the experimental data represented by equations 2.6.23 and 2.6.26, the following equation isobtained for the temperature dependence of the equilibrium relation for the manganese-sulfur cou-pled reaction in graphite-saturated melts.

(2.6.27)

The equilibrium sulfur distribution ratio as a function of slag basicity in graphite-saturated meltsshown in Fig. 2.94.

log log%%

%% %

.ΚMnSSS

MnOMn CaO T

= ( )[ ]

( )[ ] ( )

= −1 63273 85

log . .% %

%ΚSiS T

CaO MgOSiO

= − + +

63274 43 1 4

2

ΚSiSSS

SiO

Si CaO= ( )

[ ]( )

[ ]

( )

%%

%

% %2

12

1

Fundamentals of Iron and Steelmaking

137

1000800

600

400

200

10080

60

40

20

100 0.4 0.8 1.2

%M

n2

(SiO

2)

%M

nO[%

Si]

%Fe 15-24

25-44 45-62

~95

%CaO%SiO2

Fig. 2.92 Product of manganese and silicon ratios for graphite–saturated ferromanganese melts, of indicatediron contents, equilibrated with CaO–MnO–SiO2 slags at 1400°C and 1 atm CO, derived from the data of Turk-dogan and Hancock.155

log(%CaO) + 1.4B

1400°C

(a)

3.0

2.5

2.0

1.5

3.5

3.0

2.5

2.0(b)

1500°C

1550°C1600°C

3.0

2.5

2.0

1.5

1.0(c)

2.0 2.5 3.0 3.5 4.0 4.5

log(%CaO) + 1.4Blog(%CaO) + 1.4B

Fig. 2.93 (a) 1400°C; (b) 1500°C; (c) 1550°C and1600°C. Variation of equilibrium relation for the sil-icon-sulfur coupled reaction with slag basicity B forunit activity of carbon. Reference cited in Ref. 143.

Log (% [%S

i SO ]2)

1(%

[S Si iO ]2)

21 ⁄2

Log (% [%S

i SO ]2)

1(%

[S Si iO ]2)

21 ⁄2

Log (% [%S

i SO ]2)

1(%

[S Si iO ]2)

21 ⁄2

Ironmaking Volume

2.6.3.1.5 Si–Ti Coupled Reaction Delve et al.156 have studied the silicon-titanium coupled reaction ingraphite-saturated melts using blast furnace type slags:

(TiO2) + [Si] = (SiO2) + [Ti] (2.6.28)

Their experimental results, for temperatures of 1500 and 1600°C and basicities of 1 to 2, may besummarized by the following equation.

(2.6.29)

(2.6.30)

2.6.3.2 Mechanisms of Slag-Metal Reactions

2.6.3.2.1 Experimental Work Experiments were made by the authors143 to simulate the events inthe upper part of the blast furnace hearth where metal droplets pass through the slag layer.Solid pieces (4 to 5 mm dia.) of graphite-saturated iron containing Si and S were dropped onthe surface of a pool of remelted blast furnace slag (65 g) contained in a graphite tube (20mm dia.) at 1480°C; an argon atmosphere was maintained over the melt. Twenty pieces ofmetal (7 g total) were dropped one at a time at 10–20 s intervals, within 7–10 min total timeof the experiment. The metal pieces melted rapidly and descended a 10 cm deep column ofmolten slag as individual metal droplets. After the last piece was dropped the melt wasrapidly cooled. The residence time of the droplets in the slag column is estimated to be about1–2 s, if there is no appreciable buoyancy effect due to gas evolution. The metal droplets col-lected in a well at the bottom of the slag column; metal and slag were subsequently analyzedfor manganese, silicon and sulfur.

With the addition of MnO to the slag, there is silicon transfer from metal to slag. As is seen fromthe experimental results in Fig. 2.95, the extent of silicon oxidation increases with increasing%MnO in the slag via the Si–Mn coupled reaction

log .%%

.KCaOSiOSiTi = +0 46 0 39

2

ΚSiTiTi

TiO

SiO

Si= [ ]

( )( )

[ ]%

%

%

%2

2

0.4 0.8 1.2 1.6B

300

200

100

0

30%50%

1600°C

1500°C

1400°C

(%S

)[%

S]p C

O (

atm

)

Fig. 2.94 Sulfur distribution ratio forgraphite-saturated melts as a functionof slag basicity. From Ref. 143.

Fundamentals of Iron and Steelmaking

2(MnO) + [Si] → 2[Mn] + (SiO2) (2.6.31)

In addition, there is also MnO reduction by carbon in the metal droplets.

(MnO) + [C] → [Mn] + CO (2.6.32)

With the slags containing MnO > 3%, the metal droplets desiliconized down to 0.1 – 0.3% Si.Within this region, the silicon and manganese distribution ratios are within the ranges(%SiO2)/[%Si] = 120 to 350 and [%Mn]/(%MnO) = 0.7 to 1.8. These ratios give KMnSi valuesbelow the equilibrium value of 1096 derived from equation 2.6.23 for the slag basicity of 1.5.

The effect of MnO content of the slag on the extent of desulfurization of metal droplets duringdescent in the slag column is shown in Fig. 2.96. The shaded area within the range 0.010 to0.035% S corresponds to the state of slag-metal equilibrium represented by equation 2.6.26, formetal droplets containing 0.1 to 0.3% Si and the slag of basicity 1.5 containing 41% CaO, 35%SiO2 and 1.5% S.

The extremely fast rates of reactions observed in the foregoing experiments may be attributed tothe presence of a thin gas film (consisting of the vapor species CO, SiO, SiS and Mn) around themetal droplets, which provides the reaction path for the transfer of reactants to and from slag andmetal via the gas phase.

2.6.3.3 Blast Furnace Tap Chemistry Data

In a previous study157 an assessment was made of the state of slag-metal reactions in the blast fur-nace hearth from an analysis of the daily average compositions of metal and slag samples as nor-mally recorded in the plants. The plant data used were those reported by Okabe et al.158 from ChibaWorks of Kawasaki Steel and the daily average data for a period of a month from U.S. Steel plants.

In the plant data used, the melt temperatures at tap are mostly in the range 1500 ± 25°C. The aver-age slag compositions in mass percent are in the range 38–42% CaO, 8–10% MgO, 34–38% SiO2,10–12% Al2O3, 0.5–1.0% MnO, 2% S and minor amounts of other oxides. The slag basicity is about

0 4 8 12 16

Sili

con

in m

etal

(w

t %)

1.59 [%Si]i1.16 [%Si]i0.93[%Si]i0.63 [%Si]i

0.4

2.0

1.6

1.2

0.8

(MnO)i (wt %)

Fig. 2.95 Change in silicon content of metaldroplets passing through a 10 cm deep slagcolumn. From Ref. 143.

Ironmaking Volume

1.4 ± 0.15. The hot metal compositions in the tap stream are in the range: 0.4–0.8% Mn, 0.5–1.5%Si, 0.02–0.05% S, 5% C and other usual impurities.

The silicon, manganese and sulfur distribution ratios from plant data are scattered within theshaded areas in Fig. 2.97. The dotted lines are for the slag-metal equilibria at 1 atm pressure ofCO, which is close to the CO partial pressure in the hearth zone of the blast furnace. It should benoted that the equilibrium line for the Si/SiO2 ratio is based on equation 2.6.16 representing theexperimental data and the equilibrium relation in Fig. 2.88, i.e. dotted curves. It is only the sili-con distribution ratio that is scattered about the gas-slag-metal equilibrium line for the three-phase reaction

(SiO2) + 2[C] = [Si] + 2CO(g) (2.6.33)

Values of KMnSi scattered within the shaded area in Fig. 2.98 are below the equilibrium line (dot-ted). It should be pointed out that in the upper part of the slag layer, the iron oxide content will behigher than manganese oxide. Therefore, the silicon in metal droplets will be oxidized more read-ily by iron oxide in the upper part of the slag layer, resulting in the observed non-equilibrium statefor the Si–Mn coupled reaction in equation 2.6.31.

With iron ore of low basicity in the blast furnace burden, the slag basicity will be low and fur-thermore, the iron oxide content in the upper part of the slag layer is expected to be higher. It is

(MnO)i (wt. %)

Sul

fur

in m

etal

(w

t. %

)

0 4 8 12 16

[%Si]i [%S]i1.59 0.141.16 0.0840.93 0.100.63 0.14

0.12

0.16

0.08

0.04

Fig. 2.96 Change in sulfur content of metal droplets passing through a 10 cm deep slag column; shadedregion is for slag-metal equilibrium at 1480°C. From Ref. 143.

Fundamentals of Iron and Steelmaking

1.2 1.3 1.4 1.5 1.6

%CaO + %MgO%SiO2

1550°C

1400°C

1500°C

1550°C

1400°C

1400°CPlant data

Equilibrium

[%

Si]

(%S

iO2)

[%M

n](%

MnO

)(%

S)

[%S

]

1500°C

0.08

0.06

0.04

0.02

4

3

1

80

60

2

40

20

Fig. 2.97 Si, Mn and S distribution ratios are compared with the equilibrium data for graphite-saturated meltsat 1 atm CO. From Ref. 159.

presumably for this reason that a low slag basicity, the KMnSi values are much lower than the equi-librium values for the Si–Mn couple reaction.

In an earlier study of plant data from a ferromanganese blast furnace in the UK,160 it was foundthat there were departures from equilibrium for the Si oxidation by MnO in the slag in a mannersimilar to that observed for the iron blast furnace.

The plant data in Fig. 2.99 for the sulfur distribution ratio are scattered about the equilibrium linefor the Mn–S coupled reaction at 1500°C, represented by equation 2.6.27. However, the ratios

Ironmaking Volume

(%S)/[%S] in the plant data are lower than the equilibrium values for the Si–S coupled reactionrepresented by equation 2.6.26. Nevertheless, despite departures from equilibrium, the silicon andsulfur contents of the blast furnace iron change in a systematic manner, i.e. high silicon/low sulfurand low silicon/high sulfur.

It should be borne in mind that because of fluctuations in the operating conditions in the blast fur-nace, there will be variations in temperature and the extent of reaction of metal droplets duringdescent through the slag layer. Consequently, the metal droplets of varying composition collectingin the stagnant hearth will bring about the composition and temperature stratification that is com-mon to all blast furnaces.

2.7 Fundamentals of Steelmaking ReactionsIn this section of Chapter 2, the discussion of steelmaking reactions will be confined to an assess-ment of the reaction mechanisms and the state of slag-metal reactions at the time of furnace tap-ping.

1.2 1.3 1.4 1.5

1000

600

400

200

100

80

60

40

20

10

%CaO + %MgO% SiO2

[%M

n]

2 (%

SiO

2)(%

MnO

)

[%

Si]

0 2 4 6 8

120

80 1600°C

Plant data

Equilibrium

1500°C1400°C

40

[%Mn](%MnO)

(%S

)[%

S]

Fig. 2.98 KMnSi values for plantdata are compared with the equi-librium values (dotted line). FromRef. 159.

Fig. 2.99 The blast furnace data are compared with the slag–metal equilibrium values for the Mn–S coupledreaction. From Ref. 159.

Fundamentals of Iron and Steelmaking

2.7.1 Slag-Metal Equilibrium in Steelmaking The reaction equilibria in the liquid steel-slag systems have been extensively studied, both experi-mentally and theoretically by applying the principles of thermodynamics and physical chemistry.In a recent reassessment of the available experimental data on steel-slag reactions103, it became evi-dent that the equilibrium constants of slag-metal reactions vary with the slag composition in dif-ferent ways, depending on the type of reaction. For some reactions the slag basicity is the keyparameter to be considered; for another reaction the key parameter could be the mass concentra-tion of either the acidic or basic oxide components of the slag.

2.7.1.1 Oxidation of Iron

In steelmaking slags, the total number of g-mols of oxides per 100 g of slag is within the range1.65 ± 0.05. Therefore, the analysis of the slag-metal equilibrium data, in terms of the activity andmol fraction of iron oxide, can be transposed to a simple relation between the mass ratio[ppm O]/(%FeO) and the sum of the acidic oxides %SiO2 + 0.84 × %P2O5 as depicted in Fig.2.100(a). The experimental data used in the diagram are those cited in Ref. 103. There is of coursea corollary relation between the ratio [ppm O]/(%FeO) and the slag basicity as shown in Fig.2.100(b).

%SiO2 + 0.84 × %P2O5

0 10 20 30

80

40

0

1600°C

xx xx

x

xx

x x

x xx

xx

x

x

(a)

100

80

60

40

20

0

(b)

0 1 2 3 4 5 6B

1500°C

1600°C

1700°C

x

x

[ppm

O]

(%F

eO)

[ppm

O]

(%F

eO)

Fig. 2.100 Equilibrium ratio[ppm O]/(%FeO) related to (a)SiO2 and P2O5 contents and (b)slag basicity; experimental dataare those cited in Ref. 103.

Ironmaking Volume

2.7.1.2 Oxidation of Manganese

For the FeO and MnO exchange reaction involving the oxidation of manganese in steel, formulatedbelow,

(FeO) + [Mn] = (MnO) + [Fe] (2.7.1)

the equilibrium relation may be described in terms of the mass concentrations of oxides

(2.7.2)

where the equilibrium relation K′FeMndepends on temperature and slagcomposition.

The values of K′FeMn derived fromthe equilibrium constant for reaction2.7.1, given in Ref. 27 and the activ-ity coefficient ratios γFeO/γMnO in Fig.2.67, are plotted in Fig. 2.101 againstthe slag basicity. In BOF, OBM(Q-BOP) and EAF steelmaking, the slagbasicities are usually in the range 2.5to 4.0 and the melt temperature inthe vessel at the time of furnace tap-ping in most practices is between1590 and 1630°C for which the equi-librium K′FeMn is 1.9 ± 0.3. The plantanalytical data for tap samples giveK′FeMn values that are scattered aboutthe indicated slag-metal equilibriumvalues.

Morales and Fruehan161 have recentlydetermined experimentally the equi-librium constant K′FeMn for reaction2.7.1 using MgO-saturated calciumsilicate melts. Their values of K′FeMnare plotted in Fig. 2.102 together withsome data from the studies of Chip-man et al.162 and Suito et al.163. Thebroken line curve is reproduced fromFig. 2.101. Resolution of observeddifferences in the values of K′FeMnawaits future studies.

2.7.1.3 Oxidation of Carbon

With respect to the slag-metal reaction, the equilibrium relation for carbon oxidation would be

(FeO) + [C] = CO + [Fe] (2.7.3)

(2.7.4)

(2.7.5)log .ΚFC T= − +5730

5 096

ΚFCCO

FeO

p atmC

= ( )[ ]% a

′ = ( )( )[ ]

ΚFeMnMnO

FeO Mn%

% %

B

1.5 2.5 3.5 4.5

8

6

4

2

0

K′ F

eMn

1800 C

1650 C

1700 C

Fig. 2.101 Equilibrium relation in equation 2.7.2 related to slagbasicity. From Ref. 103.

Fundamentals of Iron and Steelmaking

For 1600°C, γ FeO = 1.3 at slag basicity of B = 3.2 and pCO = 1.5 atm (average CO pressure in thevessel), we obtain the following equilibrium relation between the carbon content of steel and theiron oxide content of slag.

2.7.1.4 Oxidation of Chromium

There are two valencies of chromium (Cr2+ and Cr3+) dissolved in the slag. The ratio Cr2+/Cr3+

increases with an increasing temperature, decreasing oxygen potential and decreasing slag basic-ity. Under steelmaking conditions, i.e. in the basic slags and at high oxygen potentials, the triva-lent chromium predominates in the slag. The equilibrium distribution of chromium between slagand metal for basic steelmaking slags, determined by various investigators, is shown in Fig. 2.103;slope of the line represents an average of these data.

(2.7.7)

2.7.1.5 Oxidation of Phosphorus

It was in the late 1960s that the correct formulation of the phosphorus reaction was at last realized, thus

[P] + 5/2[O] + 3/2(O2–) = (PO43–) (2.7.8)

%%

. . %CrCr

FeO( )[ ]

= ±( ) × ( )0 3 0 1

(2.7.6)

K = 108.8FC

aFeO FeON FeO FeO= ≈×

( ) = × ( )1 31 3

72 1 650 011.

..

% . %

log

K' M

n-F

e

0 1 2 3 4 5

Temperature: 1600°CMorales and Fruelhan 161

Chipman et al162

Suito et al163

From Fig. 2.101

2.0

1.5

1.0

0.5

0.0

(%CaO + %MgO) %SiO2

Basicity, B =

Fig. 2.102 Experimental values of K′FeMn measured recently by Morales and Fruehan161.

Ironmaking Volume

At low concentrations of [P] and [O], as in most of the experimental melts, their activity coeffi-cients are close to unity, therefore mass concentrations can be used in formulating the equilibriumrelation KPO for the above reaction.

(2.7.9)

The equilibrium relation KPO, known as the phosphate capacity of the slag, depends on tempera-ture and slag composition.

From a reassessment of all the available experimental data, discussed in detail in Ref. 103, it was con-cluded that CaO and MgO components of the slag, had the strongest effect on the phosphate capac-ity of the slag. Over a wide range of slag composition and for temperatures of 1550 to 1700°C, thesteel-slag equilibrium with respect to the phosphorus reaction may be represented by the equation

(2.7.10)

where BO = %CaO + 0.3 (%MgO).

2.7.1.6 Reduction of Sulfur

The sulfur transfer from metal to slag is a reduction process as represented by this equation

[S] + (O2–) = (S2–) + [O] (2.7.11)

for which the state of slag-metal equilibrium is represented by

(2.7.12)ΚSOSS

O= ( )[ ] [ ]%%

%

log,

. .ΚPO TBO= − + ×21 740

9 87 0 071

ΚPOPP

O= ( )[ ] [ ]−%%

%5

2

FeO (wt %)

0 4 8 12 16 20 24 28

(%C

r)[%

Cr]

10

8

6

4

2

Fig. 2.103 Variation of chromium distribution ratio with the iron oxide content of slag, in the (∆) open hearth164

and (o) electric arc furnace165 at tap is compared with the results of laboratory experiments166(• ).

Fundamentals of Iron and Steelmaking

As is seen from the plots in Fig. 2.104, the sulfide capacities of slags, KSO, measured in three inde-pendent studies are in general accord. The effect of temperature on KSO is masked by the scatter inthe data. The concentration of acidic oxides, e.g. %SiO2 + 0.84 × %P2O5, rather than the slag basic-ity seems to be better representation of the dependence of KSO on the slag composition.

2.7.2 State of Reactions in SteelmakingThere are numerous versions of oxygen steelmaking such as top blowing (BOF, BOP, LD, etc.),bottom blowing (OBM, Q-BOP, etc.) and combined blowing (K-OBM, LBE, etc.). The state of therefining reactions depend to some degree on the process. Bottom blowing in general provides bet-ter slag-metal mixing and reactions are closer to equilibrium. In the following section the state ofreactions for top blowing (BOF) and bottom blowing (OBM) is given. The state of reactions forcombined or mixed blowing processes would be between these two limiting cases. The analyticalplant data used in this study were on samples taken from the vessel at first turndown from the BOPand Q-BOP shops of U.S. Steel. These plant data were acquired through the kind collaboration ofthe USS research personnel at the Technical Center.

2.7.2.1 Decarburization and FeO Formation

The most important reaction in steelmaking is decarburization. It not only determines the processtime but also the FeO content of the slag, affecting yield and refining. When oxygen is injected intoan oxygen steelmaking furnace a tremendous quantity of gas is evolved, forming a gas-metal-slagemulsion which is three to four times greater in volume than the non-emulsified slag and metal.The chemical reactions take place between the metal droplets, the slag and gas in the emulsion.These reactions have been observed in the laboratory using x-ray techniques indicating in manycases, the gas phase (primarily CO) separates the slag and metal, and that gaseous intermediatesplay a role in decarburization.

%SiO2 + 0.84 × %P2O5

0 10 20 30 40 1 2 3 4 5B

1623-171516001600

°C

1600

1.2

1.0

0.8

0.6

0

0.4

0.2

k SO

=[%

O]

(%S

)[%

S]

Fig. 2.104 Sulfide capacities of slags. From Ref. 103.

Ironmaking Volume

When oxygen first contacts a liquid iron-carbon alloy it initially reacts with iron according to reaction2.7.13, even though thermodynamically it favors its reaction with carbon. This is due to the relativeabundance of iron in comparison to carbon. Carbon in the liquid metal then diffuses to the interfacereducing the FeO by reaction 2.7.14. The net reaction is the oxidation of carbon, reaction 2.7.15.

Fe + 1/2O2 = FeO (2.7.13)

FeO + C = CO + Fe (2.7.14)

C + 1/2O2 = CO (2.7.15)

However, carbon is only oxidized as fast as it can be transferred to the surface.

At high carbon contents the rate of mass transfer is high such that most of the FeO formed isreduced and the rate of decarburization is controlled by the rate of oxygen supply:

(2.7.16)

whereN·O2

= the flow rate of oxygen in moles,MC = the molecular weight of carbon (12),W = the weight of steel,

f = the fraction of the product gas which is CO; the remainder is CO2 and f isclose to unity (0.8 to 1).

Below a critical carbon content the rate of mass transfer is insufficient to react with all the injectedoxygen. In this case the rate of decarburization is given by168:

(2.7.17)

whereρ = density or steel,

%Ce = the equlibrium carbon with the slag for reaction 2.7.14 and is close to zero,mi = the mass transfer coefficient for the specific reaction site,Ai = the metal-FeO surface area for the specific reaction site.

For top blown processes the reaction takes place between the metal droplets ejected into the emul-sion and the FeO in the slag. For bottom blowing there is less of an emulsion and the reaction takesplace at the interface of the metal bath and the rising bubbles which have FeO associated withthem. The critical carbon is when the rates given by 2.7.16 and 2.7.17 are equal and is typicallyabout 0.3% C.

The actual values of mi and Aiare not known, consequently an overall decarburization constant (kC)can be defined and the rate below the critical carbon content is given by 2.7.19 and 2.7.20:

(2.7.18)

(2.7.19)

or,

(2.7.20)

where tc is the time at which the critical carbon content is obtained. The equilibrium carbon con-tent (%Ce) is close to zero. However in actual steelmaking there is a practical limit of about 0.01to 0.03 for %Ce.

ln% %

% %

C C

C Ck t te

C eC C

−( )−( ) = − −( )

d Cdt

k C CC e%

% %= − −( )

kW

m AC i ii

= ∑ρ

d Cdt W

C C m Ae i ii

%% %= − −( ) ∑ρ

d Cdt

N M

WfO C% ˙

= − +( )2100

1

Fundamentals of Iron and Steelmaking

The value of kC increases with the blowing rate since the amount of ejected droplets and bubblesincreases. Also, kc decreases with the amount of steel, (W), as indicated by 2.7.19. In actualprocesses, the blowing rate is proportional to the weight of steel and , therefore, kC has similar val-ues in most oxygen steelmaking operations. For top blowing, kC is about 0.015 s–1 and for bottomblowing 0.017 s–1. The values of the critical carbon content are also similar ranging from 0.2 to0.4% C. The rate of decarburization for a typical steelmaking process is shown in Fig. 2.105. Atthe initial stage when silicon is being oxidized, which will be discussed later, the rate of decarbur-ization is low. The value of kC is higher for bottowm blowing because mixing is more intensive andthe reaction occurs at the interface of the rising bubbles as well as the slag-metal emulsion.

Below the critical carbon content, when the rate of mass transfer of carbon is insufficient to reduceall of the FeO formed and, therefore, the FeO content of the slag increases rapidly. In actualprocesses, initially, some FeO forms because it has a low activity in the slag resulting in about 5-10 % FeO in the slag. The FeO remains constant until the critical carbon content and then the FeOincreases rapidly. The amount of FeO can be computed from a mass balance for oxygen. Specifi-cally the oxgyen not used for carbon, silicon or manganese oxidizes iron to FeO. The moles of FeOin the slag at anytime (NFeO) is given by:

(2.7.21)

where NSiO2

and NMnO2

are the moles of oxygen consumed in oxidizing Si and Mn. Since the rate ofdecarburizaiton is slightly higher for bottom and mixed blowing these processes have lower FeOcontents.

At all levels of turndown carbon, the iron oxide content of BOF slag is about twice that of OBM(Q-BOP) slag (Fig. 2.106). The dotted line depicts the slag-metal equilibrium value of(%FeO)[%C] ≈ 1.25.

As depicted in Fig. 2.107, the square root correlation also applies to the product (%FeO)[%C] forlow carbon contents, with marked departure form this empirical correlation at higher carbon con-tents. The slopes of the lines for low carbon contents are given below.

N Nd C

dtW fM

dt N NFeO OC

t

OSi

OMn= − +( )

− +( )∫ 211002 2 2

0

˙ %

Time (min)0 5 10 15

C a

nd S

i con

tent

(%

) 4

3

2

1

0

% Silicon% Carbon

5

0 0.2 0.4 0.6C (%)

30

20

10

0

FeO

(%

)

Temperature: 1610 ± 20°CBOFOBMEquilibrium

Fig. 2.105 Computed carbon and silicon contents ofsteel in oxygen steelmaking processes.

Fig. 2.106 Iron oxide-carbon relations in BOF andOBM (Q-BOP) are compared with the average equi-librium relation (-------). From Ref. 103.

Ironmaking Volume

(2.7.22)

(2.7.23)

2.7.2.2 Oxygen-Carbon Relation

Noting from the plot in Fig. 2.108, there is an interesting correlation between the product [ppm O][%C] and the carbon content of the steel. The square root correlation holds up to about 0.05% Cin BOF and up to 0.08% C in OBM(Q-BOP) steelmaking. At low carbon contents, the oxygen con-tent of steel in the BOF practice is higher than that in OBM steelmaking. For carbon contents above0.15% the product [ppm O] [%C] is essentially constant at about 30 ± 2, which is the equilibriumvalue for an average gas (CO) bubble pressure of about 1.5 atmosphere in the steel bath.

At low carbon levels in the melt near the end of the blow, much of the oxygen is consumed by theoxidation of iron, manganese and phosphorus, resulting in a lower volume of CO generation. Withthe bottom injection of argon in the BOF combined-blowing practice, and the presence of hydro-gen in the gas bubbles in OBM, the partial pressure of CO in the gas bubbles will be lowered inboth processes when the rate of CO generation decreases. A decrease in the CO partial pressureat low carbon contents will be greater in OBM than in BOF practices, because the hydrogen con-tent of gas bubbles in OBM is greater than the argon content of gas bubbles in BOF. It is pre-sumably for this reason that the concentration product [O][C] in OBM steelmaking is lower thanin the BOF combined-blowing practice, particularly at low carbon levels.

OBM (Q - BOP) with C < 0.10%,

% % . .FeO C( ) = ±2 6 0 3

BOF with C < 0.10%,

% % . .FeO C( ) = ±4 2 0 3

%C0.02 0.05 0.1 0.2 0.3 0.4 0.5 0.6

(FeO

)[%

C]

0 0.2 0.4 0.6 0.8

4

2

3

1

0

%C

Temperature: 1610 ± 20°CBOFOBM

Fig. 2.107 Variation of product (FeO)[%C] with car-bon content of steel at first turndown. From Ref. 103.

%C0.02 0.05 0.1 0.2 0.3

16

0 0.2 0.4 0.6

√%C

32

24

8

0

[ppm

O][%

C]

Temperature: 1610 ± 20°C

BOF

OBM

Fig. 2.108 Variation of product [ppm O][%C] withcarbon content of steel at first turndown. From Ref.103.

Fundamentals of Iron and Steelmaking

The non-equilibrium states of the carbon-oxygen reaction at low carbon contents in BOF andOBM(Q-BOP) are represented by the folowing empirical relations.

(2.7.24)

(2.7.25)

2.7.2.3 Desiliconization

Silicon is oxidized out of hot metal early in the process. The oxidation reaction supplies heat andthe SiO2 reacts with the CaO to form the slag.

Si + 1/2O2 = (SiO2) (2.7.26)

The thermodynamics of the reaction indicate virtually all of the Si is oxidized. The rate is con-trolled by liquid phase mass transfer, represented by the following equation:

(2.7.27)

wheremSi = mass transfer coefficient for silicon,

%Sie = the silicon content in the metal in equilibrium with the slag and isclose to zero.

As with decarburization, an overall rate parameter for Si can be defined, kSi, similar to kC. Withinour ability to estimate kSi it is about equal to kC since A, W, and are the same and mass transfercoefficients vary only as the diffusivity to the one half power. Therefore 2.7.27 simplifies to:

(2.7.28)

where %Si° is the initial silicon and kSi is the overall constant for Si and is approximately equal tokC. The rate for Si oxidadtion is shown in Fig. 2.105.

2.7.2.4 Manganese Oxide–Carbon Relation

At low carbon contents, the ratio [%Mn]/(%MnO) is also found to be proportional to Ï%wCw, rep-resented as given below.

(2.7.29)

(2.7.30)

2.7.2.5 FeO–MnO–Mn–O Relations

From the foregoing empirical correlations for the non-equilibrium states of reactions involving thecarbon content of steel, the relations obtained for the reaction of oxygen with iron and manganeseare compared in the table below with the equilibrium values for temperatures of 1610 ± 20°C andslag basicities of B = 3.2 ± 0.6.

OBM (Q - BOP) with C < 0.10%,

%

% %. .

MnMnO C

[ ]( )

= ±10 2 0 02

BOF with C < 0.10%,

%

% %. .

MnMnO C

[ ]( )

= ±10 1 0 02

ln%

%

Si

Sik tSio

= −

d Sidt

A mW

Si SiSie

%% %= − −[ ]ρ

OBM (Q - BOP) with C < 0.08%,

ppm O C[ ] = ±% 80 5

BOF with C < 0.05%,

ppm O C[ ] = ±% 135 5

Ironmaking Volume

Values forBOF OBM(Q-BOP) slag-metal

C < 0.05% C < 0.08% equilibrium__________ ____________ __________[ppm O]

32 ± 4 32 ± 5 26 ± 9_______(%FeO)

[%Mn][ppm O]13.6 ± 3.2 16.1 ± 2.6 18 ± 6_____________

(%MnO)

(MnO) 2.6 ± 0.5 2.2 ± 0.2 1.9 ± 0.2_____________

(%FeO)[%Mn]

It is seen that the concentration ratios of the reactants in low carbon steel describing the states ofoxidation of iron and manganese, are scattered about the values for the slag-metal equilibrium.However, as indicated by the plant data in Fig. 2.108, the oxidation of iron and manganese are inthe non-equilibrium states for high carbon contents in the steel at turndown. Although the concen-tration product [O][C] is close to the equilibrium value for an average CO pressure of about 1.5atm in the steel bath, the concentrations of iron oxide and manganese oxide in the slag are abovethe equilibrium values for high carbon contents in the melt.

It is concluded from these observations that:

(i) at low carbon contents the equilibrium state of iron and manganese oxidation con-trols the concentration of dissolved oxygen

(ii) at high carbon contents it is the CO–C–O equilibrium which controls the oxygencontent of the steel.

B

2.4 2.8 3.2 3.6 4.0

[%M

n] [p

pm O

]

(%M

nO)

60

40

20

0

30

20

10

0

1630°C

1630°C

1590°C

1590°C

Temperature: 1610 ± 20°C

Turndown C: 0.1-0.3%

[ppm

O]

(%F

eO)

BOF

OBM

Slag-metal equilibrium

Fig. 2.108 Non-equilibrium states of oxidation of iron and manganese at high carbon contents in steel. FromRef. 103.

2.7.2.6 State of Phosphorus Reaction

The slag/metal phosophorus distributionratios at first turndown in BOF and OBM(Q-BOP) steelmaking are plotted in Fig.2.109 against the carbon content of the steel.The plant data are for the turndown temper-atures of 1610 ± 20°C and slags containing50 ± 2% CaO and 6 ± 2% MgO. The shadedarea is for the slag-metal equilibrium for theabove stated conditions in OBM(Q-BOP),based on the empirical [O][C] relations, i.e.for C < 0.08%, [ppm O] Ï%wCw = 80 and forC > 0.15%, [ppm O][%C] = 30.

Noting that the oxygen contents of the steelat low carbon levels are greater in BOFsteelmaking, the equilibrium phosphorusdistribution ratios will likewise be greaterin BOF than in (OBM) Q-BOP steelmaking.For example, at 0.05% C and about 600 ppmO in BOF at turndown the average equilib-rium value of (%P)/[%P] is about 200 at1610°C, as compared to the average valueof 60 in OBM(Q-BOP) at 0.05% C withabout 360 ppm O.

Below 0.04% C the phosphorus distribution ratios in OBM(Q-BOP) are in general accord with thevalues for slag-metal equilibrium. However, at higher carbon contents the ratios (%P)/[%P] arewell above the equilibrium values. In the case of BOF steelmaking below 0.1% C at turndown, theratios (%P)/[%P] are much lower than the equilibrium values. On the other hand, at higher carboncontents the phosphorus distribution ratios arehigher than the equilibrium values as in the caseof OBM(Q-BOP).

The effect of temperature on the phosphorus dis-tribution ratio in OBM(Q-BOP) is shown in Fig.2.110 for melts containing 0.014% to 0.022% Cwith BO = 52 ± 2% in the slag.

2.7.2.7 State of Sulfur Reaction

A highly reducing condition that is required forextensive desulfurization of steel is opposite to theoxidizing condition necessary for steel making.However, some desulfurization is achieved duringoxygen blowing for decarburization and dephos-phorization. As seen from typical examples of theBOF and OBM(Q-BOP) plant data in Fig. 2.111,the state of steel desulfurization at turndown,described by the expression [%O](%S)/[%S], isrelated to the SiO2 and P2O5 contents of the slag.Most of the points for OBM(Q-BOP) are withinthe hatched area for the slag-metal equilibriumreproduced from Fig. 2.104. However, in the caseof BOF steelmaking the slag/metal sulfur distrib-ution ratios at turndown are about one-third or

153

0 0.1 0.2 0.3

BOFOBMEquilibrium for(O) contents in OBM

160

120

80

40

0

%C

%CaO: 48

Temperature: 1610 ± 20°C

52

(%P

)[%

P]

Fig. 2.109 Slag/metal phosphorus distribution ratios atfirst turndown in BOF and OBM(Q–BOP) practices;slag–metal equilibrium values are within the hatchedarea for Q–BOP. From Ref. 103.

1600 1640 1680 1720

200

160

120

80

40

(%P

)[%

P]

Temperature °C

Equilibrium for BO = 52% and[O] contents at

0.014% C0.022% C

Fig. 2.110 Effect of turndown temperature on theslag/metal phosphorus distribution ratios in OBM(Q-BOP) for turndown carbon contents of 0.014 to0.022% C; curves are for slag–metal equilibrium.From Ref. 103.

Fundamentals of Iron and Steelmaking

Ironmaking Volume

one-half of the slag-metal equilibrium values.At higher carbon contents, e.g. C > 0.1%, thesulfur distribution ratios in both processes arebelow the slag-metal equilibrium values.

2.7.2.8 Hydrogen in BOF and OBM(Q-BOP)Steelmaking

Hydrogen and nitrogen are removed from thesteel bath during oxygen blowing by CO car-rying off H2 and N2.

2H(in steel) → H2(g) (2.7.31)

2N(in steel) → N2(g) (2.7.32)

There is however continuous entry of bothhydrogen and nitrogen into the bath by variousmeans. In both BOF and OBM(Q-BOP) there isinvariably some leakage of water from the watercooling system of the hood into the vessel. Inthe case of OBM(Q-BOP), the natural gas(CH4) used as a tuyere coolant is a major source

of hydrogen.

The hydrogen content of steel in the tap ladle, measured by a probe called HYDRIS, is less than 5ppm in BOF steelmaking and 6 to 10 ppm H in OBM(Q-BOP) steelmaking. Because natural gas(CH4) is used as a tuyere coolant in the OBM, the hydrogen content of steel made in this vessel isalways higher than that in the BOF vessel. In both practices the re-blow will always increase thehydrogen content of the steel. A relatively small volume of CO evolved during the re-blow cannotovercome the hydrogen pickup from various sources.

2.7.2.9 The Nitrogen Reaction

As demonstrated, the decarburization reaction is reasonably well understood as well as the slag-metal re-fining reactions which approach equilibrium. The removal of nitrogen is complex anddepends on numerous operating variables. With the advent of the production of high purity inter-stitial free (IF) steels the control of nitrogen has become of great importance. For years there havebeen “rules of thumb” for achieving low nitrogen. For example, using more hot metal and lessscrap in the charge or with combined blowing processes, switching the stirring gas from nitrogento argon have resulted in lower nitrogen contents.

The sources of nitrogen in oxygen steelmaking include the hot metal, scrap, impurity nitrogen inthe oxygen, and nitrogen in the stirring gas. Nitrogen from the atmosphere is not a major factorunless at first turndown a correction or reblow is required, in which case the furnace fills up withair which is entrained into the metal when the oxygen blow restarts, resulting in a significant nitro-gen pickup of 5 to 10 ppm.

Goldstein and Fruehan169 developed a comprehensive model to predict the nitrogen reaction insteelmaking. Nitrogen is removed by diffusing to the CO bubbles in the emulsion,or to the bubblesin the bath in bottom blowing. The nitrogen atoms combine to form N2, the rate of which is con-trolled by chemical kinetics and the nitrogen gas is removed with the CO bubbles. Both mass trans-fer and chemical kinetics contribute to the overall rate of removal.

N(metal) = N(surface) (2.7.33)

2N(surface) = N2 (2.7.34)

The mixed control model presented previously is the basis for the model. There are, however, sev-eral complications. For example, all of the rate parameters are functions of temperature. The sulfur

0 10 20 30

%SiO2 + 0.84 × %P2O5

BOF 1590-1630°C, C < 0.05%OBM 1590-1700°C, C < 0.1%Slag metal equilibrium

1.2

0.8

0.4

1.2

(%S

)[%

S][%

O]

Fig. 2.111 Equilibrium and non–equilibrium states ofsulphur reaction in OBM(Q-BOP) and BOF steel-making. From Ref. 103.

Fundamentals of Iron and Steelmaking

content of the metal changes with time and the oxygen content at the surface is considerably dif-ferent from the bulk concentration. Consequently the temperature and surface contents of oxygenand sulfur must be known as functions of time. Also, scrap is melting during the process changingthe composition of the metal.

An example of the results of the model calculations are shown in Fig. 2.112 and Fig. 2.113. In Fig.2.112 the nitrogen contents are shown for two hypothetical cases for a 200 ton oxygen steelmaking con-verter blowing oxygen at 800 Nm3/min. In one case the charge contains 80% heavy scrap, 16 cm thickcontaining 50 ppm nitrogen; in the second case there is no scrap but cooling is achieved by the use ofa 15% addition of DRI containing 20 ppm nitrogen. For the case of the heavy scrap, it melts late in theprocess releasing its nitrogen after most of the CO is generated, causing the nitrogen content to increaseto 30 ppm at the end of the blow. With no scrap the final nitrogen is significantly lower at 20 ppm. Themodel also indicates if ore, which has no nitrogen, is used for cooling, levels of 10 ppm nitrogen canbe obtained. In comparing the bulk and surface nitrogen contents, it is found that the surface concen-tration is only slightly less than the bulk, indicating that the nitrogen reaction is primarily controlled bychemical kinetics. In particular, towards the end of the blow the oxygen content at the surface is high,retarding the rate. This model is useful for optimizing the process for nitrogen control. For example,the effect of oxygen purity, the time of switching the stirring gas from N2 to argon, the metal sulfurcontent and the amount and size of scrap can be determined. The effect of switching the stirring gasfrom N2 to Ar is shown in Fig. 2.113.

2.7.2.10 General Considerations

The analyses of plant data on slag and metal samples taken at first turndown have revealed thatthere are indeed equilibrium and non-equilibrium states of reactions in oxygen steelmaking. In allthe reactions considered, the carbon content of steel is found to have a decisive effect on the stateof slag-metal reactions.

0 2 4 6 8 10 12 14

Time (min)

Nig

trog

en c

onte

nt (

%)

DRI 15% with 20 ppm NScrap 20% with 50 ppm N

0.0090

0.0070

0.0060

0.0050

0.0040

0.0030

0.0020

0.0010

0.0080

Fig. 2.112 Computed nitrogen content in a 200 ton oxygen steelmaking converter for 20% heavy scrap – 80%light scrap and DRI at a blowing rate of 800 Nm3/min O2. From Ref. 167.

Ironmaking Volume

Considering the highly dynamic nature of steelmaking with oxygen blowing and the completion ofthe process in less than 20 minutes, it is not surprising that the slag-metal reactions are in the non-equilibrium states in heats with high carbon contents at turndown. With regard to low carbon heatsall the slag-metal reactions are close to the equilibrium states in bottom blown processes. In thecase of BOF steelmaking however, the states of steel dephosphorization and desulfurization arebelow the expected levels for slag-metal equilibrium. As we all recognize it is of course the bottominjection of lime, together with oxygen, that brings about a closer approach to the slag-metal equi-librium in OBM(Q-BOP) as compared to the BOF practice, particularly in low carbon heats.

References

1. L. Onsager and R. M. Fuoss, J. Phys. Chem. 36 (1932): 2687.2. A. Einstein, Ann. Phys (Leipzig) 17 (1905): 54; Z. Elektrochem (1908): 14,235.3. E. T. Turkdogan, “Physicochemical Properties of Molten Slags and Glasses,” The Metals

Society (now The Institute of Materials), London, 1983.4. J. Szekely, Fluid Flow Phenomena in Metals Processing (New York: Academic Press, 1979).5. J. Szekely and N. J. Themelis, Rate Phenomena in Process Metallurgy (New York: Wiley,

1971).6. G. H. Geiger and D. R. Poirier, Transport Phenomena in Metallurgy (Reading, MA: Addi-

son-Wesley, 1973).7. J. Szekely, J. W. Evans, and J. K. Brimacombe, The Mathematical and Physical Modelling of

Primary Metals Processing Operations New York: Wiley, 1988).8. J. Szekely, G. Carlsson, and L. Helle, Ladle Metallurgy (Berlin: Springer, 1989).9. J. Szekely and O. J. Ilegbusi, The Physical and Mathematical Modelling of Tundish Opera-

tions (Berlin: Springer, 1989).

0 5 10 15Time (min)

100

80

60

40

20

0

Nitr

ogen

(pp

m)

Si Oxidation

Decarburization Stirring gas

N2

N2–Ar

Ar

Fig. 2.113 The effect of bottom stirring practice on nitrogen removal in the BOF with N2 during the entire blow,Ar during the entire blow, and with a switch from N2 to Ar at 50% through the blow. From Ref. 167.

Fundamentals of Iron and Steelmaking

10. J. S. Sheasby, W. E. Boggs, and E. T. Turkdogan, Metal Science 18 (1984): 127.11. C. Wagner, Z. Phys. Chem., Abt B 21 (1933), 25 (in “Atom Movements,” ASM (1950): 153.12. L. Himmel, R. F. Mehl, and C. E. Birchenall, Trans. AIME 197 (1953): 827.13. P. Hembree and J. B. Wagner, Trans. AIME 245, (1969): 1547.14. P. L. Walker, F. Rusinko, and L. G. Austin, Advan. Catalysis 21 (1959): 33.15. E. T. Turkdogan et al., Carbon 6 (1968): 467.16. E. T. Turkdogan and J. V. Vinters, Carbon 7 (1969): 101; 8 (1970): 39.17. E. T. Turkdogan, R. G. Olsson, and J. V. Vinters, Carbon 8 (1970): 545.18. R. H. Tien and E. T. Turkdogan, Carbon 8 (1970): 607.19. D. A. Aderibigbe and J. Szekely, Ironmaking and Steelmaking 9 (1982): 32.20. W .M. McKewan, Trans. TMS-AIME 218 (1960): 2.21. J. M. Quets, M. E. Wadsworth, and J. R. Lewis, Trans. TMS-AIME 218 (1960): 545: 221

(1961): 1186.22. N. J. Themelis and W. H. Gauvin, A.E. Ch. E.J. 8, (1962): 437; Trans. TMS-AIME 227 (1963):

290.23. N. A. Warner, Trans. TMS-AIME 230 (1964): 163.24. R .H. Spitzer, F. S. Manning, and W. O. Philbrook, Trans. TMS-AIME 236 (1966): 726.25. E. T. Turkdogan and J. V. Vinters, Metall. Trans. 2 (1971): 3175; 3 (1972): 1561.26. P. H. Calderbank, Chem. Eng. (London) 212 (1967): CE 209.27. E. T. Turkdogan, “Fundamentals of Steelmaking,” The Institute of Materials, London, 1996.28. I. Leibson et al., A.I.Ch.E.J. 2, (1956): 296.29. V. G. Levich, Physicochemical Hydrodynamics (Englewood Cliffs: Prentice-Hall, 1962).30. S. Glasstone, K. J. Laidler, and H. Eyring, The Theory of Rate Processes (New York:

McGraw-Hill, 1941).31. C. N. Hinshelwood, Kinetics of Chemical Change, (London: Oxford University Press, 1942).32. T. Fuwa, S. Ban-ya, and T. Shinohara, Tetsu-to-Hagane 53 (1967): S328.33. M. Inouye and T. Choh, Trans. Iron Steel Inst. Japan 8 (1968): 134.34. K. Mori and K. Suzuki, Trans. Iron Steel Inst. Japan 10 (1970): 232.35. R. J. Fruehan and L. J. Martonik, Metall. Trans. B 11B (1980): 615.36. M. Byrne and G. R. Belton, Metall. Trans. B 14B (1983): 441.37. P. Glaws and R. J. Fruehan, Metall Trans. B 16B (1985): 551.38. S. Ban-ya et al., Tetus-to-Hagane 60 (1974): 1443.39. G. Sain and G. R. Belton, Metall Trans. B 5B (1974): 1027–32; 7B (1976): 403–7.40. F. Mannion and R. J Fruehan, Metall Trans. B, 20B (1989): 853.41. T. Nagasaka and R. J. Fruehan, Metall Trans. B, 25B (1994): 245.42. G. R. Belton, Metall Trans. B, 7B (1976): 35–42.43. E. A. Gulbransen, K. F. Andrew, and F. A. Brassort, Carbon 2 (1965): 421.44. J. D. Blackwood, Aust. J. Appl. Sci. 13 (1962): 199.45. S. Ergun, J. Phys. Chem. 60 (1956): 480.46. K. Hedden and A. Lowe, Carbon 5 (1967): 339.47. H. J. Grabke, Ber. Bunsenges. Physik Chem. 70 (1966): 664.48. D. A. Aderibigbe and J. Szekely, Ironmaking & Steelmaking 8 (1981): 11.49. S. Story and R. J. Fruehan, To be submitted to Metall Trans., 199750. R. J. Fruehan, B. Lally, and P. C. Glaws, Trans. ISS, I&SM, (April 1987), 31.51. E. T. Turkdogan and J. V. Vinters, Metall. Trans. 5 (1974): 11.52. E. T. Turkdogan, Physical Chemistry of High Temperature Technology (New York: Academic

Press, 1980).53. H. J. Donald, “An Annotated Bibliography,” Mellon Inst. Ind. Res. Pittsburgh, PA. 1956.54. J. V. Kehrer and H. Leidheiser, J. Phys. Chem. 58, (1954): 550.55. W .R. Walker, J. F. Rakszawski, and G. R. Imperial, J. Phys. Chem. 63 (1959): 133, 140.56. W. R. Ruston et al., Carbon 7 (1969): 47.57. R. G. Olsson and E. T. Turkdogan, Metall. Trans. 5 (1974): 21.58. J. Macak, P. Knizek, and J. Malecha, Carbon 16 (1978): 111.59. E. R. Gilliland and P. Harriott, Ind. Eng. Chem. 46 (1954): 2195.60. T. H. Byrom, J. Iron Steel Inst. 92 (1915): 106.

Ironmaking Volume

61. H. C. H. Carpenter and C. C. Smith, J. Iron Steel Inst. 96 (1918): 139.62. O. Stelling, J. Met. 10 (1958): 290.63. H. Schenck and W. Maachlanka, Arch. Eisenhuttenwes.31 (1960): 271.64. R. J. Fruehan and L. J. Martonik, Metall Trans. 4 (1973): 2129.65. S. Chapman and T. G. Cowling, The Mathematical Theory of Non-uniform Gases, 3rd ed.

(London: Cambridge University Press, 1970).66. J. O. Hirschfelder, C. F. Curtiss, and R. B. Bird, Molecular Theory of Gases and Liquids,

(New York: Wiley, 1954).67. A. Eucken, Physik.Z. 14 (1913): 324.68. M. Knudsen, Ann. Phys. (Leipzig) 28 (1909): 75.69. C. H. Bosanquet, Br. TA Rep. BR–507, September 1944.70. E. T. Turkdogan, R. G. Olsson, and J. V. Vinters, Metall. Trans. 2 (1971): 3189.71. G. K. Sigworth and J. F. Elliott, Met. Sci. 8 (1974): 298.72. E. T. Turkdogan and L. E. Leake, J. Iron and Steel Inst. 179 (1955): 39.73. E. T. Turkdogan and R. A. Hancock, 179 (1955): 155; 183 (1956): 69.74. J. Chipman et al., Trans. ASM. 44 (1952): 1215.75. J. Chipman and T. P. Floridis, Acta Met 3 (1955): 456.76. N. R. Griffing, W. D. Forgeng, and G. W. Healy, Trans. AIME 224 (1962): 148.77. J. F. Elliott, M. Gleiser, and V. Ramakrishna, Thermochemistry for Steelmaking, vol. II

(Reading, MA: Addison-Wesley, 1963).78. S. N. Singh and K. E. Blazek, J. Metals (AIME) 26(10) (1974): 17.79. M. M. Wolf and W. Kurz, Metall.Transaction B 12B (1981) 85.80. A. A. Howe, Applied Scientific Research 44 (1987): 51.81. H. Yamada, T. Sakurai, and T. Takenouchi, Tetsu-to-Hagane 76 (1990): 438.82. M. M. Wolf, in “1st European Conference on Continuous Casting”, p. 2.489. Florence, Italy,

Sept. 23–25, 1991.83. C. R. Taylor and J. Chipman, Trans. AIME 154 (1943): 228.84. P .A. Distin, S. G. Whiteway, and C. R. Masson, Can. Metall. Q. 10 (1971): 13.85. A. E. Lord and N. A. Parlee, Trans. Met. Soc. AIME 218 (1960): 644.86. D. L. Sponseller and R. A. Flinn, Trans. Met. Soc. AIME 230 (1964): 876.87. P. K. Trojan and R. A. Flinn, Trans. ASM 54 (1961): 549.88. P. J. Guichelaar et al., Metall. Trans. 2 (1971): 3305.89. B. J. Keene, A survey of extant data for the surface tension of iron and its binary alloys, NPL

Rep. DMA(A) 67, June 1983.90. E. T. Turkdogan, in Foundry Processes—Their Chemistry and Physics, ed. S. Katz and C. F.

Landefeld (New York: Plenum Press, 1988), 53.91. P. Kozakevitch, in Surface Phenomena of Metal (London: Chem. Ind., 1968), 223.92. E. Selcuk and D. H. Kirkwood, J. Iron and Steel Inst. 211 (1973): 134.93. I. Jimbo and A. W. Cramb, Iron Steel Inst. Japan International 32 (1992): 26.94. A. Kasama et al., Can. Met. Quart. 22 (1983): 9.95. L. D. Lucas, Compt. Rend. 248 (1959): 2336.96. R. N. Barfield and J. A. Kitchener, J. Iron and Steel Inst. 180 (1955): 324.97. G. Tromel et al., Arch. Eisenhuttenwes. 40 (1969): 969.98. C. R. Taylor and J. Chipman, Trans. AIME 159 (1943): 228.99. M. Timucin and A. E. Morris, Metall. Trans 1 (1970): 3193.

100. S. H. Liu, A. Morales, and R. J. Fruehan, To be submitted to Metall Trans. B, 1997.101. R. H. Rein and J. Chipman, Trans. Met. Soc. AIME 233 (1965): 415.102. T. Fujisawa and H. Sakao, Tetsu-to-Hagane 63 (1977): 1494, 1504.103. “Ethem T. Turkdogan Symposium”, pp. 253–269. The Iron and Steel Society of AIME, May

15–17, 1994.104. Y. Iguchi, S. Ban-ya and T. Fuwa, Trans. Iron and Steel Inst. Japan 9 (1969): 189.105. K. Ito and R. J. Fruehan, Metall. Trans. B 19B (1988): 419.106. D. J. Min and R. J. Fruehan, Metall Trans. B 21B (1990): 1025.107. H. Suito and R. Inoue, Tetsu-to-Hagane 73 (1987): S246.108. K. Nomura, B. Ozturk, and R. J. Fruehan, Metall Trans. B 22B (1991): 783.

Fundamentals of Iron and Steelmaking

109. S. Ban-ya and J. D. Shim, Can. Metall. Q. 21 (1982): 319.110. P. Kozakevitch, Rev. Metall. 46 (1949): 505, 572.111. K. C. Mills and B. J. Keene, Inter. Met. Rev. 26 (1981): 21.112. H. Gaye et al., Can. Metall. Q. 23 (1984): 179.113. K. Ogino et al., Trans. Iron and Steel Inst. Japan 24 (1984): 522.114. I. Jimbo and A. W. Cranb, The Sixth International Iron and Steel Congress, Naguya, ISIJ, 1990, 499.115. D. R. Gaskell, A. McLean, and R. G. Ward, Trans. Faraday Soc. 65 (1969): 1498.116. Y. Skiraishi et al., Trans. Japan Inst. Met. 19 (1978): 264.117. Yu M. et al., Soob A Gruz. SSR 32(1) (1963): 117.118. L. Segers, A. Fontana, and R. Winand, Electrochem. Acta. 23 (1978): 1275.119. J. W. Tomlinson, M. S. R. Heynes, and J. O’M. Bockris, Trans. Faraday Soc. 54 (1958): 1822.120. L. R. Barrett and A. G. Thomas, J. Glas Technol. (1959): 179s.121. H. Winterhager, L. Greiner, and R. Kammel, Forschungsberichte des Landes (Nordrhein-

Westfalen, Nr. 1630: Westdeutscher Verlag, 1966).122. E. V. Krinochkin, K. T. Kurochin, and P. V. Umrikhin, Fiz. Khim. Poverkh. (Kiev: Naukova

Dumba, Yavlenii Rasp., 1971) ,179–83.123. J. S. Machin and T. B. Yee, J. Am. Cerm. Soc. 32 (1948): 200; 37 (1954) 177.124. K. Ito and R. J. Fruehan, Metall Trans. B 20B (1989): 509.125. K. Ito and R.J. Fruehan, Metall Trans. B 20B (1989): 515.126. Y. Zhang and R. J. Fruehan, Metall Trans. B 26B (1995): 811.127. T. Tokumetsu et al., Process Technology Conference Proceedings, Toronto, ISS, 1989.128. Y. Zhang and R. J. Fruehan, Metall Trans. B. 26B (1995): 803.129. S. Ban-ya, ISIJ International 33 (1993): 2–11.130. H. Gaye and J. Lehmann, Molten Slags, Fluxes, and Salts Conference, Sydney, 1997, IS War-

rendale, PA, 27–34.131. H. Gaye and J. Welfinger, Proc. Second International Symposium on Slags and Fluxes, 1984,

TMS Warrendale, PA 357–375.132. M. Blander, A Pelton and G. Erikssen, 4th Internation Conference on Slags and Fluxes, 1992,

ISIJ, 56–60.133. I. D. Sommerville, A. McLean and Y. D. Yang, Molten Slags, Fluxes, and Salts Conference,

Sydney, 1997, ISS Warrendale PA, 375–383.134. D. J. Sosinsky and I. D. Sommerville, Metall Trans. B. 17B (1986): 331–7.135. J. G. Peacey and W. G. Davenport, The Iron Blast Furnace (Oxford: Pergamon Press, 1979).136. A. Rist and G. Bonnivard, Rev. Met. 60 (1963): 23.137. A. Rist and N. Meysson, Rev. Met. 61 (1964): 121.138. N. Meysson, J. Weber, and A. Rist, Rev. Met. 61 (1964): 623139. A. Rist and N. Meysson, Rev. Met. 62 (1965): 995.140. N. Meysson, A. Maaref, and A. Rist, Rev. Met. 62 (1965): 1161.141. F. D. Richardson and J. H. E. Jeffes, J. Iron and Steel Inst. 160 (1948): 261.142. N. Tsuchiya, M. Tokuda, and M. Ohtani, Metall. Trans B7 (1976): 315.143. E. T. Turkdogan, G. J. W. Kor, and R. J. Fruehan, Ironmaking and Steelmaking 7 (1980): 268.144. B. Ozturk and R. J. Fruehan, Metall Trans. B 16B (1985): 121.145. N. Standish and W.-K. Lu, eds., Alkalies in Blast Furnaces (Ontario: McMaster University

Press, 1973).146. K. P. Abraham and L. J. Staffansson, Scand. J. Metall. 4 (1975): 193.147. J. Davies, J. T. Moon and F. B. Traice, Ironmaking and Steelmaking 5 (1978): 151.148. J. M. Steiler, “Etude Thermodynamique des Laitiers Liquides des Systems K2O–SiO2 et

K2O–CaO–SiO2–Al2O3,” IRSID, PCM–RE 646, July 1979.149. L. L. Simmons, L. R. Lowden and T. C. Ehlert, J. Phys. Chem. 81 (1977): 709.150. Z. Pociecha and J. Biczysko, in Seminar on Problems of Air and Water Pollution Arising in

the Iron and Steel Industry, Leningrad, Aug. 1971, CI.151. E. T. Turkdogan and P .H. Josephic, Ironmaking and Steelmaking 11 (1984): 192.152. K. L. Abraham, M. W. Davies, and F. D. Richardson, J. Iron and Steel Inst. 19 (1960): 82.153. E. W. Filer and L. S. Darken, Trans. AIME 194 (1952): 253.154. W. Oelsen, Arch. Eisenhuttenwes 35 (1964): 699, 713, 1039, 1115.

Ironmaking Volume